# Supplementary Information (SI) for Inorganic Chemistry Frontiers.
# This journal is © the Partner Organisations 2024

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 2068105'
loop_
_audit_author_name
_audit_author_address
'Xinlong Wang'
;Northeast Normal University
China
;
_audit_update_record             
;
2021-03-05 deposited with the CCDC.	2024-09-02 downloaded from the CCDC.
;
_audit_creation_date             2021-02-19
_audit_creation_method           
;
Olex2 1.3
(compiled 2020.11.12 svn.r5f609507 for OlexSys, GUI svn.r6272)
;
# end Validation Reply Form
_shelx_SHELXL_version_number     2018/3
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'K4.6 Mo42 O209 Ti12'
_chemical_formula_sum            'H62 K8 Mo42 O209 Ti12'
_chemical_formula_weight         8323.57
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ti Ti 0.2776 0.4457 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/n 1'
_space_group_name_Hall           '-P 2yn'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   17.3790(9)
_cell_length_b                   36.587(2)
_cell_length_c                   39.015(2)
_cell_angle_alpha                90
_cell_angle_beta                 93.9210(10)
_cell_angle_gamma                90
_cell_volume                     24750(2)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    9850
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      25.000
_cell_measurement_theta_min      2.292
_shelx_estimated_absorpt_T_max   0.54
_shelx_estimated_absorpt_T_min   0.21
_exptl_absorpt_coefficient_mu    2.643
_exptl_absorpt_correction_T_max  0.86
_exptl_absorpt_correction_T_min  0.84
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Krause et al., 2015) was used for absorption correction.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.234
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             15656
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.2
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0727
_diffrn_reflns_av_unetI/netI     0.0796
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       40
_diffrn_reflns_limit_k_min       -43
_diffrn_reflns_limit_l_max       44
_diffrn_reflns_limit_l_min       -46
_diffrn_reflns_number            143170
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.039
_diffrn_reflns_theta_max         25.039
_diffrn_reflns_theta_min         1.371
_diffrn_ambient_temperature      173.02
_diffrn_detector                 'charge-coupled device (CCD) area detector'
_diffrn_detector_area_resol_mean 7.9
_diffrn_detector_type            'Bruker D8 VENTURE'
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_device_type  'Bruker D8 VENTURE'
_diffrn_measurement_method       '0.5° ω and 0.5° φ scans'
_diffrn_radiation_collimation    'focusing mirrors'
_diffrn_radiation_detector       'Bruker D8 VENTURE'
_diffrn_radiation_monochromator  'mirror optics'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_xray_symbol    K-L~3~
_diffrn_source                   'microfocus sealed X-ray tube'
_diffrn_source_current           30.0
_diffrn_source_power             1.35
_diffrn_source_type              'Incoatec I\ms'
_diffrn_source_voltage           45.0
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                25396
_reflns_number_total             43613
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT+ Ver. 2016.5-0 (Bruker-AXS, 2016)'
_computing_data_collection       'APEX3 Ver. 2016.5-0 (Bruker-AXS, 2016)'
_computing_data_reduction        'SAINT+ Ver. 2016.5-0 (Bruker-AXS, 2016)'
_computing_molecular_graphics    'OLEX2 (Dolomanov et al., 2009)'
_computing_publication_material  'OLEX2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL (Sheldrick, 2015b)'
_computing_structure_solution    'XT (Sheldrick, 2015a)'
_refine_diff_density_max         1.764
_refine_diff_density_min         -2.360
_refine_diff_density_rms         0.200
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.019
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     2575
_refine_ls_number_reflns         43613
_refine_ls_number_restraints     6408
_refine_ls_R_factor_all          0.1369
_refine_ls_R_factor_gt           0.0811
_refine_ls_restrained_S_all      1.004
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.1019P)²+399.4267P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2008
_refine_ls_wR_factor_ref         0.2381
_refine_special_details          ?
_olex2_refinement_description    
;
1. Restrained distances
 O8-O16 \\sim O129-O115 \\sim O30-O13 \\sim O79-O27 \\sim O45-O15 \\sim O85-O21
 with sigma of 0.01
 O190-O170 \\sim O195-O192 \\sim O185-O164 \\sim O83-O191 \\sim O163-O160 \\sim
O188-O162 \\sim O184-
 O142 \\sim O173-O159 \\sim O194-O186 \\sim O174-O172 \\sim O193-O161 \\sim
O189-O168 \\sim O167-O166 ~
 O181-O158 \\sim O180-O179 \\sim O183-O182 \\sim O187-O171 \\sim O178-O177
 with sigma of 0.01
2. Uiso/Uaniso restraints and constraints
O1 \\sim O2 \\sim O3 \\sim O4 \\sim O5 \\sim O6 \\sim O7 \\sim O8 \\sim O9
\\sim O10 \\sim O11 \\sim O12 \\sim O13 \\sim O14 \\sim O15 \\sim O16 \\sim O17
\\sim O18 \\sim O19 \\sim O20 \\sim O21 \\sim O22 \\sim O23 \\sim O24 \\sim O25
\\sim O26 \\sim O27 \\sim O28 \\sim O29 \\sim O30 \\sim O31 \\sim O32 \\sim O33
\\sim O34 \\sim O35 \\sim O36 \\sim O37 \\sim O38 \\sim O39 \\sim O40 \\sim O41
\\sim O42 \\sim O43 \\sim O44 \\sim O45 \\sim O46 \\sim O47 \\sim O48 \\sim O49
\\sim O50 \\sim O51 \\sim O52 \\sim O53 \\sim O54 \\sim O55 \\sim O56 \\sim O57
\\sim O58 \\sim O59 \\sim O60 \\sim O61 \\sim O62 \\sim O63 \\sim O64 \\sim O65
\\sim O66 \\sim O67 \\sim O68 \\sim O69 \\sim O70 \\sim O71 \\sim O72 \\sim O73
\\sim O74 \\sim O75 \\sim O76 \\sim O77 \\sim O78 \\sim O79 \\sim O80 \\sim O81
\\sim O82 \\sim O83 \\sim O84 \\sim O85 \\sim O86 \\sim O87 \\sim O88 \\sim O89
\\sim O90 \\sim O91 \\sim O92 \\sim O93 \\sim O94 \\sim O95 \\sim O96 \\sim O97
\\sim O98 \\sim O99 \\sim O100 \\sim O101 \\sim O102 \\sim O103 \\sim O104
\\sim O105 \\sim O106 \\sim O107 \\sim O108 \\sim O109 \\sim O110 \\sim O111
\\sim O112 \\sim O113 \\sim O114 \\sim O115 \\sim O116 \\sim O117 \\sim O118
\\sim O119 \\sim O120 \\sim O121 \\sim O122 \\sim O123 \\sim O124 \\sim O125
\\sim O126 \\sim O127 \\sim O128 \\sim O129 \\sim O130 \\sim O131 \\sim O132
\\sim O133 \\sim O134 \\sim O135 \\sim O136 \\sim O137 \\sim O138 \\sim O139
\\sim O140 \\sim O141 \\sim O142 \\sim O143 \\sim O144 \\sim O145 \\sim O146
\\sim O147 \\sim O148 \\sim O149 \\sim O150 \\sim O151 \\sim O152 \\sim O153
\\sim O154 \\sim O155 \\sim O156 \\sim O157 \\sim O158 \\sim O159 \\sim O160
\\sim O161 \\sim O162 \\sim O163 \\sim O164 \\sim O165 \\sim O166 \\sim O167
\\sim O168 \\sim O169 \\sim O170 \\sim O171 \\sim O172 \\sim O173 \\sim O174
\\sim O175 \\sim O176 \\sim O177 \\sim O178 \\sim O179 \\sim O180 \\sim O181
\\sim O182 \\sim O183 \\sim O184 \\sim O185 \\sim O186 \\sim O187 \\sim O188
\\sim O189 \\sim O190 \\sim O191 \\sim O192 \\sim O193 \\sim O194 \\sim O195
\\sim O196 \\sim O197 \\sim O198 \\sim O199 \\sim O200 \\sim O201 \\sim O202
\\sim O203 \\sim O204 \\sim O205 \\sim O207 \\sim O206 \\sim O208 \\sim O209:
within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.03 within 3.8A
Mo48 \\sim Mo30 \\sim Mo52: within 3.8A with sigma of 0.01 and sigma for
terminal atoms of 0.03 within 3.8A
Mo29 \\sim Mo50: within 3.8A with sigma of 0.01 and sigma for terminal atoms of
0.03 within 3.8A
Mo44 \\sim Mo42 \\sim Mo51 \\sim Mo57: within 3.8A with sigma of 0.01 and sigma
for terminal atoms of 0.03 within 3.8A
Mo40 \\sim Mo17 \\sim Mo53 \\sim Mo54: within 3.8A with sigma of 0.01 and sigma
for terminal atoms of 0.03 within 3.8A
Mo41 \\sim Mo46 \\sim Mo47 \\sim Mo49: within 3.8A with sigma of 0.01 and sigma
for terminal atoms of 0.03 within 3.8A
Mo45 \\sim Mo39 \\sim Mo55 \\sim Mo56: within 3.8A with sigma of 0.01 and sigma
for terminal atoms of 0.03 within 3.8A
3. Others
 Fixed Sof: Mo29(0.75) Mo30(0.7) Mo39(0.35) Mo17(0.23) Mo41(0.4) Mo42(0.35)
 K1(0.7) K2(0.8) K3(0.7) Mo40(0.47) Mo44(0.35) Mo45(0.2) Mo46(0.15) Mo47(0.3)
 Mo48(0.17) Mo49(0.15) Mo50(0.25) Mo51(0.2) Mo52(0.13) Mo53(0.17) Mo54(0.13)
 Mo55(0.25) Mo56(0.2) Mo57(0.1) K4(0.5) K6(0.6) K5(0.5) K7(0.4) K8(0.4)
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.51441(7) 0.60573(3) 0.72292(3) 0.0385(3) Uani 1 1 d . . . . .
Mo2 Mo 0.91274(7) 0.95672(3) 0.69585(3) 0.0404(3) Uani 1 1 d . . . . .
Mo3 Mo 0.52674(7) 0.94979(4) 0.76355(3) 0.0424(3) Uani 1 1 d . . . . .
Mo4 Mo 0.25105(7) 0.81217(4) 0.48398(3) 0.0456(3) Uani 1 1 d . . . . .
Mo5 Mo 0.63829(8) 0.81648(4) 0.41534(3) 0.0475(3) Uani 1 1 d . . . . .
Mo6 Mo 0.64420(8) 0.99672(4) 0.65833(4) 0.0472(3) Uani 1 1 d . . . . .
Mo7 Mo 0.43338(8) 0.57672(4) 0.64476(4) 0.0535(4) Uani 1 1 d . . . . .
Mo8 Mo 0.84159(8) 1.00261(4) 0.62390(4) 0.0526(4) Uani 1 1 d . . . . .
Mo9 Mo 0.63855(9) 0.58055(4) 0.61722(4) 0.0558(4) Uani 1 1 d . . . . .
Mo10 Mo 0.40514(8) 0.67227(4) 0.75887(4) 0.0544(4) Uani 1 1 d . . . . .
Mo11 Mo 0.44682(8) 0.99566(4) 0.69303(4) 0.0546(4) Uani 1 1 d . . . . .
Mo12 Mo 0.26632(8) 0.90164(4) 0.50663(4) 0.0552(4) Uani 1 1 d . . . . .
Mo13 Mo 0.82726(9) 0.58767(4) 0.57385(4) 0.0568(4) Uani 1 1 d . . . . .
Mo14 Mo 0.46697(9) 0.90226(4) 0.47381(4) 0.0573(4) Uani 1 1 d . . . . .
Mo15 Mo 0.66476(9) 0.90518(4) 0.43823(4) 0.0560(4) Uani 1 1 d . . . . .
Mo16 Mo 0.33668(8) 0.63243(5) 0.68819(4) 0.0568(4) Uani 1 1 d . . . . .
Mo43 Mo 0.98127(8) 0.89175(4) 0.75302(4) 0.0580(4) Uani 1 1 d . . . . .
Mo18 Mo 0.78005(8) 0.89769(5) 0.78512(4) 0.0585(4) Uani 1 1 d . . . . .
Mo19 Mo 0.18484(8) 0.84806(5) 0.55820(4) 0.0607(4) Uani 1 1 d . . . . .
Mo20 Mo 0.17729(8) 0.75940(5) 0.54711(4) 0.0622(4) Uani 1 1 d . . . . .
Mo21 Mo 0.79840(9) 0.76399(5) 0.43590(4) 0.0660(5) Uani 1 1 d . . . . .
Mo22 Mo 0.41567(9) 0.87764(5) 0.78644(4) 0.0645(4) Uani 1 1 d . . . . .
Mo23 Mo 0.34866(8) 0.93102(5) 0.72406(4) 0.0632(4) Uani 1 1 d . . . . .
Mo24 Mo 0.44062(9) 0.72813(5) 0.44426(4) 0.0642(4) Uani 1 1 d . . . . .
Mo25 Mo 0.81093(9) 0.85185(5) 0.44856(4) 0.0655(4) Uani 1 1 d . . . . .
Mo26 Mo 0.24790(9) 0.71810(5) 0.48408(5) 0.0678(5) Uani 1 1 d . . . . .
Mo27 Mo 0.58619(9) 0.88556(5) 0.82277(4) 0.0637(4) Uani 1 1 d . . . . .
Mo28 Mo 0.64136(10) 0.72284(5) 0.41138(4) 0.0680(5) Uani 1 1 d . . . . .
Mo29 Mo 0.65131(13) 0.70465(7) 0.54772(6) 0.0522(6) Uani 0.75 1 d . U P A 1
Mo30 Mo 0.44889(15) 0.70438(7) 0.58790(6) 0.0410(5) Uani 0.7 1 d . U P A 1
Mo31 Mo 0.97090(7) 0.66373(4) 0.72339(3) 0.0444(3) Uani 1 1 d . . . . .
Mo32 Mo 0.77124(7) 0.66038(4) 0.75657(3) 0.0470(3) Uani 1 1 d . . . . .
Mo33 Mo 0.57501(8) 0.65686(4) 0.79334(3) 0.0437(3) Uani 1 1 d . . . . .
Mo34 Mo 0.90034(7) 0.61469(3) 0.65336(3) 0.0385(3) Uani 1 1 d . . . . .
Mo35 Mo 0.97167(9) 0.94206(5) 0.61467(4) 0.0667(5) Uani 1 1 d . . . . .
Mo36 Mo 1.03933(8) 0.88886(4) 0.67671(5) 0.0621(4) Uani 1 1 d . . . . .
Mo37 Mo 0.95813(8) 0.65011(5) 0.57810(4) 0.0605(4) Uani 1 1 d . . . . .
Mo38 Mo 1.02926(8) 0.68612(4) 0.65010(4) 0.0551(4) Uani 1 1 d . . . . .
Mo39 Mo 0.6269(4) 0.78058(12) 0.72604(16) 0.0351(10) Uani 0.35 1 d . U P A 1
Mo17 Mo 0.8149(5) 0.78053(17) 0.7164(2) 0.0354(13) Uani 0.23 1 d . U P A 1
Mo41 Mo 0.6588(3) 0.90589(13) 0.56684(10) 0.0378(8) Uani 0.4 1 d . U P B 1
Mo42 Mo 0.4932(3) 0.90381(14) 0.59535(12) 0.0290(9) Uani 0.35 1 d . U P B 1
Ti1 Ti 0.61128(13) 0.68259(6) 0.71720(6) 0.0303(5) Uani 1 1 d . . . . .
Ti2 Ti 0.54711(13) 0.64591(7) 0.65054(6) 0.0331(5) Uani 1 1 d . . . . .
Ti3 Ti 0.40471(14) 0.84555(7) 0.52716(6) 0.0348(6) Uani 1 1 d . . . . .
Ti4 Ti 0.62159(14) 0.87704(6) 0.74322(7) 0.0374(6) Uani 1 1 d . . . . .
Ti5 Ti 0.55823(13) 0.92613(7) 0.68438(6) 0.0355(6) Uani 1 1 d . . . . .
Ti6 Ti 0.39503(14) 0.76273(7) 0.51542(6) 0.0374(6) Uani 1 1 d . . . . .
Ti7 Ti 0.82068(13) 0.88073(6) 0.70804(7) 0.0374(6) Uani 1 1 d . . . . .
Ti8 Ti 0.59306(14) 0.76495(7) 0.47880(6) 0.0377(6) Uani 1 1 d . . . . .
Ti9 Ti 0.60471(14) 0.84728(7) 0.49251(6) 0.0362(6) Uani 1 1 d . . . . .
Ti10 Ti 0.75781(13) 0.92969(7) 0.64926(6) 0.0368(6) Uani 1 1 d . . . . .
Ti11 Ti 0.81112(13) 0.68669(6) 0.68215(6) 0.0309(5) Uani 1 1 d . . . . .
Ti12 Ti 0.74627(13) 0.65096(7) 0.61551(6) 0.0325(5) Uani 1 1 d . . . . .
K1 K 0.6412(4) 0.7589(2) 0.6372(2) 0.101(2) Uani 0.7 1 d . . P A .
K2 K 0.6929(4) 0.56158(15) 0.79096(16) 0.092(2) Uani 0.8 1 d . . P . .
K3 K 0.8949(6) 0.5627(2) 0.7535(2) 0.116(3) Uani 0.7 1 d . . P . .
O1 O 0.5936(5) 0.6288(3) 0.6991(2) 0.0454(15) Uani 1 1 d . U . . .
O2 O 0.6456(6) 0.6334(3) 0.6311(3) 0.0499(15) Uani 1 1 d . U . . .
O3 O 0.6045(6) 0.9325(3) 0.7353(3) 0.0517(15) Uani 1 1 d . U . . .
O4 O 0.8907(6) 1.0017(3) 0.6862(3) 0.0618(18) Uani 1 1 d . U . . .
O5 O 0.7035(6) 0.9927(3) 0.7164(3) 0.0651(18) Uani 1 1 d . U . . .
O6 O 0.7329(6) 0.8845(3) 0.7378(3) 0.0542(15) Uani 1 1 d . U . . .
O7 O 0.5399(6) 0.5933(3) 0.6361(3) 0.0597(17) Uani 1 1 d . U . . .
O8 O 0.6013(5) 0.6928(3) 0.6665(2) 0.0478(15) Uani 1 1 d D U . . .
O9 O 0.2676(7) 0.6796(4) 0.5059(3) 0.079(2) Uani 1 1 d . U . . .
O10 O 0.4097(8) 0.7638(4) 0.4171(3) 0.086(3) Uani 1 1 d . U . . .
O11 O 0.4831(6) 0.7576(3) 0.4845(3) 0.0582(15) Uani 1 1 d . U . . .
O12 O 0.6121(6) 0.7293(3) 0.7308(3) 0.0515(16) Uani 1 1 d . U . . .
O13 O 0.4634(5) 0.8002(3) 0.5412(2) 0.0520(16) Uani 1 1 d D U . . .
O14 O 0.6478(6) 0.8731(3) 0.5274(3) 0.0592(16) Uani 1 1 d . U . . .
O15 O 0.5348(5) 0.8757(3) 0.7048(3) 0.0555(16) Uani 1 1 d D U . . .
O16 O 0.5245(5) 0.6906(3) 0.6798(3) 0.0499(15) Uani 1 1 d D U . . .
O17 O 0.7108(6) 0.6708(3) 0.5755(3) 0.0573(16) Uani 1 1 d . U . . .
O18 O 0.7872(7) 0.6010(4) 0.5342(3) 0.074(3) Uani 1 1 d . U . . .
O19 O 0.4153(6) 0.6158(3) 0.7345(3) 0.0548(18) Uani 1 1 d . U . . .
O20 O 0.5340(6) 0.8873(3) 0.7729(3) 0.0604(16) Uani 1 1 d . U . . .
O21 O 0.8159(5) 0.8810(3) 0.6558(3) 0.0575(15) Uani 1 1 d D U . . .
O22 O 0.3728(6) 0.8875(3) 0.4949(3) 0.0609(16) Uani 1 1 d . U . . .
O23 O 0.5704(6) 0.8897(3) 0.4615(3) 0.0629(16) Uani 1 1 d . U . . .
O24 O 0.8120(6) 0.9365(3) 0.6985(3) 0.0521(15) Uani 1 1 d . U . . .
O25 O 0.4530(6) 0.6254(3) 0.6717(3) 0.0555(15) Uani 1 1 d . U . . .
O26 O 0.8641(6) 0.9490(3) 0.6391(3) 0.0595(16) Uani 1 1 d . U . . .
O27 O 0.5892(5) 0.8005(3) 0.5187(3) 0.0540(16) Uani 1 1 d D U . . .
O28 O 0.8902(7) 0.8504(4) 0.4244(4) 0.087(4) Uani 1 1 d . U . . .
O29 O 0.2203(6) 0.8002(3) 0.5732(3) 0.0668(18) Uani 1 1 d . U . . .
O30 O 0.3871(5) 0.7992(3) 0.5551(3) 0.0563(16) Uani 1 1 d D U . . .
O31 O 0.6308(6) 0.7269(3) 0.5051(3) 0.0590(17) Uani 1 1 d . U . . .
O32 O 0.5091(6) 0.9159(3) 0.6434(3) 0.0588(16) Uani 1 1 d . U . . .
O33 O 0.7733(7) 0.9451(3) 0.7819(3) 0.075(3) Uani 1 1 d . U . . .
O34 O 0.6476(7) 0.9456(3) 0.5480(3) 0.074(2) Uani 1 1 d . U . . .
O35 O 0.8677(6) 0.8920(3) 0.7555(3) 0.0629(16) Uani 1 1 d . U . . .
O36 O 0.3553(7) 0.7315(3) 0.4755(3) 0.0679(18) Uani 1 1 d . U . . .
O37 O 0.8260(6) 0.7337(3) 0.6936(3) 0.0533(16) Uani 1 1 d . U . . .
O38 O 0.6229(6) 0.8279(3) 0.7475(3) 0.0586(17) Uani 1 1 d . U . . .
O39 O 0.4664(6) 0.6503(3) 0.7976(3) 0.0606(19) Uani 1 1 d . U . . .
O40 O 0.3190(7) 0.6611(4) 0.7756(3) 0.076(3) Uani 1 1 d . U . . .
O41 O 0.4649(6) 0.9414(3) 0.7091(3) 0.0590(16) Uani 1 1 d . U . . .
O42 O 0.6131(6) 0.8586(3) 0.3980(3) 0.0627(19) Uani 1 1 d . U . . .
O43 O 0.5183(6) 0.9949(3) 0.7510(3) 0.0634(18) Uani 1 1 d . U . . .
O44 O 0.2906(6) 0.8516(3) 0.5295(3) 0.0586(15) Uani 1 1 d . U . . .
O45 O 0.6111(5) 0.8773(3) 0.6912(3) 0.0530(16) Uani 1 1 d D U . . .
O46 O 0.7426(6) 0.8146(3) 0.4104(3) 0.0622(19) Uani 1 1 d . U . . .
O47 O 0.9474(7) 0.9940(3) 0.6162(3) 0.0686(19) Uani 1 1 d . U . . .
O48 O 0.5756(7) 0.9506(3) 0.8034(3) 0.0645(19) Uani 1 1 d . U . . .
O49 O 0.5633(6) 0.5963(3) 0.7620(3) 0.0565(18) Uani 1 1 d . U . . .
O50 O 0.8177(7) 0.7281(4) 0.4631(3) 0.083(3) Uani 1 1 d . U . . .
O51 O 0.0821(7) 0.7637(4) 0.5547(3) 0.074(2) Uani 1 1 d . U . . .
O52 O 0.3292(8) 0.8849(4) 0.8045(4) 0.088(4) Uani 1 1 d . U . . .
O53 O 0.2295(6) 0.7788(3) 0.4531(3) 0.065(3) Uani 1 1 d . U . . .
O54 O 0.9485(6) 0.9571(3) 0.7383(3) 0.0627(18) Uani 1 1 d . U . . .
O55 O 0.6018(7) 0.7849(3) 0.3866(3) 0.068(3) Uani 1 1 d . U . . .
O56 O 0.2362(6) 0.8540(3) 0.4631(3) 0.0615(19) Uani 1 1 d . U . . .
O57 O 0.4264(8) 0.8314(4) 0.7866(4) 0.089(4) Uani 1 1 d . U . . .
O58 O 0.5805(6) 0.8933(3) 0.5864(3) 0.0632(17) Uani 1 1 d . U . . .
O59 O 0.5827(6) 0.6054(3) 0.5677(3) 0.066(3) Uani 1 1 d . U . . .
O60 O 0.3886(7) 0.5895(4) 0.6063(3) 0.074(3) Uani 1 1 d . U . . .
O61 O 0.6976(7) 0.9344(4) 0.4681(3) 0.074(3) Uani 1 1 d . U . . .
O62 O 0.8773(7) 0.7679(4) 0.4131(3) 0.079(3) Uani 1 1 d . U . . .
O63 O 0.7622(7) 0.8905(3) 0.4200(3) 0.067(2) Uani 1 1 d . U . . .
O64 O 0.4808(7) 0.6818(3) 0.4795(3) 0.077(3) Uani 1 1 d . U . . .
O65 O 0.4794(7) 0.8915(4) 0.8286(3) 0.074(2) Uani 1 1 d . U . . .
O66 O 0.8134(6) 0.8040(3) 0.4676(3) 0.064(2) Uani 1 1 d . U . . .
O67 O 0.4338(6) 0.8718(3) 0.5647(3) 0.0566(16) Uani 1 1 d . U . . .
O68 O 0.7481(6) 0.9854(3) 0.6468(3) 0.0601(16) Uani 1 1 d . U . . .
O69 O 0.9960(7) 0.8466(3) 0.7595(3) 0.075(3) Uani 1 1 d . U . . .
O70 O 0.4944(7) 0.9366(3) 0.5038(3) 0.0699(18) Uani 1 1 d . U . . .
O71 O 0.1686(6) 0.8096(3) 0.5115(3) 0.0627(18) Uani 1 1 d . U . . .
O72 O 0.7730(7) 0.7065(4) 0.5252(3) 0.077(2) Uani 1 1 d . U . . .
O73 O 0.3615(6) 0.8099(3) 0.4885(3) 0.0522(16) Uani 1 1 d . U . . .
O74 O 0.2106(7) 0.7256(4) 0.5735(3) 0.077(2) Uani 1 1 d . U . . .
O75 O 0.7410(7) 0.7381(4) 0.3980(3) 0.074(2) Uani 1 1 d . U . . .
O76 O 0.0905(7) 0.8448(4) 0.5648(3) 0.074(2) Uani 1 1 d . U . . .
O77 O 0.3602(6) 0.9841(3) 0.7199(3) 0.0673(19) Uani 1 1 d . U . . .
O78 O 0.5687(6) 0.8125(3) 0.4516(3) 0.0539(16) Uani 1 1 d . U . . .
O79 O 0.6663(5) 0.8012(3) 0.5055(3) 0.0559(16) Uani 1 1 d D U . . .
O80 O 0.5636(7) 0.7882(3) 0.6931(3) 0.0672(18) Uani 1 1 d . U . . .
O81 O 0.4606(7) 0.9439(3) 0.5815(3) 0.0753(19) Uani 1 1 d . U . . .
O82 O 0.5229(7) 0.7754(3) 0.7642(3) 0.075(2) Uani 1 1 d . U . . .
O83 O 0.4692(7) 0.5296(4) 0.6368(3) 0.080(2) Uani 1 1 d D U . . .
O84 O 0.6712(6) 0.8891(3) 0.7906(3) 0.0646(17) Uani 1 1 d . U . . .
O85 O 0.7384(5) 0.8793(3) 0.6684(3) 0.0553(16) Uani 1 1 d D U . . .
O86 O 0.2265(7) 0.8715(4) 0.5923(3) 0.073(2) Uani 1 1 d . U . . .
O87 O 0.4920(7) 0.7404(3) 0.6077(3) 0.0682(18) Uani 1 1 d . U . . .
O88 O 0.2802(6) 0.7609(3) 0.5175(3) 0.0614(16) Uani 1 1 d . U . . .
O89 O 0.1561(7) 0.7309(3) 0.5035(3) 0.0728(19) Uani 1 1 d . U . . .
O90 O 0.4226(6) 0.7252(3) 0.5438(3) 0.0607(16) Uani 1 1 d . U . . .
O91 O 0.8327(6) 0.8317(3) 0.7104(3) 0.0590(16) Uani 1 1 d . U . . .
O92 O 0.4027(7) 0.9928(4) 0.6538(3) 0.074(3) Uani 1 1 d . U . . .
O93 O 0.8046(7) 0.9995(4) 0.5836(3) 0.077(3) Uani 1 1 d . U . . .
O94 O 0.2684(7) 0.9353(4) 0.7477(4) 0.085(4) Uani 1 1 d . U . . .
O95 O 0.7906(7) 0.8349(3) 0.7893(3) 0.074(3) Uani 1 1 d . U . . .
O96 O 0.7355(6) 0.5990(3) 0.5999(3) 0.0589(16) Uani 1 1 d . U . . .
O97 O 0.5518(6) 0.9813(3) 0.6814(3) 0.0594(15) Uani 1 1 d . U . . .
O98 O 0.4962(6) 0.8567(3) 0.5014(3) 0.0560(14) Uani 1 1 d . U . . .
O99 O 0.6569(6) 0.9432(3) 0.6662(3) 0.0543(14) Uani 1 1 d . U . . .
O100 O 0.6880(6) 0.8546(3) 0.4598(3) 0.0588(16) Uani 1 1 d . U . . .
O101 O 0.5521(7) 0.7343(3) 0.4386(3) 0.0672(18) Uani 1 1 d . U . . .
O102 O 0.5234(6) 0.6652(3) 0.7440(3) 0.0532(15) Uani 1 1 d . U . . .
O103 O 0.5638(7) 0.6977(3) 0.5600(3) 0.0669(18) Uani 1 1 d . U . . .
O104 O 0.6760(6) 0.7643(3) 0.4456(3) 0.0631(16) Uani 1 1 d . U . . .
O105 O 0.3831(6) 0.8830(3) 0.7382(3) 0.063(2) Uani 1 1 d . U . . .
O106 O 0.5058(6) 0.5639(3) 0.7026(3) 0.060(3) Uani 1 1 d . U . . .
O107 O 0.6026(6) 0.9980(3) 0.6170(3) 0.0646(18) Uani 1 1 d . U . . .
O108 O 0.5000(6) 0.6650(3) 0.6124(3) 0.0559(16) Uani 1 1 d . U . . .
O109 O 0.7242(6) 0.9195(3) 0.6055(3) 0.0595(16) Uani 1 1 d . U . . .
O110 O 0.9219(6) 0.6744(3) 0.6746(3) 0.0538(15) Uani 1 1 d . U . . .
O111 O 0.8565(6) 0.6630(3) 0.7260(3) 0.0541(15) Uani 1 1 d . U . . .
O112 O 0.8008(6) 0.6336(3) 0.6616(3) 0.0476(15) Uani 1 1 d . U . . .
O113 O 0.8501(6) 0.6362(3) 0.6010(3) 0.0567(16) Uani 1 1 d . U . . .
O114 O 0.7237(6) 0.6780(3) 0.7111(3) 0.0498(14) Uani 1 1 d . U . . .
O115 O 0.7279(5) 0.6961(3) 0.6445(3) 0.0510(15) Uani 1 1 d D U . . .
O116 O 1.0651(6) 0.9022(3) 0.7258(3) 0.0664(18) Uani 1 1 d . U . . .
O117 O 0.9874(6) 0.7050(3) 0.7412(3) 0.062(3) Uani 1 1 d . U . . .
O118 O 0.9310(6) 0.8947(3) 0.7027(3) 0.0610(16) Uani 1 1 d . U . . .
O119 O 0.6607(6) 0.6601(3) 0.7611(3) 0.0538(15) Uani 1 1 d . U . . .
O120 O 0.9355(6) 0.6042(3) 0.6943(3) 0.0569(17) Uani 1 1 d . U . . .
O121 O 0.6811(7) 0.5618(4) 0.6559(3) 0.078(3) Uani 1 1 d . U . . .
O122 O 0.7914(6) 0.7032(3) 0.7771(3) 0.062(3) Uani 1 1 d . U . . .
O123 O 1.0553(6) 0.6612(3) 0.6947(3) 0.0616(18) Uani 1 1 d . U . . .
O124 O 0.4270(6) 0.9372(3) 0.7734(3) 0.0615(18) Uani 1 1 d . U . . .
O125 O 1.1174(6) 0.6770(3) 0.6352(3) 0.069(2) Uani 1 1 d . U . . .
O126 O 0.1692(6) 0.8864(3) 0.5223(3) 0.0677(18) Uani 1 1 d . U . . .
O127 O 0.3127(7) 0.9212(4) 0.6840(3) 0.074(2) Uani 1 1 d . U . . .
O128 O 0.8786(6) 0.5739(3) 0.6339(3) 0.0620(18) Uani 1 1 d . U . . .
O129 O 0.8043(5) 0.6974(3) 0.6308(3) 0.0540(15) Uani 1 1 d D U . . .
O130 O 0.3493(7) 0.5811(3) 0.6734(3) 0.068(2) Uani 1 1 d . U . . .
O131 O 0.3667(7) 0.9032(4) 0.6178(3) 0.071(2) Uani 1 1 d . U . . .
O132 O 0.7424(6) 0.6048(3) 0.7246(3) 0.0627(17) Uani 1 1 d . U . . .
O133 O 1.0414(7) 0.8425(3) 0.6783(3) 0.075(2) Uani 1 1 d . U . . .
O134 O 1.1282(6) 0.9008(3) 0.6644(3) 0.071(2) Uani 1 1 d . U . . .
O135 O 0.9340(7) 0.5986(3) 0.5679(3) 0.0667(19) Uani 1 1 d . U . . .
O136 O 0.7826(7) 0.9067(4) 0.5455(3) 0.076(2) Uani 1 1 d . U . . .
O137 O 0.9883(6) 0.6293(3) 0.6325(3) 0.0582(17) Uani 1 1 d . U . . .
O138 O 1.0506(6) 0.6451(3) 0.5673(3) 0.069(2) Uani 1 1 d . U . . .
O139 O 0.5865(7) 0.6983(3) 0.8108(3) 0.062(3) Uani 1 1 d . U . . .
O140 O 0.7193(6) 0.7806(3) 0.7174(3) 0.0629(17) Uani 1 1 d . U . . .
O141 O 0.8403(7) 0.8763(4) 0.4840(3) 0.083(3) Uani 1 1 d . U . . .
O142 O 0.8007(7) 0.5383(4) 0.5765(3) 0.077(2) Uani 1 1 d D U . . .
O143 O 0.9781(6) 0.8947(3) 0.6343(3) 0.0686(17) Uani 1 1 d . U . . .
O144 O 0.3614(7) 0.7005(4) 0.6028(3) 0.078(2) Uani 1 1 d . U . . .
O145 O 0.4170(7) 0.7178(3) 0.7689(3) 0.072(3) Uani 1 1 d . U . . .
O146 O 0.3732(6) 0.6764(3) 0.7117(3) 0.0567(19) Uani 1 1 d . U . . .
O147 O 1.0009(6) 0.9485(3) 0.6728(3) 0.0601(17) Uani 1 1 d . U . . .
O148 O 0.4284(7) 0.8535(4) 0.4349(3) 0.080(3) Uani 1 1 d . U . . .
O149 O 0.9122(7) 0.6707(4) 0.5433(3) 0.074(3) Uani 1 1 d . U . . .
O150 O 0.2569(6) 0.6235(4) 0.7109(3) 0.074(3) Uani 1 1 d . U . . .
O151 O 1.0327(7) 0.7314(3) 0.6627(3) 0.071(2) Uani 1 1 d . U . . .
O152 O 0.2916(7) 0.9316(3) 0.5375(3) 0.076(3) Uani 1 1 d . U . . .
O153 O 0.7872(7) 0.7922(3) 0.6528(3) 0.0698(17) Uani 1 1 d . U . . .
O154 O 0.9672(6) 0.6925(3) 0.6080(3) 0.0639(18) Uani 1 1 d . U . . .
O155 O 0.9286(8) 0.9318(4) 0.5763(4) 0.087(3) Uani 1 1 d . U . . .
O156 O 1.0668(7) 0.9504(4) 0.6069(3) 0.075(2) Uani 1 1 d . U . . .
O157 O 0.6802(7) 0.7693(3) 0.7836(3) 0.073(2) Uani 1 1 d . U . . .
O158 O 0.4879(7) 1.0437(4) 0.6944(3) 0.082(2) Uani 1 1 d D U . . .
O159 O 0.8552(7) 0.8965(4) 0.8216(3) 0.081(2) Uani 1 1 d D U . . .
O160 O 0.5872(7) 0.5386(3) 0.6013(3) 0.077(2) Uani 1 1 d D U . . .
O161 O 0.2350(8) 0.7026(4) 0.4385(4) 0.087(2) Uani 1 1 d D U . . .
O162 O 0.9733(7) 0.6330(3) 0.7611(3) 0.072(2) Uani 1 1 d D U . . .
O163 O 0.6490(7) 0.5407(3) 0.5888(3) 0.075(2) Uani 1 1 d D U . . .
O164 O 0.6393(7) 0.6284(3) 0.8205(3) 0.070(2) Uani 1 1 d D U . . .
O165 O 0.9335(7) 0.7856(3) 0.6881(4) 0.079(2) Uani 1 1 d . U . . .
O166 O 0.6194(7) 1.0438(3) 0.6743(3) 0.0754(19) Uani 1 1 d D U . . .
O167 O 0.6806(7) 1.0446(4) 0.6624(3) 0.0768(19) Uani 1 1 d D U . . .
O168 O 0.9907(7) 0.9110(4) 0.7964(3) 0.080(2) Uani 1 1 d D U . . .
O169 O 0.6448(8) 0.6549(4) 0.5125(3) 0.079(2) Uani 1 1 d . U . . .
O170 O 0.8144(7) 1.0487(4) 0.6383(3) 0.079(2) Uani 1 1 d D U . . .
O171 O 0.5721(8) 0.7076(4) 0.3772(3) 0.088(2) Uani 1 1 d D U . . .
O172 O 0.3802(7) 0.6912(4) 0.4228(3) 0.084(2) Uani 1 1 d D U . . .
O173 O 0.7922(7) 0.8948(4) 0.8326(3) 0.081(2) Uani 1 1 d D U . . .
O174 O 0.4427(7) 0.6921(4) 0.4106(3) 0.083(2) Uani 1 1 d D U . . .
O175 O 0.4211(8) 0.6525(4) 0.5520(3) 0.081(2) Uani 1 1 d . U . . .
O176 O 0.7186(7) 0.8491(3) 0.5873(3) 0.0696(18) Uani 1 1 d . U . . .
O177 O 0.6536(7) 0.9336(4) 0.3991(3) 0.082(2) Uani 1 1 d D U . . .
O178 O 0.5931(7) 0.9343(4) 0.4119(3) 0.081(2) Uani 1 1 d D U . . .
O179 O 0.2028(7) 0.9293(4) 0.4770(3) 0.080(2) Uani 1 1 d D U . . .
O180 O 0.2659(7) 0.9308(4) 0.4673(3) 0.077(2) Uani 1 1 d D U . . .
O181 O 0.4280(7) 1.0423(4) 0.7060(4) 0.084(2) Uani 1 1 d D U . . .
O182 O 0.4661(7) 0.9301(4) 0.4350(3) 0.083(2) Uani 1 1 d D U . . .
O183 O 0.4042(7) 0.9296(4) 0.4454(3) 0.082(2) Uani 1 1 d D U . . .
O184 O 0.8615(7) 0.5415(4) 0.5660(4) 0.088(2) Uani 1 1 d D U . . .
O185 O 0.5786(7) 0.6257(4) 0.8320(3) 0.080(2) Uani 1 1 d D U . . .
O186 O 0.6551(7) 0.9081(4) 0.8553(3) 0.082(2) Uani 1 1 d D U . . .
O187 O 0.6293(8) 0.7144(4) 0.3645(4) 0.100(3) Uani 1 1 d D U . . .
O188 O 1.0333(7) 0.6331(4) 0.7489(3) 0.078(2) Uani 1 1 d D U . . .
O189 O 1.0494(7) 0.9154(4) 0.7842(4) 0.090(2) Uani 1 1 d D U . . .
O190 O 0.8764(7) 1.0494(4) 0.6283(4) 0.086(2) Uani 1 1 d D U . . .
O191 O 0.4102(8) 0.5288(4) 0.6490(4) 0.090(2) Uani 1 1 d D U . . .
O192 O 0.7760(7) 0.6306(3) 0.7947(3) 0.073(2) Uani 1 1 d D U . . .
O193 O 0.1740(8) 0.7030(4) 0.4494(4) 0.096(2) Uani 1 1 d D U . . .
O194 O 0.5927(7) 0.9089(4) 0.8646(4) 0.089(2) Uani 1 1 d D U . . .
O195 O 0.8377(7) 0.6312(3) 0.7831(3) 0.076(2) Uani 1 1 d D U . . .
O196 O 0.5949(8) 0.8410(4) 0.8322(4) 0.087(3) Uani 1 1 d . U . . .
O197 O 0.6839(7) 0.7453(3) 0.5705(3) 0.0704(17) Uani 1 1 d . U . . .
O198 O 0.3003(7) 0.6495(4) 0.6506(3) 0.073(2) Uani 1 1 d . U . . .
O199 O 0.6688(8) 0.6840(4) 0.4317(4) 0.087(3) Uani 1 1 d . U . . .
O200 O 0.4855(7) 0.8454(3) 0.6278(3) 0.0667(18) Uani 1 1 d . U . . .
O201 O 0.5865(5) 0.8050(3) 0.5913(2) 0.048(2) Uani 1 1 d . U . . .
Mo40 Mo 0.8366(2) 0.78515(8) 0.68709(10) 0.0370(7) Uani 0.47 1 d . U P A 2
O202 O 0.8710(7) 0.7729(3) 0.7495(3) 0.079(2) Uani 1 1 d . U . . .
Mo44 Mo 0.4506(3) 0.90416(15) 0.60275(13) 0.0422(10) Uani 0.35 1 d . U P B 2
Mo45 Mo 0.6127(6) 0.7766(2) 0.7532(3) 0.0395(16) Uani 0.2 1 d . U P A 2
Mo46 Mo 0.7100(6) 0.8839(3) 0.5682(3) 0.0388(19) Uani 0.15 1 d . U P A 2
Mo47 Mo 0.7016(3) 0.90576(16) 0.55910(12) 0.0325(10) Uani 0.3 1 d . U P B 3
O203 O 0.8140(11) 0.5231(5) 0.7001(5) 0.127(5) Uani 1 1 d . U . . .
O204 O 0.6606(10) 0.5225(4) 0.7278(4) 0.117(5) Uani 1 1 d . U . . .
Mo48 Mo 0.4899(5) 0.7018(2) 0.5767(2) 0.0404(18) Uani 0.17 1 d . U P A 2
Mo49 Mo 0.6669(7) 0.8859(4) 0.5753(3) 0.038(2) Uani 0.15 1 d . U P B 4
Mo50 Mo 0.6925(5) 0.7091(2) 0.5433(2) 0.0612(19) Uani 0.25 1 d . U P A 2
Mo51 Mo 0.4528(5) 0.8819(2) 0.61195(17) 0.0338(14) Uani 0.2 1 d . U P B 3
Mo52 Mo 0.4402(7) 0.6870(4) 0.5756(3) 0.041(2) Uani 0.13 1 d . U P A 3
Mo53 Mo 0.8003(6) 0.7841(2) 0.6970(3) 0.0345(19) Uani 0.17 1 d . U P A 3
Mo54 Mo 0.8569(7) 0.7806(3) 0.7100(4) 0.032(2) Uani 0.13 1 d . U P A 4
Mo55 Mo 0.6501(5) 0.77727(17) 0.7430(2) 0.0328(13) Uani 0.25 1 d . U P A 3
Mo56 Mo 0.5871(5) 0.7802(2) 0.7332(3) 0.0344(15) Uani 0.2 1 d . U P A 4
Mo57 Mo 0.4941(14) 0.8885(6) 0.6025(5) 0.039(3) Uani 0.1 1 d . U P B 4
O205 O 0.6399(10) 0.8232(5) 0.6404(5) 0.120(4) Uani 1 1 d . U . . .
K4 K 0.5425(6) 0.9983(2) 0.5482(2) 0.088(3) Uani 0.5 1 d . . P B .
K6 K 0.2219(6) 0.6505(3) 0.5847(2) 0.112(3) Uani 0.6 1 d . . P A .
O207 O 0.3971(8) 0.9993(4) 0.5189(4) 0.095(3) Uani 1 1 d . U . . .
K5 K 0.2295(6) 0.9433(4) 0.6228(3) 0.120(4) Uani 0.5 1 d . . P B .
K7 K 0.8084(7) 0.7998(5) 0.5430(3) 0.111(5) Uani 0.4 1 d . . P A .
K8 K 1.0208(8) 0.7933(4) 0.6182(3) 0.098(4) Uani 0.4 1 d . . P A .
O206 O 0.3288(7) 0.9875(3) 0.5870(3) 0.069(3) Uani 1 1 d . U . . .
O208 O 0.8765(8) 0.7570(4) 0.5943(4) 0.086(2) Uani 1 1 d . U . . .
O209 O 0.8953(8) 0.8363(4) 0.6024(4) 0.091(2) Uani 1 1 d . U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 Ti1 3.293(3) . ?
Mo1 Ti2 3.268(3) . ?
Mo1 O1 1.910(9) . ?
Mo1 O19 1.847(11) . ?
Mo1 O25 2.314(11) . ?
Mo1 O49 1.730(10) . ?
Mo1 O102 2.328(11) . ?
Mo1 O106 1.726(11) . ?
Mo2 Ti7 3.259(3) . ?
Mo2 Ti10 3.296(3) . ?
Mo2 O4 1.725(11) . ?
Mo2 O24 1.910(10) . ?
Mo2 O26 2.332(11) . ?
Mo2 O54 1.729(11) . ?
Mo2 O118 2.304(11) . ?
Mo2 O147 1.852(11) . ?
Mo3 Ti4 3.257(3) . ?
Mo3 Ti5 3.290(3) . ?
Mo3 O3 1.909(10) . ?
Mo3 O20 2.318(11) . ?
Mo3 O41 2.335(11) . ?
Mo3 O43 1.725(11) . ?
Mo3 O48 1.719(12) . ?
Mo3 O124 1.858(11) . ?
Mo4 Ti3 3.293(3) . ?
Mo4 Ti6 3.259(3) . ?
Mo4 O44 2.355(11) . ?
Mo4 O53 1.737(11) . ?
Mo4 O56 1.744(11) . ?
Mo4 O71 1.849(11) . ?
Mo4 O73 1.917(10) . ?
Mo4 O88 2.322(11) . ?
Mo5 Ti8 3.251(3) . ?
Mo5 Ti9 3.304(3) . ?
Mo5 O42 1.726(11) . ?
Mo5 O46 1.838(11) . ?
Mo5 O55 1.702(12) . ?
Mo5 O78 1.928(10) . ?
Mo5 O100 2.346(11) . ?
Mo5 O104 2.317(11) . ?
Mo6 Ti5 3.185(3) . ?
Mo6 Ti10 3.184(3) . ?
Mo6 K2 4.098(6) 2_656 ?
Mo6 O5 2.429(12) . ?
Mo6 O68 1.936(11) . ?
Mo6 O97 1.975(11) . ?
Mo6 O99 1.993(11) . ?
Mo6 O107 1.724(11) . ?
Mo6 O166 1.892(13) . ?
Mo6 O167 1.866(13) . ?
Mo7 Mo16 3.200(2) . ?
Mo7 Ti2 3.210(3) . ?
Mo7 O7 1.999(11) . ?
Mo7 O25 2.086(11) . ?
Mo7 O60 1.706(12) . ?
Mo7 O83 1.866(14) . ?
Mo7 O130 1.905(12) . ?
Mo7 O191 1.810(14) . ?
Mo8 Mo35 3.203(2) . ?
Mo8 Ti10 3.227(3) . ?
Mo8 K2 4.040(6) 2_656 ?
Mo8 O26 2.078(11) . ?
Mo8 O47 1.909(12) . ?
Mo8 O68 2.009(11) . ?
Mo8 O93 1.663(13) . ?
Mo8 O170 1.849(13) . ?
Mo8 O190 1.819(14) . ?
Mo9 Ti2 3.196(3) . ?
Mo9 Ti12 3.188(3) . ?
Mo9 O2 2.008(10) . ?
Mo9 O7 1.968(11) . ?
Mo9 O59 2.289(11) . ?
Mo9 O96 1.975(11) . ?
Mo9 O121 1.771(12) . ?
Mo9 O160 1.861(12) . ?
Mo9 O163 1.849(12) . ?
Mo10 Mo33 3.209(2) . ?
Mo10 O19 2.288(11) . ?
Mo10 O39 1.962(11) . ?
Mo10 O40 1.723(12) . ?
Mo10 O102 2.188(11) . ?
Mo10 O145 1.720(12) . ?
Mo10 O146 1.892(11) . ?
Mo11 Mo23 3.202(2) . ?
Mo11 Ti5 3.229(3) . ?
Mo11 O41 2.099(11) . ?
Mo11 O43 2.504(12) . ?
Mo11 O77 1.939(12) . ?
Mo11 O92 1.668(12) . ?
Mo11 O97 1.981(11) . ?
Mo11 O158 1.895(14) . ?
Mo11 O181 1.815(14) . ?
Mo12 Mo19 3.207(2) . ?
Mo12 Ti3 3.221(3) . ?
Mo12 O22 2.004(11) . ?
Mo12 O44 2.069(11) . ?
Mo12 O56 2.464(12) . ?
Mo12 O126 1.917(12) . ?
Mo12 O152 1.665(13) . ?
Mo12 O179 1.845(12) . ?
Mo12 O180 1.869(13) . ?
Mo13 Mo37 3.220(2) . ?
Mo13 Ti12 3.209(3) . ?
Mo13 O18 1.722(12) . ?
Mo13 O96 1.994(11) . ?
Mo13 O113 2.090(11) . ?
Mo13 O128 2.501(11) . ?
Mo13 O135 1.926(12) . ?
Mo13 O142 1.870(13) . ?
Mo13 O184 1.824(14) . ?
Mo14 Ti3 3.181(3) . ?
Mo14 Ti9 3.173(3) . ?
Mo14 O22 1.958(11) . ?
Mo14 O23 1.947(11) . ?
Mo14 O70 1.760(12) . ?
Mo14 O98 2.029(11) . ?
Mo14 O148 2.407(13) . ?
Mo14 O182 1.824(13) . ?
Mo14 O183 1.805(13) . ?
Mo14 K4 3.739(9) 3_676 ?
Mo15 Mo25 3.207(2) . ?
Mo15 Ti9 3.219(3) . ?
Mo15 O23 2.009(11) . ?
Mo15 O42 2.447(12) . ?
Mo15 O61 1.653(13) . ?
Mo15 O63 1.957(12) . ?
Mo15 O100 2.061(11) . ?
Mo15 O177 1.847(13) . ?
Mo15 O178 1.889(13) . ?
Mo16 O19 2.272(11) . ?
Mo16 O25 2.177(11) . ?
Mo16 O130 1.982(12) . ?
Mo16 O146 1.936(11) . ?
Mo16 O150 1.727(11) . ?
Mo16 O198 1.679(12) . ?
Mo43 Mo36 3.210(2) . ?
Mo43 Ti7 3.219(3) . ?
Mo43 O35 1.983(11) . ?
Mo43 O54 2.515(11) . ?
Mo43 O69 1.688(12) . ?
Mo43 O116 1.899(12) . ?
Mo43 O118 2.097(11) . ?
Mo43 O168 1.829(14) . ?
Mo43 O189 1.854(14) . ?
Mo18 Ti4 3.196(3) . ?
Mo18 Ti7 3.197(3) . ?
Mo18 O6 2.028(11) . ?
Mo18 O33 1.743(12) . ?
Mo18 O35 1.985(12) . ?
Mo18 O84 1.944(11) . ?
Mo18 O95 2.311(12) . ?
Mo18 O159 1.864(13) . ?
Mo18 O173 1.852(13) . ?
Mo19 O29 1.935(12) . ?
Mo19 O44 2.220(11) . ?
Mo19 O71 2.305(12) . ?
Mo19 O76 1.681(12) . ?
Mo19 O86 1.702(12) . ?
Mo19 O126 1.987(12) . ?
Mo20 Mo26 3.202(2) . ?
Mo20 O29 1.928(12) . ?
Mo20 O51 1.708(12) . ?
Mo20 O71 2.303(11) . ?
Mo20 O74 1.687(12) . ?
Mo20 O88 2.194(11) . ?
Mo20 O89 2.008(13) . ?
Mo21 Mo28 3.205(3) . ?
Mo21 O46 2.286(11) . ?
Mo21 O50 1.706(13) . ?
Mo21 O62 1.691(11) . ?
Mo21 O66 1.923(12) . ?
Mo21 O75 1.969(13) . ?
Mo21 O104 2.186(11) . ?
Mo22 Mo27 3.210(2) . ?
Mo22 O20 2.186(11) . ?
Mo22 O52 1.723(12) . ?
Mo22 O57 1.703(14) . ?
Mo22 O65 1.986(13) . ?
Mo22 O105 1.937(12) . ?
Mo22 O124 2.249(12) . ?
Mo23 O41 2.175(11) . ?
Mo23 O77 1.961(12) . ?
Mo23 O94 1.731(12) . ?
Mo23 O105 1.926(12) . ?
Mo23 O124 2.291(12) . ?
Mo23 O127 1.684(12) . ?
Mo24 Ti6 3.200(3) . ?
Mo24 Ti8 3.188(3) . ?
Mo24 O10 1.741(13) . ?
Mo24 O11 2.004(11) . ?
Mo24 O36 1.987(12) . ?
Mo24 O64 2.264(13) . ?
Mo24 O101 1.979(12) . ?
Mo24 O172 1.874(13) . ?
Mo24 O174 1.863(13) . ?
Mo25 O28 1.722(12) . ?
Mo25 O46 2.290(12) . ?
Mo25 O63 1.957(12) . ?
Mo25 O66 1.902(12) . ?
Mo25 O100 2.212(11) . ?
Mo25 O141 1.696(13) . ?
Mo26 Ti6 3.205(3) . ?
Mo26 O9 1.669(13) . ?
Mo26 O36 1.981(12) . ?
Mo26 O88 2.090(12) . ?
Mo26 O89 1.872(12) . ?
Mo26 O161 1.866(14) . ?
Mo26 O193 1.883(14) . ?
Mo27 Ti4 3.220(3) . ?
Mo27 O20 2.091(11) . ?
Mo27 O48 2.501(12) . ?
Mo27 O65 1.897(12) . ?
Mo27 O84 2.006(11) . ?
Mo27 O186 1.875(14) . ?
Mo27 O194 1.838(14) . ?
Mo27 O196 1.676(14) . ?
Mo28 Ti8 3.209(3) . ?
Mo28 O75 1.926(12) . ?
Mo28 O101 1.983(12) . ?
Mo28 O104 2.081(12) . ?
Mo28 O171 1.822(14) . ?
Mo28 O187 1.851(15) . ?
Mo28 O199 1.683(14) . ?
Mo29 K1 4.030(9) . ?
Mo29 O17 1.902(11) . ?
Mo29 O31 1.864(10) . ?
Mo29 O72 2.346(13) . ?
Mo29 O103 1.646(12) . ?
Mo29 O169 2.280(13) . ?
Mo29 O197 1.804(13) . ?
Mo30 O87 1.677(12) . ?
Mo30 O90 1.910(11) . ?
Mo30 O103 2.350(12) . ?
Mo30 O108 1.913(11) . ?
Mo30 O144 1.670(13) . ?
Mo30 O175 2.390(13) . ?
Mo31 Mo38 3.205(2) . ?
Mo31 Ti11 3.224(3) . ?
Mo31 K3 4.124(8) . ?
Mo31 O110 2.070(10) . ?
Mo31 O111 1.998(10) . ?
Mo31 O117 1.679(11) . ?
Mo31 O120 2.515(11) . ?
Mo31 O123 1.907(11) . ?
Mo31 O162 1.849(12) . ?
Mo31 O188 1.810(13) . ?
Mo32 Ti1 3.188(3) . ?
Mo32 Ti11 3.180(3) . ?
Mo32 K2 4.120(6) . ?
Mo32 O111 1.966(11) . ?
Mo32 O114 2.010(10) . ?
Mo32 O119 1.941(11) . ?
Mo32 O122 1.784(11) . ?
Mo32 O132 2.421(12) . ?
Mo32 O192 1.843(12) . ?
Mo32 O195 1.838(12) . ?
Mo33 Ti1 3.219(3) . ?
Mo33 K2 4.048(6) . ?
Mo33 O39 1.921(11) . ?
Mo33 O102 2.088(10) . ?
Mo33 O119 2.016(11) . ?
Mo33 O139 1.670(11) . ?
Mo33 O164 1.816(12) . ?
Mo33 O185 1.888(13) . ?
Mo34 Ti11 3.293(3) . ?
Mo34 Ti12 3.251(2) . ?
Mo34 O110 2.357(11) . ?
Mo34 O112 1.910(10) . ?
Mo34 O113 2.304(11) . ?
Mo34 O120 1.713(10) . ?
Mo34 O128 1.704(11) . ?
Mo34 O137 1.859(11) . ?
Mo35 O26 2.170(11) . ?
Mo35 O47 1.949(12) . ?
Mo35 O143 1.894(12) . ?
Mo35 O147 2.303(12) . ?
Mo35 O155 1.669(14) . ?
Mo35 O156 1.728(12) . ?
Mo36 O116 1.998(12) . ?
Mo36 O118 2.207(11) . ?
Mo36 O133 1.696(13) . ?
Mo36 O134 1.705(11) . ?
Mo36 O143 1.917(12) . ?
Mo36 O147 2.285(11) . ?
Mo37 O113 2.194(11) . ?
Mo37 O135 1.964(12) . ?
Mo37 O137 2.281(11) . ?
Mo37 O138 1.698(11) . ?
Mo37 O149 1.703(12) . ?
Mo37 O154 1.942(12) . ?
Mo38 O110 2.195(11) . ?
Mo38 O123 1.989(11) . ?
Mo38 O125 1.708(11) . ?
Mo38 O137 2.286(11) . ?
Mo38 O151 1.728(12) . ?
Mo38 O154 1.918(11) . ?
Mo38 K8 4.115(15) . ?
Mo39 K1 3.581(11) . ?
Mo39 O12 1.905(11) . ?
Mo39 O38 1.926(12) . ?
Mo39 O80 1.657(13) . ?
Mo39 O82 2.424(14) . ?
Mo39 O140 1.664(13) . ?
Mo39 O157 2.407(14) . ?
Mo17 O37 1.945(12) . ?
Mo17 O91 1.916(12) . ?
Mo17 O140 1.664(14) . ?
Mo17 O165 2.409(15) . ?
Mo17 O202 1.591(15) . ?
Mo41 Mo42 3.156(8) . ?
Mo41 O14 1.950(12) . ?
Mo41 O34 1.633(13) . ?
Mo41 O58 1.670(12) . ?
Mo41 O109 1.893(11) . ?
Mo41 O136 2.360(14) . ?
Mo41 O176 2.434(13) . ?
Mo41 K4 3.980(10) . ?
Mo42 O32 1.928(12) . ?
Mo42 O58 1.626(13) . ?
Mo42 O67 1.922(11) . ?
Mo42 O81 1.649(14) . ?
Mo42 O131 2.421(13) . ?
Mo42 O200 2.492(13) . ?
Mo42 K4 4.036(10) . ?
Ti1 Ti2 3.068(3) . ?
Ti1 O1 2.106(10) . ?
Ti1 O8 2.008(10) . ?
Ti1 O12 1.788(10) . ?
Ti1 O16 2.047(10) . ?
Ti1 O102 2.014(10) . ?
Ti1 O114 1.991(10) . ?
Ti1 O119 2.038(11) . ?
Ti2 O1 2.102(10) . ?
Ti2 O2 1.974(10) . ?
Ti2 O7 2.005(11) . ?
Ti2 O8 2.034(10) . ?
Ti2 O16 2.048(10) . ?
Ti2 O25 2.026(10) . ?
Ti2 O108 1.790(10) . ?
Ti3 Ti6 3.068(4) . ?
Ti3 O13 2.004(10) . ?
Ti3 O22 2.037(11) . ?
Ti3 O30 2.051(11) . ?
Ti3 O44 2.003(11) . ?
Ti3 O67 1.796(11) . ?
Ti3 O73 2.095(11) . ?
Ti3 O98 1.981(11) . ?
Ti4 Ti5 3.060(4) . ?
Ti4 O3 2.070(11) . ?
Ti4 O6 1.979(10) . ?
Ti4 O15 2.052(11) . ?
Ti4 O20 2.010(11) . ?
Ti4 O38 1.807(11) . ?
Ti4 O45 2.026(11) . ?
Ti4 O84 2.035(12) . ?
Ti5 O3 2.104(11) . ?
Ti5 O15 2.061(11) . ?
Ti5 O32 1.799(11) . ?
Ti5 O41 2.021(11) . ?
Ti5 O45 2.019(11) . ?
Ti5 O97 2.025(11) . ?
Ti5 O99 2.001(11) . ?
Ti6 O11 2.020(11) . ?
Ti6 O13 2.036(10) . ?
Ti6 O30 2.054(11) . ?
Ti6 O36 2.014(12) . ?
Ti6 O73 2.081(10) . ?
Ti6 O88 2.005(11) . ?
Ti6 O90 1.807(11) . ?
Ti7 Ti10 3.053(4) . ?
Ti7 O6 1.983(10) . ?
Ti7 O21 2.034(11) . ?
Ti7 O24 2.079(11) . ?
Ti7 O35 2.014(12) . ?
Ti7 O85 2.035(11) . ?
Ti7 O91 1.806(11) . ?
Ti7 O118 2.010(11) . ?
Ti8 Ti9 3.064(4) . ?
Ti8 O11 1.959(11) . ?
Ti8 O27 2.034(11) . ?
Ti8 O31 1.826(11) . ?
Ti8 O78 2.067(11) . ?
Ti8 O79 2.070(11) . ?
Ti8 O101 2.018(12) . ?
Ti8 O104 2.003(11) . ?
Ti9 O14 1.780(11) . ?
Ti9 O23 2.032(11) . ?
Ti9 O27 2.020(11) . ?
Ti9 O78 2.104(11) . ?
Ti9 O79 2.041(11) . ?
Ti9 O98 1.971(11) . ?
Ti9 O100 2.012(11) . ?
Ti10 O21 2.053(11) . ?
Ti10 O24 2.096(11) . ?
Ti10 O26 2.043(11) . ?
Ti10 O68 2.046(11) . ?
Ti10 O85 2.025(11) . ?
Ti10 O99 1.978(10) . ?
Ti10 O109 1.804(11) . ?
Ti11 Ti12 3.056(3) . ?
Ti11 O37 1.791(10) . ?
Ti11 O110 2.018(10) . ?
Ti11 O111 2.030(11) . ?
Ti11 O112 2.104(10) . ?
Ti11 O114 1.981(10) . ?
Ti11 O115 2.020(10) . ?
Ti11 O129 2.035(11) . ?
Ti12 O2 1.997(10) . ?
Ti12 O17 1.794(10) . ?
Ti12 O96 2.002(11) . ?
Ti12 O112 2.074(10) . ?
Ti12 O113 2.002(11) . ?
Ti12 O115 2.039(10) . ?
Ti12 O129 2.045(11) . ?
K1 O8 2.784(11) . ?
K1 O80 2.850(15) . ?
K1 O87 2.846(14) . ?
K1 O115 2.751(12) . ?
K1 O140 3.417(15) . ?
K1 O153 2.842(15) . ?
K1 O197 2.800(15) . ?
K1 O201 2.594(11) . ?
K1 Mo40 3.917(9) . ?
K1 Mo53 3.614(14) . ?
K1 O205 2.355(19) . ?
K2 K3 3.895(12) . ?
K2 O4 2.807(13) 2_646 ?
K2 O5 3.120(13) 2_646 ?
K2 O49 2.759(12) . ?
K2 O132 3.201(13) . ?
K2 O164 2.883(14) . ?
K2 O167 2.825(14) 2_646 ?
K2 O170 2.811(15) 2_646 ?
K2 O192 2.908(14) . ?
K2 O204 2.870(18) . ?
K3 O5 3.335(14) 2_646 ?
K3 O43 2.913(14) 2_646 ?
K3 O120 2.892(13) . ?
K3 O132 3.203(14) . ?
K3 O158 2.863(16) 2_646 ?
K3 O162 2.919(15) . ?
K3 O166 2.927(15) 2_646 ?
K3 O195 2.963(15) . ?
K3 O203 2.83(2) . ?
O8 O16 1.466(8) . ?
O9 K6 3.396(17) . ?
O12 Mo45 1.939(12) . ?
O12 Mo55 1.924(12) . ?
O12 Mo56 1.918(12) . ?
O13 O30 1.466(8) . ?
O14 Mo46 1.902(14) . ?
O14 Mo47 1.916(12) . ?
O14 Mo49 1.933(14) . ?
O15 O45 1.464(8) . ?
O17 Mo50 1.892(13) . ?
O21 O85 1.466(8) . ?
O27 O79 1.470(8) . ?
O31 Mo50 1.892(12) . ?
O32 Mo44 1.875(11) . ?
O32 Mo51 1.960(13) . ?
O32 Mo57 1.89(2) . ?
O34 Mo47 1.770(14) . ?
O34 Mo49 2.441(19) . ?
O34 K4 2.656(16) . ?
O37 Mo40 1.911(11) . ?
O37 Mo53 1.905(14) . ?
O37 Mo54 1.896(14) . ?
O38 Mo45 1.900(13) . ?
O38 Mo55 1.921(12) . ?
O38 Mo56 1.921(13) . ?
O51 K8 2.968(18) 1_455 ?
O58 Mo44 2.419(13) . ?
O58 Mo46 2.431(16) . ?
O58 Mo47 2.466(13) . ?
O58 Mo49 1.614(17) . ?
O58 Mo57 1.68(3) . ?
O66 K7 2.951(17) . ?
O67 Mo44 1.904(11) . ?
O67 Mo51 1.886(12) . ?
O67 Mo57 1.85(2) . ?
O70 K4 3.167(15) 3_676 ?
O70 K4 2.932(15) . ?
O72 Mo50 1.614(15) . ?
O74 K6 2.788(17) . ?
O76 K8 3.114(18) 1_455 ?
O79 K7 2.784(15) . ?
O80 Mo45 2.477(16) . ?
O80 Mo55 2.409(14) . ?
O80 Mo56 1.614(16) . ?
O81 Mo44 1.688(14) . ?
O81 Mo57 2.25(2) . ?
O81 K4 2.817(16) . ?
O82 Mo45 1.646(16) . ?
O82 Mo55 2.412(15) . ?
O82 Mo56 1.709(16) . ?
O83 O191 1.162(8) . ?
O86 K5 2.882(19) . ?
O87 Mo48 1.856(16) . ?
O87 Mo52 2.458(18) . ?
O90 Mo48 1.884(12) . ?
O90 Mo52 1.880(15) . ?
O91 Mo40 1.935(11) . ?
O91 Mo53 1.894(14) . ?
O91 Mo54 1.919(15) . ?
O103 Mo48 1.486(15) . ?
O103 Mo50 2.408(15) . ?
O103 Mo52 2.304(17) . ?
O107 K4 2.812(14) . ?
O108 Mo48 1.936(13) . ?
O108 Mo52 1.895(15) . ?
O109 Mo46 1.956(15) . ?
O109 Mo47 1.895(12) . ?
O109 Mo49 1.931(14) . ?
O115 O129 1.465(8) . ?
O125 K6 2.935(15) 1_655 ?
O127 K5 2.822(18) . ?
O131 Mo44 1.610(13) . ?
O131 Mo51 1.716(14) . ?
O131 Mo57 2.39(3) . ?
O131 K5 2.817(17) . ?
O133 K8 2.960(19) . ?
O134 K5 2.922(16) 1_655 ?
O136 Mo46 1.795(18) . ?
O136 Mo47 1.539(14) . ?
O136 Mo49 2.508(17) . ?
O138 K6 3.013(15) 1_655 ?
O140 Mo40 2.431(12) . ?
O140 Mo45 2.401(15) . ?
O140 Mo53 1.667(16) . ?
O140 Mo54 2.427(16) . ?
O140 Mo55 1.620(14) . ?
O140 Mo56 2.420(14) . ?
O142 O184 1.165(8) . ?
O144 Mo48 2.517(16) . ?
O144 Mo52 1.857(19) . ?
O144 K6 3.082(17) . ?
O151 K8 2.854(19) . ?
O153 Mo40 1.562(13) . ?
O153 Mo53 1.750(18) . ?
O153 Mo54 2.504(19) . ?
O156 K5 2.864(16) 1_655 ?
O157 Mo45 1.632(16) . ?
O157 Mo55 1.662(15) . ?
O157 Mo56 2.494(16) . ?
O158 O181 1.166(8) . ?
O159 O173 1.206(8) . ?
O160 O163 1.212(8) . ?
O161 O193 1.170(8) . ?
O162 O188 1.175(8) . ?
O164 O185 1.178(8) . ?
O165 Mo40 1.681(13) . ?
O165 Mo53 2.364(17) . ?
O165 Mo54 1.640(18) . ?
O165 K8 3.225(18) . ?
O166 O167 1.189(8) . ?
O168 O189 1.165(8) . ?
O169 Mo50 2.437(16) . ?
O170 O190 1.170(8) . ?
O171 O187 1.166(8) . ?
O172 O174 1.216(8) . ?
O175 Mo48 2.338(16) . ?
O175 Mo52 1.584(19) . ?
O176 Mo46 1.480(18) . ?
O176 Mo47 2.356(14) . ?
O176 Mo49 1.669(19) . ?
O176 K7 3.01(2) . ?
O177 O178 1.194(8) . ?
O179 O180 1.186(8) . ?
O182 O183 1.176(8) . ?
O182 K4 2.708(17) 3_676 ?
O183 K4 2.800(16) 3_676 ?
O186 O194 1.167(8) . ?
O192 O195 1.192(8) . ?
O197 Mo50 1.709(15) . ?
O197 K7 3.18(2) . ?
O198 K6 2.827(15) . ?
O200 Mo44 2.421(13) . ?
O200 Mo51 1.563(14) . ?
O200 Mo57 1.87(3) . ?
Mo40 O202 2.509(14) . ?
O202 Mo53 2.353(18) . ?
O202 Mo54 1.57(2) . ?
Mo46 K7 3.69(2) . ?
Mo50 K7 3.884(18) . ?
Mo52 K6 4.062(16) . ?
K4 K4 3.946(17) 3_676 ?
K4 O207 2.885(18) 3_676 ?
K4 O207 2.702(18) . ?
K5 O206 2.809(16) . ?
K7 K8 4.562(18) . ?
K7 O208 2.745(19) . ?
K7 O209 2.99(2) . ?
K8 O208 2.933(19) . ?
K8 O209 2.72(2) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Ti2 Mo1 Ti1 55.76(6) . . ?
O1 Mo1 Ti1 36.9(3) . . ?
O1 Mo1 Ti2 37.5(3) . . ?
O1 Mo1 O25 75.3(4) . . ?
O1 Mo1 O102 74.1(4) . . ?
O19 Mo1 Ti1 109.6(3) . . ?
O19 Mo1 Ti2 110.0(3) . . ?
O19 Mo1 O1 138.2(4) . . ?
O19 Mo1 O25 76.4(4) . . ?
O19 Mo1 O102 76.6(4) . . ?
O25 Mo1 Ti1 83.3(3) . . ?
O25 Mo1 Ti2 37.9(3) . . ?
O25 Mo1 O102 91.7(4) . . ?
O49 Mo1 Ti1 90.4(3) . . ?
O49 Mo1 Ti2 138.4(4) . . ?
O49 Mo1 O1 101.0(5) . . ?
O49 Mo1 O19 103.6(5) . . ?
O49 Mo1 O25 173.2(5) . . ?
O49 Mo1 O102 81.7(4) . . ?
O102 Mo1 Ti1 37.2(3) . . ?
O102 Mo1 Ti2 82.8(3) . . ?
O106 Mo1 Ti1 139.1(4) . . ?
O106 Mo1 Ti2 91.0(4) . . ?
O106 Mo1 O1 102.2(5) . . ?
O106 Mo1 O19 103.6(5) . . ?
O106 Mo1 O25 81.9(5) . . ?
O106 Mo1 O49 104.5(5) . . ?
O106 Mo1 O102 173.4(4) . . ?
Ti7 Mo2 Ti10 55.51(7) . . ?
O4 Mo2 Ti7 137.9(4) . . ?
O4 Mo2 Ti10 90.3(4) . . ?
O4 Mo2 O24 101.0(5) . . ?
O4 Mo2 O26 81.2(5) . . ?
O4 Mo2 O54 105.1(5) . . ?
O4 Mo2 O118 172.5(5) . . ?
O4 Mo2 O147 103.1(5) . . ?
O24 Mo2 Ti7 37.0(3) . . ?
O24 Mo2 Ti10 36.5(3) . . ?
O24 Mo2 O26 74.4(4) . . ?
O24 Mo2 O118 74.5(4) . . ?
O26 Mo2 Ti7 83.5(3) . . ?
O26 Mo2 Ti10 37.9(3) . . ?
O54 Mo2 Ti7 90.9(4) . . ?
O54 Mo2 Ti10 139.2(4) . . ?
O54 Mo2 O24 102.8(5) . . ?
O54 Mo2 O26 173.5(5) . . ?
O54 Mo2 O118 81.9(5) . . ?
O54 Mo2 O147 102.2(5) . . ?
O118 Mo2 Ti7 37.7(3) . . ?
O118 Mo2 Ti10 82.5(3) . . ?
O118 Mo2 O26 91.6(4) . . ?
O147 Mo2 Ti7 111.3(3) . . ?
O147 Mo2 Ti10 110.8(4) . . ?
O147 Mo2 O24 139.1(5) . . ?
O147 Mo2 O26 77.1(4) . . ?
O147 Mo2 O118 77.5(4) . . ?
Ti4 Mo3 Ti5 55.73(7) . . ?
O3 Mo3 Ti4 36.7(3) . . ?
O3 Mo3 Ti5 36.9(3) . . ?
O3 Mo3 O20 74.4(4) . . ?
O3 Mo3 O41 74.4(4) . . ?
O20 Mo3 Ti4 37.7(3) . . ?
O20 Mo3 Ti5 82.9(3) . . ?
O20 Mo3 O41 91.7(4) . . ?
O41 Mo3 Ti4 83.1(3) . . ?
O41 Mo3 Ti5 37.5(3) . . ?
O43 Mo3 Ti4 138.4(4) . . ?
O43 Mo3 Ti5 90.1(4) . . ?
O43 Mo3 O3 101.7(5) . . ?
O43 Mo3 O20 172.4(5) . . ?
O43 Mo3 O41 80.9(5) . . ?
O43 Mo3 O124 103.5(5) . . ?
O48 Mo3 Ti4 90.4(4) . . ?
O48 Mo3 Ti5 138.5(4) . . ?
O48 Mo3 O3 101.7(5) . . ?
O48 Mo3 O20 81.8(5) . . ?
O48 Mo3 O41 173.2(5) . . ?
O48 Mo3 O43 105.5(6) . . ?
O48 Mo3 O124 103.2(5) . . ?
O124 Mo3 Ti4 110.0(4) . . ?
O124 Mo3 Ti5 110.2(4) . . ?
O124 Mo3 O3 138.0(5) . . ?
O124 Mo3 O20 76.4(4) . . ?
O124 Mo3 O41 77.2(4) . . ?
Ti6 Mo4 Ti3 55.83(6) . . ?
O44 Mo4 Ti3 37.0(3) . . ?
O44 Mo4 Ti6 83.0(3) . . ?
O53 Mo4 Ti3 138.1(4) . . ?
O53 Mo4 Ti6 89.7(4) . . ?
O53 Mo4 O44 172.5(5) . . ?
O53 Mo4 O56 106.0(5) . . ?
O53 Mo4 O71 103.2(5) . . ?
O53 Mo4 O73 101.6(5) . . ?
O53 Mo4 O88 81.5(5) . . ?
O56 Mo4 Ti3 90.1(4) . . ?
O56 Mo4 Ti6 138.4(4) . . ?
O56 Mo4 O44 80.8(5) . . ?
O56 Mo4 O71 102.6(5) . . ?
O56 Mo4 O73 101.3(5) . . ?
O56 Mo4 O88 172.2(5) . . ?
O71 Mo4 Ti3 110.8(3) . . ?
O71 Mo4 Ti6 111.0(3) . . ?
O71 Mo4 O44 77.9(4) . . ?
O71 Mo4 O73 139.0(5) . . ?
O71 Mo4 O88 77.3(4) . . ?
O73 Mo4 Ti3 36.6(3) . . ?
O73 Mo4 Ti6 37.1(3) . . ?
O73 Mo4 O44 73.6(4) . . ?
O73 Mo4 O88 74.6(4) . . ?
O88 Mo4 Ti3 82.7(3) . . ?
O88 Mo4 Ti6 37.6(3) . . ?
O88 Mo4 O44 91.6(4) . . ?
Ti8 Mo5 Ti9 55.72(7) . . ?
O42 Mo5 Ti8 138.4(4) . . ?
O42 Mo5 Ti9 89.8(4) . . ?
O42 Mo5 O46 102.6(5) . . ?
O42 Mo5 O78 101.5(5) . . ?
O42 Mo5 O100 80.2(5) . . ?
O42 Mo5 O104 172.2(5) . . ?
O46 Mo5 Ti8 110.5(3) . . ?
O46 Mo5 Ti9 110.2(4) . . ?
O46 Mo5 O78 138.4(5) . . ?
O46 Mo5 O100 77.5(5) . . ?
O46 Mo5 O104 77.0(5) . . ?
O55 Mo5 Ti8 90.5(4) . . ?
O55 Mo5 Ti9 138.6(4) . . ?
O55 Mo5 O42 105.9(6) . . ?
O55 Mo5 O46 103.4(5) . . ?
O55 Mo5 O78 102.0(5) . . ?
O55 Mo5 O100 173.3(5) . . ?
O55 Mo5 O104 81.7(5) . . ?
O78 Mo5 Ti8 37.0(3) . . ?
O78 Mo5 Ti9 36.8(3) . . ?
O78 Mo5 O100 73.8(4) . . ?
O78 Mo5 O104 74.6(4) . . ?
O100 Mo5 Ti8 83.0(3) . . ?
O100 Mo5 Ti9 37.1(3) . . ?
O104 Mo5 Ti8 37.7(3) . . ?
O104 Mo5 Ti9 83.0(3) . . ?
O104 Mo5 O100 92.1(4) . . ?
Ti5 Mo6 K2 129.73(11) . 2_656 ?
Ti10 Mo6 Ti5 73.67(7) . . ?
Ti10 Mo6 K2 94.96(10) . 2_656 ?
O5 Mo6 Ti5 80.3(3) . . ?
O5 Mo6 Ti10 80.2(3) . . ?
O5 Mo6 K2 49.4(3) . 2_656 ?
O68 Mo6 Ti5 111.4(3) . . ?
O68 Mo6 Ti10 38.1(3) . . ?
O68 Mo6 K2 67.2(3) . 2_656 ?
O68 Mo6 O5 82.0(4) . . ?
O68 Mo6 O97 147.7(5) . . ?
O68 Mo6 O99 74.3(4) . . ?
O97 Mo6 Ti5 37.8(3) . . ?
O97 Mo6 Ti10 111.1(3) . . ?
O97 Mo6 K2 120.1(3) . 2_656 ?
O97 Mo6 O5 82.3(4) . . ?
O97 Mo6 O99 74.6(4) . . ?
O99 Mo6 Ti5 37.2(3) . . ?
O99 Mo6 Ti10 36.5(3) . . ?
O99 Mo6 K2 115.4(3) . 2_656 ?
O99 Mo6 O5 76.2(4) . . ?
O107 Mo6 Ti5 98.3(4) . . ?
O107 Mo6 Ti10 98.1(4) . . ?
O107 Mo6 K2 131.9(4) . 2_656 ?
O107 Mo6 O5 178.1(5) . . ?
O107 Mo6 O68 97.3(5) . . ?
O107 Mo6 O97 97.5(5) . . ?
O107 Mo6 O99 101.9(5) . . ?
O107 Mo6 O166 101.1(6) . . ?
O107 Mo6 O167 99.9(6) . . ?
O166 Mo6 Ti5 120.7(4) . . ?
O166 Mo6 Ti10 153.5(4) . . ?
O166 Mo6 K2 58.6(4) . 2_656 ?
O166 Mo6 O5 80.7(5) . . ?
O166 Mo6 O68 120.6(5) . . ?
O166 Mo6 O97 84.2(5) . . ?
O166 Mo6 O99 150.4(5) . . ?
O167 Mo6 Ti5 153.9(4) . . ?
O167 Mo6 Ti10 121.6(4) . . ?
O167 Mo6 K2 36.5(4) . 2_656 ?
O167 Mo6 O5 81.7(5) . . ?
O167 Mo6 O68 84.6(5) . . ?
O167 Mo6 O97 120.7(5) . . ?
O167 Mo6 O99 151.2(5) . . ?
O167 Mo6 O166 36.9(3) . . ?
Mo16 Mo7 Ti2 78.68(6) . . ?
O7 Mo7 Mo16 114.9(3) . . ?
O7 Mo7 Ti2 36.8(3) . . ?
O7 Mo7 O25 72.8(4) . . ?
O25 Mo7 Mo16 42.5(3) . . ?
O25 Mo7 Ti2 38.0(3) . . ?
O60 Mo7 Mo16 93.8(4) . . ?
O60 Mo7 Ti2 95.0(4) . . ?
O60 Mo7 O7 98.1(5) . . ?
O60 Mo7 O25 105.0(5) . . ?
O60 Mo7 O83 104.1(6) . . ?
O60 Mo7 O130 99.8(6) . . ?
O60 Mo7 O191 104.8(6) . . ?
O83 Mo7 Mo16 150.5(4) . . ?
O83 Mo7 Ti2 121.9(4) . . ?
O83 Mo7 O7 85.9(5) . . ?
O83 Mo7 O25 145.9(5) . . ?
O83 Mo7 O130 117.0(5) . . ?
O130 Mo7 Mo16 35.4(4) . . ?
O130 Mo7 Ti2 112.7(4) . . ?
O130 Mo7 O7 146.1(5) . . ?
O130 Mo7 O25 74.8(5) . . ?
O191 Mo7 Mo16 116.1(4) . . ?
O191 Mo7 Ti2 153.9(4) . . ?
O191 Mo7 O7 121.7(5) . . ?
O191 Mo7 O25 144.2(5) . . ?
O191 Mo7 O83 36.8(3) . . ?
O191 Mo7 O130 80.9(6) . . ?
Mo35 Mo8 Ti10 78.42(6) . . ?
Mo35 Mo8 K2 127.40(10) . 2_656 ?
Ti10 Mo8 K2 95.39(11) . 2_656 ?
O26 Mo8 Mo35 42.2(3) . . ?
O26 Mo8 Ti10 38.1(3) . . ?
O26 Mo8 K2 107.8(3) . 2_656 ?
O47 Mo8 Mo35 34.3(4) . . ?
O47 Mo8 Ti10 111.8(4) . . ?
O47 Mo8 K2 114.6(4) . 2_656 ?
O47 Mo8 O26 74.0(5) . . ?
O47 Mo8 O68 146.6(5) . . ?
O68 Mo8 Mo35 115.6(3) . . ?
O68 Mo8 Ti10 37.7(3) . . ?
O68 Mo8 K2 68.4(3) . 2_656 ?
O68 Mo8 O26 73.7(4) . . ?
O93 Mo8 Mo35 94.4(5) . . ?
O93 Mo8 Ti10 94.6(4) . . ?
O93 Mo8 K2 138.2(5) . 2_656 ?
O93 Mo8 O26 105.0(6) . . ?
O93 Mo8 O47 98.9(6) . . ?
O93 Mo8 O68 97.3(5) . . ?
O93 Mo8 O170 105.1(6) . . ?
O93 Mo8 O190 105.0(6) . . ?
O170 Mo8 Mo35 149.5(4) . . ?
O170 Mo8 Ti10 122.0(4) . . ?
O170 Mo8 K2 37.6(4) . 2_656 ?
O170 Mo8 O26 145.2(5) . . ?
O170 Mo8 O47 117.8(5) . . ?
O170 Mo8 O68 85.4(5) . . ?
O190 Mo8 Mo35 115.4(4) . . ?
O190 Mo8 Ti10 154.5(4) . . ?
O190 Mo8 K2 59.1(4) . 2_656 ?
O190 Mo8 O26 143.7(5) . . ?
O190 Mo8 O47 81.5(5) . . ?
O190 Mo8 O68 121.8(5) . . ?
O190 Mo8 O170 37.2(3) . . ?
Ti12 Mo9 Ti2 73.31(7) . . ?
O2 Mo9 Ti2 36.2(3) . . ?
O2 Mo9 Ti12 37.1(3) . . ?
O2 Mo9 O59 81.9(4) . . ?
O7 Mo9 Ti2 36.8(3) . . ?
O7 Mo9 Ti12 110.1(3) . . ?
O7 Mo9 O2 73.1(4) . . ?
O7 Mo9 O59 83.8(4) . . ?
O7 Mo9 O96 146.2(5) . . ?
O59 Mo9 Ti2 81.5(3) . . ?
O59 Mo9 Ti12 83.0(3) . . ?
O96 Mo9 Ti2 110.0(3) . . ?
O96 Mo9 Ti12 37.0(3) . . ?
O96 Mo9 O2 74.1(4) . . ?
O96 Mo9 O59 84.2(4) . . ?
O121 Mo9 Ti2 97.6(4) . . ?
O121 Mo9 Ti12 96.8(4) . . ?
O121 Mo9 O2 97.4(5) . . ?
O121 Mo9 O7 95.5(5) . . ?
O121 Mo9 O59 179.1(6) . . ?
O121 Mo9 O96 96.1(5) . . ?
O121 Mo9 O160 97.3(6) . . ?
O121 Mo9 O163 98.8(6) . . ?
O160 Mo9 Ti2 120.9(4) . . ?
O160 Mo9 Ti12 158.2(4) . . ?
O160 Mo9 O2 154.6(5) . . ?
O160 Mo9 O7 84.9(5) . . ?
O160 Mo9 O59 83.1(5) . . ?
O160 Mo9 O96 124.6(5) . . ?
O163 Mo9 Ti2 155.0(4) . . ?
O163 Mo9 Ti12 122.9(4) . . ?
O163 Mo9 O2 156.1(5) . . ?
O163 Mo9 O7 122.4(5) . . ?
O163 Mo9 O59 82.0(5) . . ?
O163 Mo9 O96 86.8(5) . . ?
O163 Mo9 O160 38.1(3) . . ?
O19 Mo10 Mo33 85.4(3) . . ?
O39 Mo10 Mo33 33.9(3) . . ?
O39 Mo10 O19 84.1(4) . . ?
O39 Mo10 O102 71.6(4) . . ?
O40 Mo10 Mo33 126.7(4) . . ?
O40 Mo10 O19 92.1(5) . . ?
O40 Mo10 O39 92.8(5) . . ?
O40 Mo10 O102 158.1(5) . . ?
O40 Mo10 O146 100.6(5) . . ?
O102 Mo10 Mo33 40.2(3) . . ?
O102 Mo10 O19 71.5(4) . . ?
O145 Mo10 Mo33 89.0(4) . . ?
O145 Mo10 O19 163.4(5) . . ?
O145 Mo10 O39 99.8(5) . . ?
O145 Mo10 O40 103.7(6) . . ?
O145 Mo10 O102 94.3(5) . . ?
O145 Mo10 O146 99.7(5) . . ?
O146 Mo10 Mo33 128.4(3) . . ?
O146 Mo10 O19 72.1(4) . . ?
O146 Mo10 O39 152.9(5) . . ?
O146 Mo10 O102 88.3(4) . . ?
Mo23 Mo11 Ti5 78.25(6) . . ?
O41 Mo11 Mo23 42.4(3) . . ?
O41 Mo11 Ti5 37.5(3) . . ?
O41 Mo11 O43 70.4(4) . . ?
O43 Mo11 Mo23 84.0(3) . . ?
O43 Mo11 Ti5 79.7(3) . . ?
O77 Mo11 Mo23 35.0(4) . . ?
O77 Mo11 Ti5 112.2(4) . . ?
O77 Mo11 O41 74.9(5) . . ?
O77 Mo11 O43 82.3(4) . . ?
O77 Mo11 O97 145.9(5) . . ?
O92 Mo11 Mo23 94.5(5) . . ?
O92 Mo11 Ti5 95.5(4) . . ?
O92 Mo11 O41 105.3(5) . . ?
O92 Mo11 O43 175.2(5) . . ?
O92 Mo11 O77 99.1(6) . . ?
O92 Mo11 O97 98.3(5) . . ?
O92 Mo11 O158 103.5(6) . . ?
O92 Mo11 O181 103.6(6) . . ?
O97 Mo11 Mo23 114.5(3) . . ?
O97 Mo11 Ti5 36.8(3) . . ?
O97 Mo11 O41 72.3(4) . . ?
O97 Mo11 O43 78.3(4) . . ?
O158 Mo11 Mo23 152.0(4) . . ?
O158 Mo11 Ti5 120.4(4) . . ?
O158 Mo11 O41 145.0(5) . . ?
O158 Mo11 O43 79.7(5) . . ?
O158 Mo11 O77 119.5(5) . . ?
O158 Mo11 O97 84.3(5) . . ?
O181 Mo11 Mo23 118.5(4) . . ?
O181 Mo11 Ti5 152.9(4) . . ?
O181 Mo11 O41 146.2(5) . . ?
O181 Mo11 O43 81.1(5) . . ?
O181 Mo11 O77 83.8(5) . . ?
O181 Mo11 O97 120.0(5) . . ?
O181 Mo11 O158 36.5(3) . . ?
Mo19 Mo12 Ti3 78.98(6) . . ?
O22 Mo12 Mo19 116.1(3) . . ?
O22 Mo12 Ti3 37.5(3) . . ?
O22 Mo12 O44 72.8(4) . . ?
O22 Mo12 O56 79.3(4) . . ?
O44 Mo12 Mo19 43.4(3) . . ?
O44 Mo12 Ti3 37.0(3) . . ?
O44 Mo12 O56 72.5(4) . . ?
O56 Mo12 Mo19 85.3(3) . . ?
O56 Mo12 Ti3 80.8(2) . . ?
O126 Mo12 Mo19 35.5(3) . . ?
O126 Mo12 Ti3 113.2(3) . . ?
O126 Mo12 O22 147.6(5) . . ?
O126 Mo12 O44 76.3(5) . . ?
O126 Mo12 O56 82.2(5) . . ?
O152 Mo12 Mo19 93.1(5) . . ?
O152 Mo12 Ti3 94.8(4) . . ?
O152 Mo12 O22 97.7(5) . . ?
O152 Mo12 O44 103.5(5) . . ?
O152 Mo12 O56 175.5(5) . . ?
O152 Mo12 O126 98.9(6) . . ?
O152 Mo12 O179 102.0(6) . . ?
O152 Mo12 O180 101.9(6) . . ?
O179 Mo12 Mo19 117.2(4) . . ?
O179 Mo12 Ti3 155.6(4) . . ?
O179 Mo12 O22 121.4(5) . . ?
O179 Mo12 O44 148.5(5) . . ?
O179 Mo12 O56 82.4(5) . . ?
O179 Mo12 O126 81.8(5) . . ?
O179 Mo12 O180 37.2(3) . . ?
O180 Mo12 Mo19 152.5(4) . . ?
O180 Mo12 Ti3 122.0(4) . . ?
O180 Mo12 O22 85.0(5) . . ?
O180 Mo12 O44 148.1(5) . . ?
O180 Mo12 O56 81.3(5) . . ?
O180 Mo12 O126 118.3(5) . . ?
Ti12 Mo13 Mo37 78.15(6) . . ?
O18 Mo13 Mo37 94.9(5) . . ?
O18 Mo13 Ti12 94.9(4) . . ?
O18 Mo13 O96 96.4(5) . . ?
O18 Mo13 O113 105.4(5) . . ?
O18 Mo13 O128 174.0(5) . . ?
O18 Mo13 O135 99.6(6) . . ?
O18 Mo13 O142 103.7(6) . . ?
O18 Mo13 O184 103.3(6) . . ?
O96 Mo13 Mo37 114.4(3) . . ?
O96 Mo13 Ti12 36.6(3) . . ?
O96 Mo13 O113 72.3(4) . . ?
O96 Mo13 O128 79.0(4) . . ?
O113 Mo13 Mo37 42.5(3) . . ?
O113 Mo13 Ti12 37.4(3) . . ?
O113 Mo13 O128 69.7(4) . . ?
O128 Mo13 Mo37 83.6(3) . . ?
O128 Mo13 Ti12 79.1(3) . . ?
O135 Mo13 Mo37 34.5(3) . . ?
O135 Mo13 Ti12 111.7(3) . . ?
O135 Mo13 O96 145.9(5) . . ?
O135 Mo13 O113 74.5(4) . . ?
O135 Mo13 O128 82.5(4) . . ?
O142 Mo13 Mo37 149.2(4) . . ?
O142 Mo13 Ti12 123.4(4) . . ?
O142 Mo13 O96 87.9(5) . . ?
O142 Mo13 O113 146.3(5) . . ?
O142 Mo13 O128 80.1(5) . . ?
O142 Mo13 O135 116.8(5) . . ?
O184 Mo13 Mo37 115.4(4) . . ?
O184 Mo13 Ti12 155.9(4) . . ?
O184 Mo13 O96 124.0(5) . . ?
O184 Mo13 O113 144.9(5) . . ?
O184 Mo13 O128 82.6(5) . . ?
O184 Mo13 O135 81.1(5) . . ?
O184 Mo13 O142 36.7(3) . . ?
Ti3 Mo14 K4 140.64(18) . 3_676 ?
Ti9 Mo14 Ti3 73.80(7) . . ?
Ti9 Mo14 K4 133.66(19) . 3_676 ?
O22 Mo14 Ti3 38.1(3) . . ?
O22 Mo14 Ti9 111.6(3) . . ?
O22 Mo14 O98 74.7(4) . . ?
O22 Mo14 O148 81.6(5) . . ?
O22 Mo14 K4 109.9(4) . 3_676 ?
O23 Mo14 Ti3 111.6(3) . . ?
O23 Mo14 Ti9 38.0(3) . . ?
O23 Mo14 O22 148.3(5) . . ?
O23 Mo14 O98 74.6(4) . . ?
O23 Mo14 O148 83.8(5) . . ?
O23 Mo14 K4 101.5(4) . 3_676 ?
O70 Mo14 Ti3 96.8(4) . . ?
O70 Mo14 Ti9 97.7(4) . . ?
O70 Mo14 O22 96.6(5) . . ?
O70 Mo14 O23 96.8(5) . . ?
O70 Mo14 O98 100.8(5) . . ?
O70 Mo14 O148 177.4(5) . . ?
O70 Mo14 O182 98.1(6) . . ?
O70 Mo14 O183 97.9(6) . . ?
O70 Mo14 K4 57.6(4) . 3_676 ?
O98 Mo14 Ti3 37.0(3) . . ?
O98 Mo14 Ti9 36.9(3) . . ?
O98 Mo14 O148 76.9(4) . . ?
O98 Mo14 K4 157.9(3) . 3_676 ?
O148 Mo14 Ti3 80.6(3) . . ?
O148 Mo14 Ti9 81.3(3) . . ?
O148 Mo14 K4 124.8(3) . 3_676 ?
O182 Mo14 Ti3 157.5(4) . . ?
O182 Mo14 Ti9 120.5(4) . . ?
O182 Mo14 O22 122.9(5) . . ?
O182 Mo14 O23 83.2(5) . . ?
O182 Mo14 O98 152.4(5) . . ?
O182 Mo14 O148 84.5(6) . . ?
O182 Mo14 K4 43.0(5) . 3_676 ?
O183 Mo14 Ti3 123.1(4) . . ?
O183 Mo14 Ti9 155.2(4) . . ?
O183 Mo14 O22 85.6(5) . . ?
O183 Mo14 O23 120.6(5) . . ?
O183 Mo14 O98 154.2(5) . . ?
O183 Mo14 O148 83.9(5) . . ?
O183 Mo14 O182 37.8(3) . . ?
O183 Mo14 K4 45.9(5) . 3_676 ?
Mo25 Mo15 Ti9 78.85(6) . . ?
O23 Mo15 Mo25 115.8(3) . . ?
O23 Mo15 Ti9 37.4(3) . . ?
O23 Mo15 O42 79.6(4) . . ?
O23 Mo15 O100 72.9(4) . . ?
O42 Mo15 Mo25 84.8(3) . . ?
O42 Mo15 Ti9 80.9(3) . . ?
O61 Mo15 Mo25 94.2(5) . . ?
O61 Mo15 Ti9 94.3(4) . . ?
O61 Mo15 O23 96.7(5) . . ?
O61 Mo15 O42 175.2(5) . . ?
O61 Mo15 O63 99.7(6) . . ?
O61 Mo15 O100 104.1(5) . . ?
O61 Mo15 O177 103.3(6) . . ?
O61 Mo15 O178 101.7(6) . . ?
O63 Mo15 Mo25 35.0(3) . . ?
O63 Mo15 Ti9 112.7(3) . . ?
O63 Mo15 O23 147.2(5) . . ?
O63 Mo15 O42 82.2(4) . . ?
O63 Mo15 O100 75.6(5) . . ?
O100 Mo15 Mo25 43.2(3) . . ?
O100 Mo15 Ti9 37.2(3) . . ?
O100 Mo15 O42 71.9(4) . . ?
O177 Mo15 Mo25 118.9(4) . . ?
O177 Mo15 Ti9 153.4(4) . . ?
O177 Mo15 O23 119.3(5) . . ?
O177 Mo15 O42 81.3(5) . . ?
O177 Mo15 O63 84.1(5) . . ?
O177 Mo15 O100 148.2(5) . . ?
O177 Mo15 O178 37.3(3) . . ?
O178 Mo15 Mo25 154.0(4) . . ?
O178 Mo15 Ti9 119.9(4) . . ?
O178 Mo15 O23 82.9(5) . . ?
O178 Mo15 O42 81.0(5) . . ?
O178 Mo15 O63 120.7(5) . . ?
O178 Mo15 O100 146.3(5) . . ?
O19 Mo16 Mo7 86.6(3) . . ?
O25 Mo16 Mo7 40.3(3) . . ?
O25 Mo16 O19 71.5(4) . . ?
O130 Mo16 Mo7 33.8(3) . . ?
O130 Mo16 O19 84.5(4) . . ?
O130 Mo16 O25 71.3(4) . . ?
O146 Mo16 Mo7 127.8(3) . . ?
O146 Mo16 O19 71.7(4) . . ?
O146 Mo16 O25 87.5(4) . . ?
O146 Mo16 O130 152.3(5) . . ?
O150 Mo16 Mo7 128.3(5) . . ?
O150 Mo16 O19 90.1(5) . . ?
O150 Mo16 O25 157.4(5) . . ?
O150 Mo16 O130 94.5(6) . . ?
O150 Mo16 O146 99.5(5) . . ?
O198 Mo16 Mo7 87.4(4) . . ?
O198 Mo16 O19 164.8(5) . . ?
O198 Mo16 O25 95.1(5) . . ?
O198 Mo16 O130 98.1(6) . . ?
O198 Mo16 O146 101.4(6) . . ?
O198 Mo16 O150 104.5(6) . . ?
Mo36 Mo43 Ti7 78.82(6) . . ?
O35 Mo43 Mo36 114.9(3) . . ?
O35 Mo43 Ti7 36.7(3) . . ?
O35 Mo43 O54 78.2(4) . . ?
O35 Mo43 O118 72.1(4) . . ?
O54 Mo43 Mo36 84.3(3) . . ?
O54 Mo43 Ti7 79.7(3) . . ?
O69 Mo43 Mo36 93.0(5) . . ?
O69 Mo43 Ti7 94.3(4) . . ?
O69 Mo43 O35 98.0(5) . . ?
O69 Mo43 O54 173.8(5) . . ?
O69 Mo43 O116 99.6(6) . . ?
O69 Mo43 O118 103.9(6) . . ?
O69 Mo43 O168 103.7(6) . . ?
O69 Mo43 O189 106.0(6) . . ?
O116 Mo43 Mo36 35.6(4) . . ?
O116 Mo43 Ti7 113.0(4) . . ?
O116 Mo43 O35 146.1(5) . . ?
O116 Mo43 O54 81.4(4) . . ?
O116 Mo43 O118 75.6(5) . . ?
O118 Mo43 Mo36 43.1(3) . . ?
O118 Mo43 Ti7 37.4(3) . . ?
O118 Mo43 O54 70.4(4) . . ?
O168 Mo43 Mo36 148.9(4) . . ?
O168 Mo43 Ti7 124.9(4) . . ?
O168 Mo43 O35 88.9(5) . . ?
O168 Mo43 O54 81.3(5) . . ?
O168 Mo43 O116 114.5(5) . . ?
O168 Mo43 O118 148.3(5) . . ?
O168 Mo43 O189 36.9(3) . . ?
O189 Mo43 Mo36 113.4(4) . . ?
O189 Mo43 Ti7 155.2(4) . . ?
O189 Mo43 O35 124.0(5) . . ?
O189 Mo43 O54 80.2(5) . . ?
O189 Mo43 O116 78.1(6) . . ?
O189 Mo43 O118 142.9(5) . . ?
Ti4 Mo18 Ti7 73.19(7) . . ?
O6 Mo18 Ti4 36.6(3) . . ?
O6 Mo18 Ti7 36.7(3) . . ?
O6 Mo18 O95 81.5(4) . . ?
O33 Mo18 Ti4 98.4(4) . . ?
O33 Mo18 Ti7 98.3(4) . . ?
O33 Mo18 O6 98.6(5) . . ?
O33 Mo18 O35 96.5(5) . . ?
O33 Mo18 O84 96.1(5) . . ?
O33 Mo18 O95 179.3(5) . . ?
O33 Mo18 O159 96.9(6) . . ?
O33 Mo18 O173 97.5(6) . . ?
O35 Mo18 Ti4 110.2(3) . . ?
O35 Mo18 Ti7 37.2(3) . . ?
O35 Mo18 O6 73.9(4) . . ?
O35 Mo18 O95 83.0(5) . . ?
O84 Mo18 Ti4 37.6(3) . . ?
O84 Mo18 Ti7 110.6(3) . . ?
O84 Mo18 O6 74.1(4) . . ?
O84 Mo18 O35 147.0(5) . . ?
O84 Mo18 O95 84.5(5) . . ?
O95 Mo18 Ti4 82.1(3) . . ?
O95 Mo18 Ti7 81.5(3) . . ?
O159 Mo18 Ti4 156.8(4) . . ?
O159 Mo18 Ti7 121.6(4) . . ?
O159 Mo18 O6 155.2(5) . . ?
O159 Mo18 O35 85.2(5) . . ?
O159 Mo18 O84 123.3(5) . . ?
O159 Mo18 O95 82.8(5) . . ?
O173 Mo18 Ti4 122.2(4) . . ?
O173 Mo18 Ti7 155.8(4) . . ?
O173 Mo18 O6 155.3(5) . . ?
O173 Mo18 O35 122.5(5) . . ?
O173 Mo18 O84 85.7(5) . . ?
O173 Mo18 O95 82.5(5) . . ?
O173 Mo18 O159 37.9(3) . . ?
O29 Mo19 Mo12 126.7(4) . . ?
O29 Mo19 O44 87.0(4) . . ?
O29 Mo19 O71 72.9(5) . . ?
O29 Mo19 O126 151.3(5) . . ?
O44 Mo19 Mo12 39.8(3) . . ?
O44 Mo19 O71 72.4(4) . . ?
O71 Mo19 Mo12 84.9(3) . . ?
O76 Mo19 Mo12 128.1(4) . . ?
O76 Mo19 O29 100.6(6) . . ?
O76 Mo19 O44 158.7(5) . . ?
O76 Mo19 O71 90.6(5) . . ?
O76 Mo19 O86 106.4(6) . . ?
O76 Mo19 O126 94.0(5) . . ?
O86 Mo19 Mo12 90.0(4) . . ?
O86 Mo19 O29 96.3(6) . . ?
O86 Mo19 O44 92.4(5) . . ?
O86 Mo19 O71 161.5(5) . . ?
O86 Mo19 O126 103.0(6) . . ?
O126 Mo19 Mo12 34.1(3) . . ?
O126 Mo19 O44 71.5(4) . . ?
O126 Mo19 O71 82.5(5) . . ?
O29 Mo20 Mo26 128.0(4) . . ?
O29 Mo20 O71 73.0(4) . . ?
O29 Mo20 O88 87.6(5) . . ?
O29 Mo20 O89 153.0(5) . . ?
O51 Mo20 Mo26 127.1(4) . . ?
O51 Mo20 O29 100.5(6) . . ?
O51 Mo20 O71 90.4(5) . . ?
O51 Mo20 O88 157.3(5) . . ?
O51 Mo20 O89 94.0(6) . . ?
O71 Mo20 Mo26 85.7(3) . . ?
O74 Mo20 Mo26 89.4(5) . . ?
O74 Mo20 O29 98.1(6) . . ?
O74 Mo20 O51 105.0(6) . . ?
O74 Mo20 O71 163.6(5) . . ?
O74 Mo20 O88 94.7(5) . . ?
O74 Mo20 O89 100.0(6) . . ?
O88 Mo20 Mo26 40.4(3) . . ?
O88 Mo20 O71 71.6(4) . . ?
O89 Mo20 Mo26 33.0(3) . . ?
O89 Mo20 O71 84.4(5) . . ?
O89 Mo20 O88 71.1(5) . . ?
O46 Mo21 Mo28 85.6(3) . . ?
O50 Mo21 Mo28 87.2(5) . . ?
O50 Mo21 O46 162.4(5) . . ?
O50 Mo21 O66 100.0(6) . . ?
O50 Mo21 O75 99.5(6) . . ?
O50 Mo21 O104 92.7(5) . . ?
O62 Mo21 Mo28 126.0(5) . . ?
O62 Mo21 O46 92.2(5) . . ?
O62 Mo21 O50 105.1(6) . . ?
O62 Mo21 O66 101.3(6) . . ?
O62 Mo21 O75 91.9(6) . . ?
O62 Mo21 O104 157.6(5) . . ?
O66 Mo21 Mo28 128.6(3) . . ?
O66 Mo21 O46 72.4(4) . . ?
O66 Mo21 O75 152.7(5) . . ?
O66 Mo21 O104 88.6(5) . . ?
O75 Mo21 Mo28 34.2(3) . . ?
O75 Mo21 O46 83.4(5) . . ?
O75 Mo21 O104 71.5(5) . . ?
O104 Mo21 Mo28 40.1(3) . . ?
O104 Mo21 O46 71.5(4) . . ?
O20 Mo22 Mo27 40.3(3) . . ?
O20 Mo22 O124 72.0(4) . . ?
O52 Mo22 Mo27 127.6(5) . . ?
O52 Mo22 O20 159.1(6) . . ?
O52 Mo22 O65 94.3(6) . . ?
O52 Mo22 O105 100.1(6) . . ?
O52 Mo22 O124 92.0(5) . . ?
O57 Mo22 Mo27 89.5(5) . . ?
O57 Mo22 O20 93.3(5) . . ?
O57 Mo22 O52 104.5(7) . . ?
O57 Mo22 O65 101.3(6) . . ?
O57 Mo22 O105 97.4(6) . . ?
O57 Mo22 O124 162.3(5) . . ?
O65 Mo22 Mo27 33.4(3) . . ?
O65 Mo22 O20 71.3(5) . . ?
O65 Mo22 O124 83.6(5) . . ?
O105 Mo22 Mo27 128.3(3) . . ?
O105 Mo22 O20 88.1(4) . . ?
O105 Mo22 O65 152.7(5) . . ?
O105 Mo22 O124 72.9(5) . . ?
O124 Mo22 Mo27 85.4(3) . . ?
O41 Mo23 Mo11 40.6(3) . . ?
O41 Mo23 O124 72.5(4) . . ?
O77 Mo23 Mo11 34.6(3) . . ?
O77 Mo23 O41 72.7(4) . . ?
O77 Mo23 O124 85.1(5) . . ?
O94 Mo23 Mo11 127.1(5) . . ?
O94 Mo23 O41 157.6(6) . . ?
O94 Mo23 O77 92.6(6) . . ?
O94 Mo23 O105 100.2(6) . . ?
O94 Mo23 O124 89.9(5) . . ?
O105 Mo23 Mo11 128.3(3) . . ?
O105 Mo23 O41 87.7(4) . . ?
O105 Mo23 O77 153.7(5) . . ?
O105 Mo23 O124 72.2(4) . . ?
O124 Mo23 Mo11 86.7(3) . . ?
O127 Mo23 Mo11 88.9(4) . . ?
O127 Mo23 O41 94.6(5) . . ?
O127 Mo23 O77 99.7(6) . . ?
O127 Mo23 O94 104.6(6) . . ?
O127 Mo23 O105 99.2(6) . . ?
O127 Mo23 O124 164.4(5) . . ?
Ti8 Mo24 Ti6 73.38(7) . . ?
O10 Mo24 Ti6 98.4(5) . . ?
O10 Mo24 Ti8 98.8(5) . . ?
O10 Mo24 O11 99.0(6) . . ?
O10 Mo24 O36 96.5(6) . . ?
O10 Mo24 O64 179.9(7) . . ?
O10 Mo24 O101 96.4(6) . . ?
O10 Mo24 O172 97.4(6) . . ?
O10 Mo24 O174 97.0(6) . . ?
O11 Mo24 Ti6 37.5(3) . . ?
O11 Mo24 Ti8 36.0(3) . . ?
O11 Mo24 O64 81.1(4) . . ?
O36 Mo24 Ti6 37.2(3) . . ?
O36 Mo24 Ti8 110.3(3) . . ?
O36 Mo24 O11 74.6(5) . . ?
O36 Mo24 O64 83.5(5) . . ?
O64 Mo24 Ti6 81.6(3) . . ?
O64 Mo24 Ti8 81.2(3) . . ?
O101 Mo24 Ti6 110.8(3) . . ?
O101 Mo24 Ti8 37.5(3) . . ?
O101 Mo24 O11 73.5(5) . . ?
O101 Mo24 O36 147.1(5) . . ?
O101 Mo24 O64 83.6(5) . . ?
O172 Mo24 Ti6 120.6(4) . . ?
O172 Mo24 Ti8 156.7(4) . . ?
O172 Mo24 O11 154.6(5) . . ?
O172 Mo24 O36 84.3(5) . . ?
O172 Mo24 O64 82.6(5) . . ?
O172 Mo24 O101 123.8(5) . . ?
O174 Mo24 Ti6 155.4(4) . . ?
O174 Mo24 Ti8 122.8(4) . . ?
O174 Mo24 O11 155.4(5) . . ?
O174 Mo24 O36 121.9(5) . . ?
O174 Mo24 O64 82.9(5) . . ?
O174 Mo24 O101 86.3(5) . . ?
O174 Mo24 O172 38.0(3) . . ?
O28 Mo25 Mo15 127.3(5) . . ?
O28 Mo25 O46 91.4(6) . . ?
O28 Mo25 O63 92.3(6) . . ?
O28 Mo25 O66 100.9(6) . . ?
O28 Mo25 O100 158.3(6) . . ?
O46 Mo25 Mo15 84.8(3) . . ?
O63 Mo25 Mo15 35.0(3) . . ?
O63 Mo25 O46 82.8(5) . . ?
O63 Mo25 O100 72.2(4) . . ?
O66 Mo25 Mo15 127.3(3) . . ?
O66 Mo25 O46 72.7(5) . . ?
O66 Mo25 O63 152.3(5) . . ?
O66 Mo25 O100 87.7(4) . . ?
O100 Mo25 Mo15 39.6(3) . . ?
O100 Mo25 O46 72.0(4) . . ?
O141 Mo25 Mo15 88.5(5) . . ?
O141 Mo25 O28 104.8(7) . . ?
O141 Mo25 O46 163.3(5) . . ?
O141 Mo25 O63 100.3(6) . . ?
O141 Mo25 O66 99.7(6) . . ?
O141 Mo25 O100 93.1(5) . . ?
Mo20 Mo26 Ti6 78.71(7) . . ?
O9 Mo26 Mo20 94.7(5) . . ?
O9 Mo26 Ti6 96.0(4) . . ?
O9 Mo26 O36 97.6(6) . . ?
O9 Mo26 O88 106.0(5) . . ?
O9 Mo26 O89 98.9(6) . . ?
O9 Mo26 O161 103.8(6) . . ?
O9 Mo26 O193 103.1(6) . . ?
O36 Mo26 Mo20 115.3(4) . . ?
O36 Mo26 Ti6 37.0(3) . . ?
O36 Mo26 O88 72.8(5) . . ?
O88 Mo26 Mo20 42.9(3) . . ?
O88 Mo26 Ti6 37.6(3) . . ?
O89 Mo26 Mo20 35.8(4) . . ?
O89 Mo26 Ti6 113.4(4) . . ?
O89 Mo26 O36 147.7(5) . . ?
O89 Mo26 O88 76.1(5) . . ?
O89 Mo26 O193 78.8(6) . . ?
O161 Mo26 Mo20 148.0(4) . . ?
O161 Mo26 Ti6 124.0(4) . . ?
O161 Mo26 O36 88.1(5) . . ?
O161 Mo26 O88 146.3(6) . . ?
O161 Mo26 O89 114.3(6) . . ?
O161 Mo26 O193 36.4(3) . . ?
O193 Mo26 Mo20 114.3(4) . . ?
O193 Mo26 Ti6 155.6(5) . . ?
O193 Mo26 O36 123.8(6) . . ?
O193 Mo26 O88 143.9(6) . . ?
Mo22 Mo27 Ti4 78.29(6) . . ?
O20 Mo27 Mo22 42.5(3) . . ?
O20 Mo27 Ti4 37.4(3) . . ?
O20 Mo27 O48 70.8(4) . . ?
O48 Mo27 Mo22 84.6(3) . . ?
O48 Mo27 Ti4 79.3(3) . . ?
O65 Mo27 Mo22 35.2(4) . . ?
O65 Mo27 Ti4 112.3(4) . . ?
O65 Mo27 O20 75.1(5) . . ?
O65 Mo27 O48 82.9(5) . . ?
O65 Mo27 O84 146.7(5) . . ?
O84 Mo27 Mo22 115.3(3) . . ?
O84 Mo27 Ti4 37.5(3) . . ?
O84 Mo27 O20 73.0(4) . . ?
O84 Mo27 O48 77.9(4) . . ?
O186 Mo27 Mo22 150.0(4) . . ?
O186 Mo27 Ti4 122.7(4) . . ?
O186 Mo27 O20 146.4(5) . . ?
O186 Mo27 O48 79.5(5) . . ?
O186 Mo27 O65 116.9(5) . . ?
O186 Mo27 O84 86.0(5) . . ?
O194 Mo27 Mo22 115.7(4) . . ?
O194 Mo27 Ti4 153.7(4) . . ?
O194 Mo27 O20 144.0(5) . . ?
O194 Mo27 O48 80.0(5) . . ?
O194 Mo27 O65 80.9(6) . . ?
O194 Mo27 O84 121.4(5) . . ?
O194 Mo27 O186 36.6(3) . . ?
O196 Mo27 Mo22 94.4(5) . . ?
O196 Mo27 Ti4 95.5(5) . . ?
O196 Mo27 O20 105.1(6) . . ?
O196 Mo27 O48 174.9(6) . . ?
O196 Mo27 O65 99.1(6) . . ?
O196 Mo27 O84 98.1(6) . . ?
O196 Mo27 O186 103.6(7) . . ?
O196 Mo27 O194 105.0(7) . . ?
Mo21 Mo28 Ti8 78.17(7) . . ?
O75 Mo28 Mo21 35.1(4) . . ?
O75 Mo28 Ti8 111.9(4) . . ?
O75 Mo28 O101 146.6(5) . . ?
O75 Mo28 O104 74.7(5) . . ?
O101 Mo28 Mo21 115.0(4) . . ?
O101 Mo28 Ti8 37.0(3) . . ?
O101 Mo28 O104 72.9(5) . . ?
O104 Mo28 Mo21 42.6(3) . . ?
O104 Mo28 Ti8 37.4(3) . . ?
O171 Mo28 Mo21 150.3(4) . . ?
O171 Mo28 Ti8 123.4(4) . . ?
O171 Mo28 O75 116.8(6) . . ?
O171 Mo28 O101 87.4(6) . . ?
O171 Mo28 O104 147.2(6) . . ?
O171 Mo28 O187 37.0(3) . . ?
O187 Mo28 Mo21 114.2(5) . . ?
O187 Mo28 Ti8 150.5(5) . . ?
O187 Mo28 O75 79.8(6) . . ?
O187 Mo28 O101 121.6(6) . . ?
O187 Mo28 O104 139.7(6) . . ?
O199 Mo28 Mo21 92.7(5) . . ?
O199 Mo28 Ti8 95.8(5) . . ?
O199 Mo28 O75 98.2(6) . . ?
O199 Mo28 O101 97.6(6) . . ?
O199 Mo28 O104 104.6(6) . . ?
O199 Mo28 O171 103.8(7) . . ?
O199 Mo28 O187 109.6(7) . . ?
O17 Mo29 K1 83.2(4) . . ?
O17 Mo29 O72 76.3(4) . . ?
O17 Mo29 O169 80.0(5) . . ?
O31 Mo29 K1 122.8(4) . . ?
O31 Mo29 O17 148.8(5) . . ?
O31 Mo29 O72 77.0(4) . . ?
O31 Mo29 O169 79.1(5) . . ?
O72 Mo29 K1 113.9(4) . . ?
O103 Mo29 K1 74.1(4) . . ?
O103 Mo29 O17 102.2(5) . . ?
O103 Mo29 O31 101.7(5) . . ?
O103 Mo29 O72 171.3(6) . . ?
O103 Mo29 O169 92.6(6) . . ?
O103 Mo29 O197 104.4(6) . . ?
O169 Mo29 K1 155.9(3) . . ?
O169 Mo29 O72 78.8(5) . . ?
O197 Mo29 K1 36.7(4) . . ?
O197 Mo29 O17 96.7(5) . . ?
O197 Mo29 O31 96.6(5) . . ?
O197 Mo29 O72 84.3(5) . . ?
O197 Mo29 O169 163.1(5) . . ?
O87 Mo30 O90 99.9(5) . . ?
O87 Mo30 O103 85.8(5) . . ?
O87 Mo30 O108 100.6(5) . . ?
O87 Mo30 O175 163.7(6) . . ?
O90 Mo30 O103 77.5(4) . . ?
O90 Mo30 O108 145.7(5) . . ?
O90 Mo30 O175 76.2(5) . . ?
O103 Mo30 O175 77.9(5) . . ?
O108 Mo30 O103 76.9(4) . . ?
O108 Mo30 O175 76.3(5) . . ?
O144 Mo30 O87 107.2(6) . . ?
O144 Mo30 O90 100.4(5) . . ?
O144 Mo30 O103 167.0(6) . . ?
O144 Mo30 O108 99.5(5) . . ?
O144 Mo30 O175 89.1(6) . . ?
Mo38 Mo31 Ti11 78.61(6) . . ?
Mo38 Mo31 K3 127.60(13) . . ?
Ti11 Mo31 K3 95.40(15) . . ?
O110 Mo31 Mo38 42.8(3) . . ?
O110 Mo31 Ti11 37.4(3) . . ?
O110 Mo31 K3 108.2(3) . . ?
O110 Mo31 O120 71.1(4) . . ?
O111 Mo31 Mo38 115.2(3) . . ?
O111 Mo31 Ti11 37.2(3) . . ?
O111 Mo31 K3 68.5(3) . . ?
O111 Mo31 O110 72.7(4) . . ?
O111 Mo31 O120 78.3(4) . . ?
O117 Mo31 Mo38 94.8(4) . . ?
O117 Mo31 Ti11 95.1(4) . . ?
O117 Mo31 K3 137.6(4) . . ?
O117 Mo31 O110 105.0(5) . . ?
O117 Mo31 O111 97.7(5) . . ?
O117 Mo31 O120 175.0(4) . . ?
O117 Mo31 O123 99.8(5) . . ?
O117 Mo31 O162 102.9(6) . . ?
O117 Mo31 O188 104.6(6) . . ?
O120 Mo31 Mo38 84.3(3) . . ?
O120 Mo31 Ti11 79.9(2) . . ?
O120 Mo31 K3 43.8(3) . . ?
O123 Mo31 Mo38 35.5(3) . . ?
O123 Mo31 Ti11 113.0(3) . . ?
O123 Mo31 K3 113.4(4) . . ?
O123 Mo31 O110 75.7(4) . . ?
O123 Mo31 O111 146.9(5) . . ?
O123 Mo31 O120 82.3(4) . . ?
O162 Mo31 Mo38 150.9(4) . . ?
O162 Mo31 Ti11 121.8(4) . . ?
O162 Mo31 K3 38.7(4) . . ?
O162 Mo31 O110 146.4(5) . . ?
O162 Mo31 O111 85.4(5) . . ?
O162 Mo31 O120 79.9(5) . . ?
O162 Mo31 O123 117.4(5) . . ?
O188 Mo31 Mo38 115.7(4) . . ?
O188 Mo31 Ti11 154.0(4) . . ?
O188 Mo31 K3 58.6(4) . . ?
O188 Mo31 O110 144.7(5) . . ?
O188 Mo31 O111 121.6(5) . . ?
O188 Mo31 O120 80.2(5) . . ?
O188 Mo31 O123 80.6(5) . . ?
O188 Mo31 O162 37.5(3) . . ?
Ti1 Mo32 K2 94.80(10) . . ?
Ti11 Mo32 Ti1 73.76(6) . . ?
Ti11 Mo32 K2 131.34(11) . . ?
O111 Mo32 Ti1 111.4(3) . . ?
O111 Mo32 Ti11 38.0(3) . . ?
O111 Mo32 K2 121.3(3) . . ?
O111 Mo32 O114 74.4(4) . . ?
O111 Mo32 O132 82.3(4) . . ?
O114 Mo32 Ti1 37.0(3) . . ?
O114 Mo32 Ti11 36.9(3) . . ?
O114 Mo32 K2 116.3(3) . . ?
O114 Mo32 O132 76.0(4) . . ?
O119 Mo32 Ti1 37.8(3) . . ?
O119 Mo32 Ti11 111.4(3) . . ?
O119 Mo32 K2 67.3(3) . . ?
O119 Mo32 O111 148.0(4) . . ?
O119 Mo32 O114 74.5(4) . . ?
O119 Mo32 O132 82.7(4) . . ?
O122 Mo32 Ti1 97.5(4) . . ?
O122 Mo32 Ti11 95.5(4) . . ?
O122 Mo32 K2 133.1(4) . . ?
O122 Mo32 O111 95.5(5) . . ?
O122 Mo32 O114 99.8(5) . . ?
O122 Mo32 O119 97.3(5) . . ?
O122 Mo32 O132 175.6(5) . . ?
O122 Mo32 O192 99.2(6) . . ?
O122 Mo32 O195 99.2(6) . . ?
O132 Mo32 Ti1 79.8(3) . . ?
O132 Mo32 Ti11 80.5(3) . . ?
O132 Mo32 K2 50.9(3) . . ?
O192 Mo32 Ti1 122.0(4) . . ?
O192 Mo32 Ti11 156.4(4) . . ?
O192 Mo32 K2 38.3(4) . . ?
O192 Mo32 O111 121.6(5) . . ?
O192 Mo32 O114 153.6(5) . . ?
O192 Mo32 O119 85.0(5) . . ?
O192 Mo32 O132 85.2(5) . . ?
O195 Mo32 Ti1 155.9(4) . . ?
O195 Mo32 Ti11 121.5(4) . . ?
O195 Mo32 K2 61.1(4) . . ?
O195 Mo32 O111 84.2(5) . . ?
O195 Mo32 O114 152.6(5) . . ?
O195 Mo32 O119 122.2(5) . . ?
O195 Mo32 O132 84.4(5) . . ?
O195 Mo32 O192 37.8(3) . . ?
Mo10 Mo33 Ti1 78.14(6) . . ?
Mo10 Mo33 K2 126.45(10) . . ?
Ti1 Mo33 K2 95.70(11) . . ?
O39 Mo33 Mo10 34.7(3) . . ?
O39 Mo33 Ti1 111.9(3) . . ?
O39 Mo33 K2 113.3(4) . . ?
O39 Mo33 O102 74.7(4) . . ?
O39 Mo33 O119 146.5(5) . . ?
O102 Mo33 Mo10 42.6(3) . . ?
O102 Mo33 Ti1 37.5(3) . . ?
O102 Mo33 K2 106.9(3) . . ?
O119 Mo33 Mo10 115.2(3) . . ?
O119 Mo33 Ti1 37.7(3) . . ?
O119 Mo33 K2 68.9(3) . . ?
O119 Mo33 O102 73.0(4) . . ?
O139 Mo33 Mo10 95.3(4) . . ?
O139 Mo33 Ti1 94.9(4) . . ?
O139 Mo33 K2 138.2(4) . . ?
O139 Mo33 O39 99.7(5) . . ?
O139 Mo33 O102 106.0(5) . . ?
O139 Mo33 O119 97.3(5) . . ?
O139 Mo33 O164 103.4(6) . . ?
O139 Mo33 O185 103.1(6) . . ?
O164 Mo33 Mo10 149.0(4) . . ?
O164 Mo33 Ti1 123.7(4) . . ?
O164 Mo33 K2 39.3(4) . . ?
O164 Mo33 O39 116.5(5) . . ?
O164 Mo33 O102 146.1(5) . . ?
O164 Mo33 O119 86.9(5) . . ?
O164 Mo33 O185 37.0(3) . . ?
O185 Mo33 Mo10 114.8(4) . . ?
O185 Mo33 Ti1 156.3(4) . . ?
O185 Mo33 K2 60.6(4) . . ?
O185 Mo33 O39 80.4(5) . . ?
O185 Mo33 O102 144.3(5) . . ?
O185 Mo33 O119 123.2(5) . . ?
Ti12 Mo34 Ti11 55.67(6) . . ?
O110 Mo34 Ti11 37.4(3) . . ?
O110 Mo34 Ti12 83.5(3) . . ?
O112 Mo34 Ti11 36.8(3) . . ?
O112 Mo34 Ti12 37.0(3) . . ?
O112 Mo34 O110 74.3(4) . . ?
O112 Mo34 O113 74.5(4) . . ?
O113 Mo34 Ti11 82.6(3) . . ?
O113 Mo34 Ti12 37.6(3) . . ?
O113 Mo34 O110 92.1(4) . . ?
O120 Mo34 Ti11 90.5(4) . . ?
O120 Mo34 Ti12 138.2(4) . . ?
O120 Mo34 O110 81.0(4) . . ?
O120 Mo34 O112 101.2(5) . . ?
O120 Mo34 O113 172.7(5) . . ?
O120 Mo34 O137 102.8(5) . . ?
O128 Mo34 Ti11 139.2(4) . . ?
O128 Mo34 Ti12 90.2(4) . . ?
O128 Mo34 O110 173.0(5) . . ?
O128 Mo34 O112 102.5(5) . . ?
O128 Mo34 O113 81.1(5) . . ?
O128 Mo34 O120 105.8(5) . . ?
O128 Mo34 O137 102.8(5) . . ?
O137 Mo34 Ti11 109.8(3) . . ?
O137 Mo34 Ti12 111.1(3) . . ?
O137 Mo34 O110 76.7(4) . . ?
O137 Mo34 O112 138.6(5) . . ?
O137 Mo34 O113 77.7(4) . . ?
O26 Mo35 Mo8 40.0(3) . . ?
O26 Mo35 O147 72.2(4) . . ?
O47 Mo35 Mo8 33.5(3) . . ?
O47 Mo35 O26 71.2(4) . . ?
O47 Mo35 O147 84.4(5) . . ?
O143 Mo35 Mo8 127.5(4) . . ?
O143 Mo35 O26 87.6(5) . . ?
O143 Mo35 O47 152.4(5) . . ?
O143 Mo35 O147 72.1(5) . . ?
O147 Mo35 Mo8 85.8(3) . . ?
O155 Mo35 Mo8 88.8(5) . . ?
O155 Mo35 O26 94.2(5) . . ?
O155 Mo35 O47 99.3(6) . . ?
O155 Mo35 O143 99.7(6) . . ?
O155 Mo35 O147 164.0(5) . . ?
O155 Mo35 O156 105.0(6) . . ?
O156 Mo35 Mo8 126.1(4) . . ?
O156 Mo35 O26 156.8(6) . . ?
O156 Mo35 O47 92.6(5) . . ?
O156 Mo35 O143 101.6(5) . . ?
O156 Mo35 O147 90.3(5) . . ?
O116 Mo36 Mo43 33.5(3) . . ?
O116 Mo36 O118 71.2(4) . . ?
O116 Mo36 O147 82.8(4) . . ?
O118 Mo36 Mo43 40.5(3) . . ?
O118 Mo36 O147 71.5(4) . . ?
O133 Mo36 Mo43 90.3(4) . . ?
O133 Mo36 O116 101.9(6) . . ?
O133 Mo36 O118 95.5(5) . . ?
O133 Mo36 O134 104.4(6) . . ?
O133 Mo36 O143 98.8(6) . . ?
O133 Mo36 O147 164.2(5) . . ?
O134 Mo36 Mo43 126.9(4) . . ?
O134 Mo36 O116 93.4(5) . . ?
O134 Mo36 O118 157.1(5) . . ?
O134 Mo36 O143 100.9(6) . . ?
O134 Mo36 O147 90.2(5) . . ?
O143 Mo36 Mo43 127.3(3) . . ?
O143 Mo36 O116 151.0(5) . . ?
O143 Mo36 O118 86.8(5) . . ?
O143 Mo36 O147 72.1(5) . . ?
O147 Mo36 Mo43 85.5(3) . . ?
O113 Mo37 Mo13 40.1(3) . . ?
O113 Mo37 O137 72.1(4) . . ?
O135 Mo37 Mo13 33.8(3) . . ?
O135 Mo37 O113 71.5(4) . . ?
O135 Mo37 O137 84.3(5) . . ?
O137 Mo37 Mo13 85.9(3) . . ?
O138 Mo37 Mo13 126.1(4) . . ?
O138 Mo37 O113 157.9(5) . . ?
O138 Mo37 O135 92.3(5) . . ?
O138 Mo37 O137 91.9(5) . . ?
O138 Mo37 O149 104.5(6) . . ?
O138 Mo37 O154 101.2(5) . . ?
O149 Mo37 Mo13 88.9(5) . . ?
O149 Mo37 O113 93.4(5) . . ?
O149 Mo37 O135 100.4(6) . . ?
O149 Mo37 O137 162.6(5) . . ?
O149 Mo37 O154 98.0(6) . . ?
O154 Mo37 Mo13 128.8(3) . . ?
O154 Mo37 O113 88.7(4) . . ?
O154 Mo37 O135 153.6(5) . . ?
O154 Mo37 O137 72.8(4) . . ?
Mo31 Mo38 K8 120.44(18) . . ?
O110 Mo38 Mo31 39.8(3) . . ?
O110 Mo38 O137 72.3(4) . . ?
O110 Mo38 K8 107.7(3) . . ?
O123 Mo38 Mo31 33.8(3) . . ?
O123 Mo38 O110 71.3(4) . . ?
O123 Mo38 O137 83.9(4) . . ?
O123 Mo38 K8 134.7(4) . . ?
O125 Mo38 Mo31 126.8(4) . . ?
O125 Mo38 O110 156.7(5) . . ?
O125 Mo38 O123 93.0(5) . . ?
O125 Mo38 O137 89.3(5) . . ?
O125 Mo38 O151 105.7(6) . . ?
O125 Mo38 O154 101.4(5) . . ?
O125 Mo38 K8 95.6(5) . . ?
O137 Mo38 Mo31 85.7(3) . . ?
O137 Mo38 K8 140.5(3) . . ?
O151 Mo38 Mo31 89.9(4) . . ?
O151 Mo38 O110 94.4(5) . . ?
O151 Mo38 O123 100.9(5) . . ?
O151 Mo38 O137 163.9(5) . . ?
O151 Mo38 O154 97.6(5) . . ?
O151 Mo38 K8 34.1(4) . . ?
O154 Mo38 Mo31 127.0(3) . . ?
O154 Mo38 O110 87.2(4) . . ?
O154 Mo38 O123 152.5(5) . . ?
O154 Mo38 O137 73.1(4) . . ?
O154 Mo38 K8 67.5(4) . . ?
O12 Mo39 K1 83.9(4) . . ?
O12 Mo39 O38 146.5(6) . . ?
O12 Mo39 O82 75.7(5) . . ?
O12 Mo39 O157 77.6(5) . . ?
O38 Mo39 K1 128.8(4) . . ?
O38 Mo39 O82 75.7(5) . . ?
O38 Mo39 O157 76.8(5) . . ?
O80 Mo39 K1 51.2(5) . . ?
O80 Mo39 O12 98.9(6) . . ?
O80 Mo39 O38 98.3(6) . . ?
O80 Mo39 O82 90.4(6) . . ?
O80 Mo39 O140 116.2(7) . . ?
O80 Mo39 O157 161.0(6) . . ?
O82 Mo39 K1 132.9(4) . . ?
O140 Mo39 K1 70.8(5) . . ?
O140 Mo39 O12 99.1(6) . . ?
O140 Mo39 O38 98.8(6) . . ?
O140 Mo39 O82 153.5(6) . . ?
O140 Mo39 O157 82.8(6) . . ?
O157 Mo39 K1 144.9(4) . . ?
O157 Mo39 O82 70.7(5) . . ?
O37 Mo17 O165 75.2(5) . . ?
O91 Mo17 O37 141.6(6) . . ?
O91 Mo17 O165 73.7(5) . . ?
O140 Mo17 O37 98.1(6) . . ?
O140 Mo17 O91 99.9(6) . . ?
O140 Mo17 O165 153.7(7) . . ?
O202 Mo17 O37 98.2(7) . . ?
O202 Mo17 O91 100.1(7) . . ?
O202 Mo17 O140 122.6(8) . . ?
O202 Mo17 O165 83.7(7) . . ?
Mo42 Mo41 K4 67.8(2) . . ?
O14 Mo41 Mo42 102.8(4) . . ?
O14 Mo41 O136 76.8(5) . . ?
O14 Mo41 O176 75.5(5) . . ?
O14 Mo41 K4 111.0(4) . . ?
O34 Mo41 Mo42 95.6(5) . . ?
O34 Mo41 O14 100.9(6) . . ?
O34 Mo41 O58 112.1(7) . . ?
O34 Mo41 O109 100.0(6) . . ?
O34 Mo41 O136 85.0(6) . . ?
O34 Mo41 O176 160.3(6) . . ?
O34 Mo41 K4 28.3(5) . . ?
O58 Mo41 Mo42 16.5(4) . . ?
O58 Mo41 O14 98.8(5) . . ?
O58 Mo41 O109 99.9(5) . . ?
O58 Mo41 O136 162.9(6) . . ?
O58 Mo41 O176 87.5(5) . . ?
O58 Mo41 K4 84.2(5) . . ?
O109 Mo41 Mo42 103.8(4) . . ?
O109 Mo41 O14 144.2(5) . . ?
O109 Mo41 O136 76.4(5) . . ?
O109 Mo41 O176 75.1(5) . . ?
O109 Mo41 K4 101.1(4) . . ?
O136 Mo41 Mo42 179.4(4) . . ?
O136 Mo41 O176 75.4(5) . . ?
O136 Mo41 K4 112.8(4) . . ?
O176 Mo41 Mo42 104.1(3) . . ?
O176 Mo41 K4 170.2(4) . . ?
Mo41 Mo42 K4 65.9(2) . . ?
O32 Mo42 Mo41 105.3(4) . . ?
O32 Mo42 O131 74.0(5) . . ?
O32 Mo42 O200 73.3(5) . . ?
O32 Mo42 K4 103.1(4) . . ?
O58 Mo42 Mo41 17.0(4) . . ?
O58 Mo42 O32 100.9(6) . . ?
O58 Mo42 O67 101.1(6) . . ?
O58 Mo42 O81 116.4(7) . . ?
O58 Mo42 O131 163.5(6) . . ?
O58 Mo42 O200 89.4(5) . . ?
O58 Mo42 K4 82.8(5) . . ?
O67 Mo42 Mo41 105.0(4) . . ?
O67 Mo42 O32 141.2(5) . . ?
O67 Mo42 O131 75.9(5) . . ?
O67 Mo42 O200 75.4(4) . . ?
O67 Mo42 K4 111.1(4) . . ?
O81 Mo42 Mo41 99.5(5) . . ?
O81 Mo42 O32 98.0(6) . . ?
O81 Mo42 O67 100.3(6) . . ?
O81 Mo42 O131 80.0(6) . . ?
O81 Mo42 O200 154.1(6) . . ?
O81 Mo42 K4 33.7(5) . . ?
O131 Mo42 Mo41 179.0(4) . . ?
O131 Mo42 O200 74.1(4) . . ?
O131 Mo42 K4 113.5(4) . . ?
O200 Mo42 Mo41 106.4(3) . . ?
O200 Mo42 K4 170.6(4) . . ?
Mo32 Ti1 Mo1 100.52(7) . . ?
Mo32 Ti1 Mo33 72.55(6) . . ?
Mo33 Ti1 Mo1 63.54(5) . . ?
Ti2 Ti1 Mo1 61.71(6) . . ?
Ti2 Ti1 Mo32 123.46(9) . . ?
Ti2 Ti1 Mo33 124.86(9) . . ?
O1 Ti1 Mo1 33.0(3) . . ?
O1 Ti1 Mo32 91.5(3) . . ?
O1 Ti1 Mo33 90.2(3) . . ?
O1 Ti1 Ti2 43.1(3) . . ?
O8 Ti1 Mo1 102.4(3) . . ?
O8 Ti1 Mo32 122.4(3) . . ?
O8 Ti1 Mo33 162.5(3) . . ?
O8 Ti1 Ti2 40.9(3) . . ?
O8 Ti1 O1 80.9(4) . . ?
O8 Ti1 O16 42.4(3) . . ?
O8 Ti1 O102 123.6(4) . . ?
O8 Ti1 O119 155.1(4) . . ?
O12 Ti1 Mo1 142.2(3) . . ?
O12 Ti1 Mo32 96.4(3) . . ?
O12 Ti1 Mo33 90.3(3) . . ?
O12 Ti1 Ti2 131.6(4) . . ?
O12 Ti1 O1 171.8(4) . . ?
O12 Ti1 O8 96.4(5) . . ?
O12 Ti1 O16 93.7(5) . . ?
O12 Ti1 O102 98.0(4) . . ?
O12 Ti1 O114 97.3(4) . . ?
O12 Ti1 O119 98.1(5) . . ?
O16 Ti1 Mo1 79.4(3) . . ?
O16 Ti1 Mo32 162.9(3) . . ?
O16 Ti1 Mo33 121.2(3) . . ?
O16 Ti1 Ti2 41.5(3) . . ?
O16 Ti1 O1 79.1(4) . . ?
O102 Ti1 Mo1 44.4(3) . . ?
O102 Ti1 Mo32 109.7(3) . . ?
O102 Ti1 Mo33 39.1(3) . . ?
O102 Ti1 Ti2 93.3(3) . . ?
O102 Ti1 O1 77.3(4) . . ?
O102 Ti1 O16 82.4(4) . . ?
O102 Ti1 O119 74.1(4) . . ?
O114 Ti1 Mo1 116.5(3) . . ?
O114 Ti1 Mo32 37.4(3) . . ?
O114 Ti1 Mo33 109.9(3) . . ?
O114 Ti1 Ti2 99.5(3) . . ?
O114 Ti1 O1 90.2(4) . . ?
O114 Ti1 O8 85.3(4) . . ?
O114 Ti1 O16 127.5(4) . . ?
O114 Ti1 O102 145.2(4) . . ?
O114 Ti1 O119 72.9(4) . . ?
O119 Ti1 Mo1 77.7(3) . . ?
O119 Ti1 Mo32 35.7(3) . . ?
O119 Ti1 Mo33 37.2(3) . . ?
O119 Ti1 Ti2 130.2(3) . . ?
O119 Ti1 O1 87.1(4) . . ?
O119 Ti1 O16 154.9(4) . . ?
Mo7 Ti2 Mo1 64.11(6) . . ?
Mo9 Ti2 Mo1 97.79(7) . . ?
Mo9 Ti2 Mo7 72.68(6) . . ?
Ti1 Ti2 Mo1 62.53(6) . . ?
Ti1 Ti2 Mo7 126.21(9) . . ?
Ti1 Ti2 Mo9 120.67(9) . . ?
O1 Ti2 Mo1 33.6(3) . . ?
O1 Ti2 Mo7 91.5(3) . . ?
O1 Ti2 Mo9 88.4(3) . . ?
O1 Ti2 Ti1 43.2(3) . . ?
O2 Ti2 Mo1 115.7(3) . . ?
O2 Ti2 Mo7 109.6(3) . . ?
O2 Ti2 Mo9 37.0(3) . . ?
O2 Ti2 Ti1 98.8(3) . . ?
O2 Ti2 O1 89.3(4) . . ?
O2 Ti2 O7 73.0(4) . . ?
O2 Ti2 O8 85.3(4) . . ?
O2 Ti2 O16 127.2(4) . . ?
O2 Ti2 O25 144.7(5) . . ?
O7 Ti2 Mo1 78.5(3) . . ?
O7 Ti2 Mo7 36.6(3) . . ?
O7 Ti2 Mo9 36.1(3) . . ?
O7 Ti2 Ti1 132.0(3) . . ?
O7 Ti2 O1 88.9(4) . . ?
O7 Ti2 O8 156.0(4) . . ?
O7 Ti2 O16 155.7(4) . . ?
O7 Ti2 O25 73.9(5) . . ?
O8 Ti2 Mo1 102.6(3) . . ?
O8 Ti2 Mo7 163.0(3) . . ?
O8 Ti2 Mo9 121.5(3) . . ?
O8 Ti2 Ti1 40.3(3) . . ?
O8 Ti2 O1 80.4(4) . . ?
O8 Ti2 O16 42.1(3) . . ?
O16 Ti2 Mo1 80.0(3) . . ?
O16 Ti2 Mo7 121.9(3) . . ?
O16 Ti2 Mo9 160.7(3) . . ?
O16 Ti2 Ti1 41.5(3) . . ?
O16 Ti2 O1 79.2(4) . . ?
O25 Ti2 Mo1 44.6(3) . . ?
O25 Ti2 Mo7 39.3(3) . . ?
O25 Ti2 Mo9 109.1(3) . . ?
O25 Ti2 Ti1 94.2(3) . . ?
O25 Ti2 O1 78.1(4) . . ?
O25 Ti2 O8 123.8(4) . . ?
O25 Ti2 O16 82.9(4) . . ?
O108 Ti2 Mo1 142.8(4) . . ?
O108 Ti2 Mo7 90.3(4) . . ?
O108 Ti2 Mo9 99.6(4) . . ?
O108 Ti2 Ti1 130.7(4) . . ?
O108 Ti2 O1 171.9(5) . . ?
O108 Ti2 O2 97.5(5) . . ?
O108 Ti2 O7 97.2(5) . . ?
O108 Ti2 O8 95.8(5) . . ?
O108 Ti2 O16 93.2(5) . . ?
O108 Ti2 O25 98.5(5) . . ?
Mo12 Ti3 Mo4 62.84(6) . . ?
Mo14 Ti3 Mo4 101.97(7) . . ?
Mo14 Ti3 Mo12 72.74(6) . . ?
Ti6 Ti3 Mo4 61.51(7) . . ?
Ti6 Ti3 Mo12 124.04(9) . . ?
Ti6 Ti3 Mo14 124.35(10) . . ?
O13 Ti3 Mo4 102.3(3) . . ?
O13 Ti3 Mo12 162.3(3) . . ?
O13 Ti3 Mo14 122.0(3) . . ?
O13 Ti3 Ti6 41.0(3) . . ?
O13 Ti3 O22 154.8(4) . . ?
O13 Ti3 O30 42.4(3) . . ?
O13 Ti3 O73 80.3(4) . . ?
O22 Ti3 Mo4 77.6(3) . . ?
O22 Ti3 Mo12 36.8(3) . . ?
O22 Ti3 Mo14 36.4(3) . . ?
O22 Ti3 Ti6 129.9(3) . . ?
O22 Ti3 O30 155.1(4) . . ?
O22 Ti3 O73 87.4(4) . . ?
O30 Ti3 Mo4 79.6(3) . . ?
O30 Ti3 Mo12 121.6(3) . . ?
O30 Ti3 Mo14 163.2(3) . . ?
O30 Ti3 Ti6 41.7(3) . . ?
O30 Ti3 O73 78.9(4) . . ?
O44 Ti3 Mo4 45.1(3) . . ?
O44 Ti3 Mo12 38.5(3) . . ?
O44 Ti3 Mo14 109.9(3) . . ?
O44 Ti3 Ti6 94.1(3) . . ?
O44 Ti3 O13 124.4(4) . . ?
O44 Ti3 O22 73.6(4) . . ?
O44 Ti3 O30 83.3(4) . . ?
O44 Ti3 O73 78.1(4) . . ?
O67 Ti3 Mo4 142.1(4) . . ?
O67 Ti3 Mo12 91.5(3) . . ?
O67 Ti3 Mo14 95.5(4) . . ?
O67 Ti3 Ti6 131.3(4) . . ?
O67 Ti3 O13 96.3(5) . . ?
O67 Ti3 O22 98.7(5) . . ?
O67 Ti3 O30 93.1(5) . . ?
O67 Ti3 O44 97.4(5) . . ?
O67 Ti3 O73 171.1(5) . . ?
O67 Ti3 O98 96.5(5) . . ?
O73 Ti3 Mo4 33.1(3) . . ?
O73 Ti3 Mo12 89.6(3) . . ?
O73 Ti3 Mo14 93.3(3) . . ?
O73 Ti3 Ti6 42.6(3) . . ?
O98 Ti3 Mo4 117.8(3) . . ?
O98 Ti3 Mo12 110.7(3) . . ?
O98 Ti3 Mo14 38.1(3) . . ?
O98 Ti3 Ti6 99.5(3) . . ?
O98 Ti3 O13 84.2(4) . . ?
O98 Ti3 O22 74.0(4) . . ?
O98 Ti3 O30 126.4(4) . . ?
O98 Ti3 O44 146.3(5) . . ?
O98 Ti3 O73 91.3(4) . . ?
Mo18 Ti4 Mo3 96.60(7) . . ?
Mo18 Ti4 Mo27 72.47(7) . . ?
Mo27 Ti4 Mo3 63.45(6) . . ?
Ti5 Ti4 Mo3 62.67(7) . . ?
Ti5 Ti4 Mo18 119.89(9) . . ?
Ti5 Ti4 Mo27 125.71(9) . . ?
O3 Ti4 Mo3 33.5(3) . . ?
O3 Ti4 Mo18 87.4(3) . . ?
O3 Ti4 Mo27 90.8(3) . . ?
O3 Ti4 Ti5 43.3(3) . . ?
O6 Ti4 Mo3 115.3(3) . . ?
O6 Ti4 Mo18 37.6(3) . . ?
O6 Ti4 Mo27 110.1(3) . . ?
O6 Ti4 Ti5 98.2(3) . . ?
O6 Ti4 O3 88.9(4) . . ?
O6 Ti4 O15 126.8(4) . . ?
O6 Ti4 O20 145.2(5) . . ?
O6 Ti4 O45 85.0(4) . . ?
O6 Ti4 O84 73.2(5) . . ?
O15 Ti4 Mo3 80.7(3) . . ?
O15 Ti4 Mo18 160.7(3) . . ?
O15 Ti4 Mo27 121.8(3) . . ?
O15 Ti4 Ti5 42.1(3) . . ?
O15 Ti4 O3 79.8(4) . . ?
O20 Ti4 Mo3 44.9(3) . . ?
O20 Ti4 Mo18 108.8(3) . . ?
O20 Ti4 Mo27 39.2(3) . . ?
O20 Ti4 Ti5 94.3(3) . . ?
O20 Ti4 O3 78.3(4) . . ?
O20 Ti4 O15 82.9(4) . . ?
O20 Ti4 O45 123.8(4) . . ?
O20 Ti4 O84 74.1(5) . . ?
O38 Ti4 Mo3 142.6(4) . . ?
O38 Ti4 Mo18 100.5(4) . . ?
O38 Ti4 Mo27 90.5(4) . . ?
O38 Ti4 Ti5 131.0(4) . . ?
O38 Ti4 O3 172.0(5) . . ?
O38 Ti4 O6 98.1(5) . . ?
O38 Ti4 O15 92.8(5) . . ?
O38 Ti4 O20 97.9(5) . . ?
O38 Ti4 O45 95.6(5) . . ?
O38 Ti4 O84 97.5(5) . . ?
O45 Ti4 Mo3 103.2(3) . . ?
O45 Ti4 Mo18 121.8(3) . . ?
O45 Ti4 Mo27 162.8(3) . . ?
O45 Ti4 Ti5 40.8(3) . . ?
O45 Ti4 O3 81.0(4) . . ?
O45 Ti4 O15 42.1(3) . . ?
O45 Ti4 O84 156.0(4) . . ?
O84 Ti4 Mo3 77.9(3) . . ?
O84 Ti4 Mo18 35.6(3) . . ?
O84 Ti4 Mo27 36.9(3) . . ?
O84 Ti4 Ti5 131.5(3) . . ?
O84 Ti4 O3 88.3(4) . . ?
O84 Ti4 O15 155.9(4) . . ?
Mo6 Ti5 Mo3 101.41(7) . . ?
Mo6 Ti5 Mo11 72.07(7) . . ?
Mo11 Ti5 Mo3 63.58(6) . . ?
Ti4 Ti5 Mo3 61.60(7) . . ?
Ti4 Ti5 Mo6 124.25(9) . . ?
Ti4 Ti5 Mo11 124.87(9) . . ?
O3 Ti5 Mo3 33.1(3) . . ?
O3 Ti5 Mo6 93.1(3) . . ?
O3 Ti5 Mo11 90.4(3) . . ?
O3 Ti5 Ti4 42.4(3) . . ?
O15 Ti5 Mo3 79.7(3) . . ?
O15 Ti5 Mo6 163.4(3) . . ?
O15 Ti5 Mo11 121.9(3) . . ?
O15 Ti5 Ti4 41.8(3) . . ?
O15 Ti5 O3 78.8(4) . . ?
O32 Ti5 Mo3 142.1(4) . . ?
O32 Ti5 Mo6 95.2(4) . . ?
O32 Ti5 Mo11 90.3(4) . . ?
O32 Ti5 Ti4 132.0(4) . . ?
O32 Ti5 O3 171.5(5) . . ?
O32 Ti5 O15 93.6(5) . . ?
O32 Ti5 O41 97.7(5) . . ?
O32 Ti5 O45 96.7(5) . . ?
O32 Ti5 O97 97.8(5) . . ?
O32 Ti5 O99 96.7(5) . . ?
O41 Ti5 Mo3 44.7(3) . . ?
O41 Ti5 Mo6 109.7(3) . . ?
O41 Ti5 Mo11 39.3(3) . . ?
O41 Ti5 Ti4 93.7(3) . . ?
O41 Ti5 O3 77.7(4) . . ?
O41 Ti5 O15 82.9(4) . . ?
O41 Ti5 O97 73.1(4) . . ?
O45 Ti5 Mo3 102.3(3) . . ?
O45 Ti5 Mo6 122.7(3) . . ?
O45 Ti5 Mo11 162.7(3) . . ?
O45 Ti5 Ti4 40.9(3) . . ?
O45 Ti5 O3 80.4(4) . . ?
O45 Ti5 O15 42.0(3) . . ?
O45 Ti5 O41 123.7(4) . . ?
O45 Ti5 O97 155.9(4) . . ?
O97 Ti5 Mo3 77.3(3) . . ?
O97 Ti5 Mo6 36.7(3) . . ?
O97 Ti5 Mo11 35.8(3) . . ?
O97 Ti5 Ti4 130.1(3) . . ?
O97 Ti5 O3 87.8(4) . . ?
O97 Ti5 O15 154.6(4) . . ?
O99 Ti5 Mo3 116.9(3) . . ?
O99 Ti5 Mo6 37.0(3) . . ?
O99 Ti5 Mo11 109.0(3) . . ?
O99 Ti5 Ti4 100.1(3) . . ?
O99 Ti5 O3 91.1(4) . . ?
O99 Ti5 O15 127.8(4) . . ?
O99 Ti5 O41 144.9(5) . . ?
O99 Ti5 O45 85.9(4) . . ?
O99 Ti5 O97 73.4(4) . . ?
Mo24 Ti6 Mo4 97.03(7) . . ?
Mo24 Ti6 Mo26 72.90(7) . . ?
Mo26 Ti6 Mo4 64.35(6) . . ?
Ti3 Ti6 Mo4 62.66(7) . . ?
Ti3 Ti6 Mo24 120.40(10) . . ?
Ti3 Ti6 Mo26 126.47(9) . . ?
O11 Ti6 Mo4 114.9(3) . . ?
O11 Ti6 Mo24 37.2(3) . . ?
O11 Ti6 Mo26 110.0(3) . . ?
O11 Ti6 Ti3 98.4(3) . . ?
O11 Ti6 O13 85.3(4) . . ?
O11 Ti6 O30 127.0(4) . . ?
O11 Ti6 O73 88.5(4) . . ?
O13 Ti6 Mo4 102.7(3) . . ?
O13 Ti6 Mo24 121.7(3) . . ?
O13 Ti6 Mo26 162.8(3) . . ?
O13 Ti6 Ti3 40.2(3) . . ?
O13 Ti6 O30 42.0(3) . . ?
O13 Ti6 O73 79.9(4) . . ?
O30 Ti6 Mo4 80.5(3) . . ?
O30 Ti6 Mo24 160.7(3) . . ?
O30 Ti6 Mo26 121.7(3) . . ?
O30 Ti6 Ti3 41.6(3) . . ?
O30 Ti6 O73 79.1(4) . . ?
O36 Ti6 Mo4 79.0(3) . . ?
O36 Ti6 Mo24 36.6(3) . . ?
O36 Ti6 Mo26 36.3(3) . . ?
O36 Ti6 Ti3 133.4(4) . . ?
O36 Ti6 O11 73.7(5) . . ?
O36 Ti6 O13 157.2(5) . . ?
O36 Ti6 O30 155.9(4) . . ?
O36 Ti6 O73 90.6(5) . . ?
O73 Ti6 Mo4 33.8(3) . . ?
O73 Ti6 Mo24 88.1(3) . . ?
O73 Ti6 Mo26 92.4(3) . . ?
O73 Ti6 Ti3 42.9(3) . . ?
O88 Ti6 Mo4 45.0(3) . . ?
O88 Ti6 Mo24 109.2(3) . . ?
O88 Ti6 Mo26 39.5(3) . . ?
O88 Ti6 Ti3 94.1(3) . . ?
O88 Ti6 O11 144.9(5) . . ?
O88 Ti6 O13 123.4(4) . . ?
O88 Ti6 O30 82.7(4) . . ?
O88 Ti6 O36 73.9(5) . . ?
O88 Ti6 O73 78.6(4) . . ?
O90 Ti6 Mo4 144.8(4) . . ?
O90 Ti6 Mo24 99.2(4) . . ?
O90 Ti6 Mo26 91.0(4) . . ?
O90 Ti6 Ti3 130.5(4) . . ?
O90 Ti6 O11 96.6(5) . . ?
O90 Ti6 O13 95.0(5) . . ?
O90 Ti6 O30 93.4(5) . . ?
O90 Ti6 O36 96.1(5) . . ?
O90 Ti6 O73 172.6(5) . . ?
O90 Ti6 O88 100.0(5) . . ?
Mo43 Ti7 Mo2 63.68(6) . . ?
Mo18 Ti7 Mo2 96.54(7) . . ?
Mo18 Ti7 Mo43 72.65(7) . . ?
Ti10 Ti7 Mo2 62.86(7) . . ?
Ti10 Ti7 Mo43 126.05(9) . . ?
Ti10 Ti7 Mo18 120.14(9) . . ?
O6 Ti7 Mo2 115.5(3) . . ?
O6 Ti7 Mo43 110.2(3) . . ?
O6 Ti7 Mo18 37.7(3) . . ?
O6 Ti7 Ti10 98.5(3) . . ?
O6 Ti7 O21 127.2(4) . . ?
O6 Ti7 O24 89.2(4) . . ?
O6 Ti7 O35 74.2(4) . . ?
O6 Ti7 O85 85.3(4) . . ?
O6 Ti7 O118 145.2(5) . . ?
O21 Ti7 Mo2 80.6(3) . . ?
O21 Ti7 Mo43 121.4(3) . . ?
O21 Ti7 Mo18 160.9(3) . . ?
O21 Ti7 Ti10 41.9(3) . . ?
O21 Ti7 O24 79.5(4) . . ?
O21 Ti7 O85 42.2(3) . . ?
O24 Ti7 Mo2 33.5(3) . . ?
O24 Ti7 Mo43 91.4(3) . . ?
O24 Ti7 Mo18 87.7(3) . . ?
O24 Ti7 Ti10 43.2(3) . . ?
O35 Ti7 Mo2 77.7(3) . . ?
O35 Ti7 Mo43 36.0(3) . . ?
O35 Ti7 Mo18 36.6(3) . . ?
O35 Ti7 Ti10 132.2(3) . . ?
O35 Ti7 O21 154.9(4) . . ?
O35 Ti7 O24 89.0(4) . . ?
O35 Ti7 O85 157.5(4) . . ?
O85 Ti7 Mo2 103.7(3) . . ?
O85 Ti7 Mo43 162.9(3) . . ?
O85 Ti7 Mo18 122.1(3) . . ?
O85 Ti7 Ti10 41.1(3) . . ?
O85 Ti7 O24 81.4(4) . . ?
O91 Ti7 Mo2 142.9(4) . . ?
O91 Ti7 Mo43 90.2(4) . . ?
O91 Ti7 Mo18 100.2(4) . . ?
O91 Ti7 Ti10 130.9(4) . . ?
O91 Ti7 O6 97.5(5) . . ?
O91 Ti7 O21 93.0(5) . . ?
O91 Ti7 O24 172.1(5) . . ?
O91 Ti7 O35 96.8(5) . . ?
O91 Ti7 O85 95.0(5) . . ?
O91 Ti7 O118 98.6(5) . . ?
O118 Ti7 Mo2 44.5(3) . . ?
O118 Ti7 Mo43 39.4(3) . . ?
O118 Ti7 Mo18 108.8(3) . . ?
O118 Ti7 Ti10 93.9(3) . . ?
O118 Ti7 O21 82.4(4) . . ?
O118 Ti7 O24 77.9(4) . . ?
O118 Ti7 O35 73.4(5) . . ?
O118 Ti7 O85 123.6(4) . . ?
Mo24 Ti8 Mo5 99.23(7) . . ?
Mo24 Ti8 Mo28 72.96(7) . . ?
Mo28 Ti8 Mo5 64.14(6) . . ?
Ti9 Ti8 Mo5 63.02(7) . . ?
Ti9 Ti8 Mo24 122.17(9) . . ?
Ti9 Ti8 Mo28 126.68(10) . . ?
O11 Ti8 Mo5 117.1(3) . . ?
O11 Ti8 Mo24 36.9(3) . . ?
O11 Ti8 Mo28 109.9(3) . . ?
O11 Ti8 Ti9 99.7(3) . . ?
O11 Ti8 O27 85.2(4) . . ?
O11 Ti8 O78 90.4(4) . . ?
O11 Ti8 O79 127.1(4) . . ?
O11 Ti8 O101 73.6(5) . . ?
O11 Ti8 O104 145.4(5) . . ?
O27 Ti8 Mo5 103.5(3) . . ?
O27 Ti8 Mo24 121.6(3) . . ?
O27 Ti8 Mo28 163.5(3) . . ?
O27 Ti8 Ti9 40.7(3) . . ?
O27 Ti8 O78 80.7(4) . . ?
O27 Ti8 O79 42.0(3) . . ?
O31 Ti8 Mo5 140.7(4) . . ?
O31 Ti8 Mo24 99.8(4) . . ?
O31 Ti8 Mo28 89.4(4) . . ?
O31 Ti8 Ti9 129.5(4) . . ?
O31 Ti8 O11 98.4(5) . . ?
O31 Ti8 O27 95.1(5) . . ?
O31 Ti8 O78 169.9(5) . . ?
O31 Ti8 O79 91.3(5) . . ?
O31 Ti8 O101 96.1(5) . . ?
O31 Ti8 O104 96.1(5) . . ?
O78 Ti8 Mo5 34.1(3) . . ?
O78 Ti8 Mo24 90.2(3) . . ?
O78 Ti8 Mo28 92.2(3) . . ?
O78 Ti8 Ti9 43.2(3) . . ?
O78 Ti8 O79 79.4(4) . . ?
O79 Ti8 Mo5 80.7(3) . . ?
O79 Ti8 Mo24 161.5(3) . . ?
O79 Ti8 Mo28 122.2(3) . . ?
O79 Ti8 Ti9 41.5(3) . . ?
O101 Ti8 Mo5 79.7(3) . . ?
O101 Ti8 Mo24 36.7(3) . . ?
O101 Ti8 Mo28 36.3(3) . . ?
O101 Ti8 Ti9 134.3(4) . . ?
O101 Ti8 O27 157.3(4) . . ?
O101 Ti8 O78 91.1(5) . . ?
O101 Ti8 O79 156.8(4) . . ?
O104 Ti8 Mo5 45.0(3) . . ?
O104 Ti8 Mo24 109.6(3) . . ?
O104 Ti8 Mo28 39.1(3) . . ?
O104 Ti8 Ti9 94.8(4) . . ?
O104 Ti8 O27 124.5(5) . . ?
O104 Ti8 O78 79.0(4) . . ?
O104 Ti8 O79 83.6(4) . . ?
O104 Ti8 O101 73.8(5) . . ?
Mo14 Ti9 Mo5 100.61(7) . . ?
Mo14 Ti9 Mo15 72.84(6) . . ?
Mo15 Ti9 Mo5 62.58(6) . . ?
Ti8 Ti9 Mo5 61.26(7) . . ?
Ti8 Ti9 Mo14 122.91(9) . . ?
Ti8 Ti9 Mo15 123.55(9) . . ?
O14 Ti9 Mo5 141.9(4) . . ?
O14 Ti9 Mo14 96.4(4) . . ?
O14 Ti9 Mo15 90.9(4) . . ?
O14 Ti9 Ti8 132.4(4) . . ?
O14 Ti9 O23 98.1(5) . . ?
O14 Ti9 O27 97.2(5) . . ?
O14 Ti9 O78 171.7(5) . . ?
O14 Ti9 O79 93.5(5) . . ?
O14 Ti9 O98 97.6(5) . . ?
O14 Ti9 O100 97.5(5) . . ?
O23 Ti9 Mo5 77.4(3) . . ?
O23 Ti9 Mo14 36.2(3) . . ?
O23 Ti9 Mo15 36.9(3) . . ?
O23 Ti9 Ti8 129.4(3) . . ?
O23 Ti9 O78 87.2(4) . . ?
O23 Ti9 O79 154.9(4) . . ?
O27 Ti9 Mo5 102.1(3) . . ?
O27 Ti9 Mo14 121.9(3) . . ?
O27 Ti9 Mo15 161.9(3) . . ?
O27 Ti9 Ti8 41.1(3) . . ?
O27 Ti9 O23 154.7(4) . . ?
O27 Ti9 O78 80.1(4) . . ?
O27 Ti9 O79 42.4(3) . . ?
O78 Ti9 Mo5 33.3(3) . . ?
O78 Ti9 Mo14 91.6(3) . . ?
O78 Ti9 Mo15 89.5(3) . . ?
O78 Ti9 Ti8 42.3(3) . . ?
O79 Ti9 Mo5 79.7(3) . . ?
O79 Ti9 Mo14 162.7(3) . . ?
O79 Ti9 Mo15 121.2(3) . . ?
O79 Ti9 Ti8 42.2(3) . . ?
O79 Ti9 O78 79.2(4) . . ?
O98 Ti9 Mo5 116.7(3) . . ?
O98 Ti9 Mo14 38.1(3) . . ?
O98 Ti9 Mo15 110.9(3) . . ?
O98 Ti9 Ti8 98.6(3) . . ?
O98 Ti9 O23 74.1(4) . . ?
O98 Ti9 O27 84.1(4) . . ?
O98 Ti9 O78 90.0(4) . . ?
O98 Ti9 O79 126.4(4) . . ?
O98 Ti9 O100 145.7(5) . . ?
O100 Ti9 Mo5 44.6(3) . . ?
O100 Ti9 Mo14 109.5(3) . . ?
O100 Ti9 Mo15 38.3(3) . . ?
O100 Ti9 Ti8 93.6(3) . . ?
O100 Ti9 O23 73.5(5) . . ?
O100 Ti9 O27 124.1(4) . . ?
O100 Ti9 O78 77.9(4) . . ?
O100 Ti9 O79 83.0(4) . . ?
Mo6 Ti10 Mo2 101.36(8) . . ?
Mo6 Ti10 Mo8 72.15(7) . . ?
Mo8 Ti10 Mo2 63.40(6) . . ?
Ti7 Ti10 Mo2 61.63(7) . . ?
Ti7 Ti10 Mo6 124.15(9) . . ?
Ti7 Ti10 Mo8 124.72(9) . . ?
O21 Ti10 Mo2 79.4(3) . . ?
O21 Ti10 Mo6 163.2(3) . . ?
O21 Ti10 Mo8 121.8(3) . . ?
O21 Ti10 Ti7 41.4(3) . . ?
O21 Ti10 O24 78.7(4) . . ?
O24 Ti10 Mo2 32.8(3) . . ?
O24 Ti10 Mo6 92.8(3) . . ?
O24 Ti10 Mo8 89.9(3) . . ?
O24 Ti10 Ti7 42.8(3) . . ?
O26 Ti10 Mo2 44.6(3) . . ?
O26 Ti10 Mo6 109.3(3) . . ?
O26 Ti10 Mo8 38.8(3) . . ?
O26 Ti10 Ti7 93.8(3) . . ?
O26 Ti10 O21 83.2(4) . . ?
O26 Ti10 O24 77.4(4) . . ?
O26 Ti10 O68 73.7(4) . . ?
O68 Ti10 Mo2 77.8(3) . . ?
O68 Ti10 Mo6 35.7(3) . . ?
O68 Ti10 Mo8 36.9(3) . . ?
O68 Ti10 Ti7 130.1(3) . . ?
O68 Ti10 O21 155.2(4) . . ?
O68 Ti10 O24 87.4(4) . . ?
O85 Ti10 Mo2 102.7(3) . . ?
O85 Ti10 Mo6 122.7(3) . . ?
O85 Ti10 Mo8 162.8(3) . . ?
O85 Ti10 Ti7 41.4(3) . . ?
O85 Ti10 O21 42.1(3) . . ?
O85 Ti10 O24 81.2(4) . . ?
O85 Ti10 O26 124.2(4) . . ?
O85 Ti10 O68 155.2(4) . . ?
O99 Ti10 Mo2 116.8(3) . . ?
O99 Ti10 Mo6 36.9(3) . . ?
O99 Ti10 Mo8 109.0(3) . . ?
O99 Ti10 Ti7 100.1(3) . . ?
O99 Ti10 O21 127.9(4) . . ?
O99 Ti10 O24 90.9(4) . . ?
O99 Ti10 O26 144.4(5) . . ?
O99 Ti10 O68 72.2(4) . . ?
O99 Ti10 O85 86.0(4) . . ?
O109 Ti10 Mo2 141.6(4) . . ?
O109 Ti10 Mo6 95.8(4) . . ?
O109 Ti10 Mo8 90.3(4) . . ?
O109 Ti10 Ti7 131.7(4) . . ?
O109 Ti10 O21 93.6(5) . . ?
O109 Ti10 O24 171.0(5) . . ?
O109 Ti10 O26 97.3(5) . . ?
O109 Ti10 O68 98.1(5) . . ?
O109 Ti10 O85 96.2(5) . . ?
O109 Ti10 O99 97.5(5) . . ?
Mo31 Ti11 Mo34 63.40(5) . . ?
Mo32 Ti11 Mo31 72.51(6) . . ?
Mo32 Ti11 Mo34 101.91(7) . . ?
Ti12 Ti11 Mo31 124.62(9) . . ?
Ti12 Ti11 Mo32 123.82(9) . . ?
Ti12 Ti11 Mo34 61.48(6) . . ?
O37 Ti11 Mo31 91.2(3) . . ?
O37 Ti11 Mo32 95.7(4) . . ?
O37 Ti11 Mo34 142.2(3) . . ?
O37 Ti11 Ti12 131.4(4) . . ?
O37 Ti11 O110 97.3(5) . . ?
O37 Ti11 O111 99.1(5) . . ?
O37 Ti11 O112 171.3(5) . . ?
O37 Ti11 O114 96.5(5) . . ?
O37 Ti11 O115 95.8(5) . . ?
O37 Ti11 O129 93.4(5) . . ?
O110 Ti11 Mo31 38.5(3) . . ?
O110 Ti11 Mo32 109.6(3) . . ?
O110 Ti11 Mo34 45.2(3) . . ?
O110 Ti11 Ti12 94.6(3) . . ?
O110 Ti11 O111 73.1(4) . . ?
O110 Ti11 O112 78.2(4) . . ?
O110 Ti11 O115 125.0(4) . . ?
O110 Ti11 O129 83.7(4) . . ?
O111 Ti11 Mo31 36.5(3) . . ?
O111 Ti11 Mo32 36.6(3) . . ?
O111 Ti11 Mo34 77.4(3) . . ?
O111 Ti11 Ti12 129.4(3) . . ?
O111 Ti11 O112 86.9(4) . . ?
O111 Ti11 O129 154.8(4) . . ?
O112 Ti11 Mo31 89.9(3) . . ?
O112 Ti11 Mo32 92.9(3) . . ?
O112 Ti11 Mo34 33.0(3) . . ?
O112 Ti11 Ti12 42.6(3) . . ?
O114 Ti11 Mo31 110.0(3) . . ?
O114 Ti11 Mo32 37.5(3) . . ?
O114 Ti11 Mo34 117.7(3) . . ?
O114 Ti11 Ti12 99.5(3) . . ?
O114 Ti11 O110 145.6(4) . . ?
O114 Ti11 O111 73.7(4) . . ?
O114 Ti11 O112 91.2(4) . . ?
O114 Ti11 O115 84.5(4) . . ?
O114 Ti11 O129 126.7(4) . . ?
O115 Ti11 Mo31 163.1(3) . . ?
O115 Ti11 Mo32 121.8(3) . . ?
O115 Ti11 Mo34 102.7(3) . . ?
O115 Ti11 Ti12 41.4(3) . . ?
O115 Ti11 O111 154.7(4) . . ?
O115 Ti11 O112 80.9(4) . . ?
O115 Ti11 O129 42.3(3) . . ?
O129 Ti11 Mo31 122.1(3) . . ?
O129 Ti11 Mo32 162.7(3) . . ?
O129 Ti11 Mo34 79.4(3) . . ?
O129 Ti11 Ti12 41.6(3) . . ?
O129 Ti11 O112 78.8(4) . . ?
Mo9 Ti12 Mo13 72.90(7) . . ?
Mo9 Ti12 Mo34 97.30(7) . . ?
Mo13 Ti12 Mo34 63.86(5) . . ?
Ti11 Ti12 Mo9 120.72(9) . . ?
Ti11 Ti12 Mo13 126.20(9) . . ?
Ti11 Ti12 Mo34 62.86(6) . . ?
O2 Ti12 Mo9 37.4(3) . . ?
O2 Ti12 Mo13 110.2(3) . . ?
O2 Ti12 Mo34 116.2(3) . . ?
O2 Ti12 Ti11 99.2(3) . . ?
O2 Ti12 O96 73.7(4) . . ?
O2 Ti12 O112 89.8(4) . . ?
O2 Ti12 O113 145.4(5) . . ?
O2 Ti12 O115 85.4(4) . . ?
O2 Ti12 O129 127.2(4) . . ?
O17 Ti12 Mo9 100.3(4) . . ?
O17 Ti12 Mo13 89.3(4) . . ?
O17 Ti12 Mo34 141.7(4) . . ?
O17 Ti12 Ti11 130.7(4) . . ?
O17 Ti12 O2 98.0(5) . . ?
O17 Ti12 O96 95.8(5) . . ?
O17 Ti12 O112 171.3(5) . . ?
O17 Ti12 O113 97.3(5) . . ?
O17 Ti12 O115 95.5(5) . . ?
O17 Ti12 O129 93.0(5) . . ?
O96 Ti12 Mo9 36.4(3) . . ?
O96 Ti12 Mo13 36.5(3) . . ?
O96 Ti12 Mo34 78.9(3) . . ?
O96 Ti12 Ti11 133.3(3) . . ?
O96 Ti12 O112 90.0(4) . . ?
O96 Ti12 O113 74.0(5) . . ?
O96 Ti12 O115 157.4(4) . . ?
O96 Ti12 O129 155.9(4) . . ?
O112 Ti12 Mo9 88.2(3) . . ?
O112 Ti12 Mo13 91.6(3) . . ?
O112 Ti12 Mo34 33.7(3) . . ?
O112 Ti12 Ti11 43.4(3) . . ?
O113 Ti12 Mo9 109.2(3) . . ?
O113 Ti12 Mo13 39.3(3) . . ?
O113 Ti12 Mo34 44.6(3) . . ?
O113 Ti12 Ti11 94.0(3) . . ?
O113 Ti12 O112 78.1(4) . . ?
O113 Ti12 O115 123.6(4) . . ?
O113 Ti12 O129 82.6(4) . . ?
O115 Ti12 Mo9 121.9(3) . . ?
O115 Ti12 Mo13 162.9(3) . . ?
O115 Ti12 Mo34 103.6(3) . . ?
O115 Ti12 Ti11 40.9(3) . . ?
O115 Ti12 O112 81.2(4) . . ?
O115 Ti12 O129 42.0(3) . . ?
O129 Ti12 Mo9 160.8(3) . . ?
O129 Ti12 Mo13 121.5(3) . . ?
O129 Ti12 Mo34 80.3(3) . . ?
O129 Ti12 Ti11 41.4(3) . . ?
O129 Ti12 O112 79.2(4) . . ?
O8 K1 Mo39 76.0(3) . . ?
O8 K1 O80 82.4(4) . . ?
O8 K1 O87 73.4(4) . . ?
O8 K1 O140 85.4(3) . . ?
O8 K1 O153 121.9(4) . . ?
O8 K1 O197 108.5(4) . . ?
O8 K1 Mo40 103.9(3) . . ?
O8 K1 Mo53 99.1(3) . . ?
O80 K1 Mo39 26.9(3) . . ?
O80 K1 O140 52.5(3) . . ?
O80 K1 Mo40 88.1(3) . . ?
O80 K1 Mo53 77.9(4) . . ?
O87 K1 Mo39 108.8(3) . . ?
O87 K1 O80 86.2(4) . . ?
O87 K1 O140 136.0(4) . . ?
O87 K1 Mo40 174.0(4) . . ?
O87 K1 Mo53 163.3(4) . . ?
O115 K1 Mo39 99.1(3) . . ?
O115 K1 O8 51.9(3) . . ?
O115 K1 O80 121.3(4) . . ?
O115 K1 O87 108.7(4) . . ?
O115 K1 O140 85.3(3) . . ?
O115 K1 O153 82.0(4) . . ?
O115 K1 O197 76.7(4) . . ?
O115 K1 Mo40 72.7(3) . . ?
O115 K1 Mo53 75.9(3) . . ?
O140 K1 Mo39 27.4(2) . . ?
O140 K1 Mo40 37.9(2) . . ?
O140 K1 Mo53 27.3(3) . . ?
O153 K1 Mo39 79.5(3) . . ?
O153 K1 O80 97.9(4) . . ?
O153 K1 O87 164.5(4) . . ?
O153 K1 O140 54.0(3) . . ?
O153 K1 Mo40 19.5(3) . . ?
O153 K1 Mo53 28.4(3) . . ?
O197 K1 Mo39 168.4(4) . . ?
O197 K1 O80 161.4(4) . . ?
O197 K1 O87 82.7(4) . . ?
O197 K1 O140 141.1(4) . . ?
O197 K1 O153 89.1(4) . . ?
O197 K1 Mo40 103.3(3) . . ?
O197 K1 Mo53 113.9(4) . . ?
O201 K1 Mo39 118.6(3) . . ?
O201 K1 O8 139.4(4) . . ?
O201 K1 O80 96.5(4) . . ?
O201 K1 O87 66.1(4) . . ?
O201 K1 O115 141.9(5) . . ?
O201 K1 O140 125.8(4) . . ?
O201 K1 O153 98.6(4) . . ?
O201 K1 O197 65.3(4) . . ?
O201 K1 Mo40 116.6(3) . . ?
O201 K1 Mo53 120.5(4) . . ?
O205 K1 Mo39 74.1(5) . . ?
O205 K1 O8 147.4(6) . . ?
O205 K1 O80 65.0(5) . . ?
O205 K1 O87 104.3(5) . . ?
O205 K1 O115 146.6(6) . . ?
O205 K1 O140 74.0(5) . . ?
O205 K1 O153 64.7(5) . . ?
O205 K1 O197 103.3(6) . . ?
O205 K1 O201 51.9(5) . . ?
O205 K1 Mo40 74.9(5) . . ?
O205 K1 Mo53 73.8(5) . . ?
Mo8 K2 Mo33 109.71(17) 2_646 . ?
K3 K2 Mo8 120.15(18) . 2_646 ?
K3 K2 Mo33 118.07(18) . . ?
O4 K2 Mo8 38.1(2) 2_646 2_646 ?
O4 K2 Mo33 113.0(3) 2_646 . ?
O4 K2 K3 128.8(3) 2_646 . ?
O4 K2 O5 73.4(3) 2_646 2_646 ?
O4 K2 O132 144.6(4) 2_646 . ?
O4 K2 O164 110.3(4) 2_646 . ?
O4 K2 O167 91.2(4) 2_646 2_646 ?
O4 K2 O170 59.9(4) 2_646 2_646 ?
O4 K2 O192 158.1(4) 2_646 . ?
O4 K2 O204 79.0(4) 2_646 . ?
O5 K2 Mo8 76.3(2) 2_646 2_646 ?
O5 K2 Mo33 173.4(3) 2_646 . ?
O5 K2 K3 55.5(3) 2_646 . ?
O5 K2 O132 97.8(4) 2_646 . ?
O49 K2 Mo8 114.8(3) . 2_646 ?
O49 K2 Mo33 38.0(2) . . ?
O49 K2 K3 125.0(3) . . ?
O49 K2 O4 93.7(4) . 2_646 ?
O49 K2 O5 142.6(4) . 2_646 ?
O49 K2 O132 72.5(3) . . ?
O49 K2 O164 59.8(4) . . ?
O49 K2 O167 160.4(4) . 2_646 ?
O49 K2 O170 112.9(4) . 2_646 ?
O49 K2 O192 90.5(4) . . ?
O49 K2 O204 76.8(4) . . ?
O132 K2 Mo8 172.7(3) . 2_646 ?
O132 K2 Mo33 76.0(2) . . ?
O132 K2 K3 52.6(3) . . ?
O164 K2 Mo8 93.1(3) . 2_646 ?
O164 K2 Mo33 23.5(2) . . ?
O164 K2 K3 117.7(3) . . ?
O164 K2 O5 157.7(4) . 2_646 ?
O164 K2 O132 91.0(3) . . ?
O164 K2 O192 54.3(4) . . ?
O167 K2 Mo8 60.4(3) 2_646 2_646 ?
O167 K2 Mo33 123.2(3) 2_646 . ?
O167 K2 K3 64.0(3) 2_646 . ?
O167 K2 O5 56.9(4) 2_646 2_646 ?
O167 K2 O132 112.9(4) 2_646 . ?
O167 K2 O164 100.8(4) 2_646 . ?
O167 K2 O192 78.2(4) 2_646 . ?
O167 K2 O204 122.8(5) 2_646 . ?
O170 K2 Mo8 23.7(3) 2_646 2_646 ?
O170 K2 Mo33 93.7(3) 2_646 . ?
O170 K2 K3 118.2(3) 2_646 . ?
O170 K2 O5 91.2(4) 2_646 2_646 ?
O170 K2 O132 155.4(4) 2_646 . ?
O170 K2 O164 73.3(4) 2_646 . ?
O170 K2 O167 54.3(4) 2_646 2_646 ?
O170 K2 O192 98.7(4) 2_646 . ?
O170 K2 O204 137.8(5) 2_646 . ?
O192 K2 Mo8 121.5(3) . 2_646 ?
O192 K2 Mo33 60.1(3) . . ?
O192 K2 K3 63.4(3) . . ?
O192 K2 O5 114.7(4) . 2_646 ?
O192 K2 O132 56.8(3) . . ?
O204 K2 Mo8 114.2(4) . 2_646 ?
O204 K2 Mo33 112.3(3) . . ?
O204 K2 K3 79.1(4) . . ?
O204 K2 O5 66.4(4) . 2_646 ?
O204 K2 O132 66.3(4) . . ?
O204 K2 O164 135.7(4) . . ?
O204 K2 O192 122.9(5) . . ?
K2 K3 Mo31 115.5(2) . . ?
O5 K3 Mo31 165.9(3) 2_646 . ?
O5 K3 K2 50.4(2) 2_646 . ?
O43 K3 Mo31 124.7(4) 2_646 . ?
O43 K3 K2 119.8(3) 2_646 . ?
O43 K3 O5 69.4(3) 2_646 2_646 ?
O43 K3 O132 143.9(4) 2_646 . ?
O43 K3 O162 121.1(5) 2_646 . ?
O43 K3 O166 86.3(4) 2_646 2_646 ?
O43 K3 O195 158.9(5) 2_646 . ?
O120 K3 Mo31 37.0(2) . . ?
O120 K3 K2 125.5(3) . . ?
O120 K3 O5 147.5(4) . 2_646 ?
O120 K3 O43 104.1(4) . 2_646 ?
O120 K3 O132 73.0(3) . . ?
O120 K3 O162 58.7(4) . . ?
O120 K3 O166 159.0(5) . 2_646 ?
O120 K3 O195 88.5(4) . . ?
O132 K3 Mo31 75.0(3) . . ?
O132 K3 K2 52.5(3) . . ?
O132 K3 O5 93.5(4) . 2_646 ?
O158 K3 Mo31 101.2(4) 2_646 . ?
O158 K3 K2 110.3(4) 2_646 . ?
O158 K3 O5 85.5(4) 2_646 2_646 ?
O158 K3 O43 59.3(4) 2_646 2_646 ?
O158 K3 O120 119.6(5) 2_646 . ?
O158 K3 O132 153.9(5) 2_646 . ?
O158 K3 O162 80.6(4) 2_646 . ?
O158 K3 O166 50.4(4) 2_646 2_646 ?
O158 K3 O195 99.8(4) 2_646 . ?
O162 K3 Mo31 23.3(2) . . ?
O162 K3 K2 113.4(4) . . ?
O162 K3 O5 152.6(4) . 2_646 ?
O162 K3 O132 88.9(4) . . ?
O162 K3 O166 100.3(4) . 2_646 ?
O162 K3 O195 51.7(4) . . ?
O166 K3 Mo31 122.3(4) 2_646 . ?
O166 K3 K2 59.9(3) 2_646 . ?
O166 K3 O5 53.2(3) 2_646 2_646 ?
O166 K3 O132 109.2(4) 2_646 . ?
O166 K3 O195 76.8(4) 2_646 . ?
O195 K3 Mo31 58.3(3) . . ?
O195 K3 K2 61.8(3) . . ?
O195 K3 O5 108.6(4) . 2_646 ?
O195 K3 O132 55.8(4) . . ?
O203 K3 Mo31 113.7(4) . . ?
O203 K3 K2 81.7(5) . . ?
O203 K3 O5 68.0(5) . 2_646 ?
O203 K3 O43 75.8(5) . 2_646 ?
O203 K3 O120 79.5(5) . . ?
O203 K3 O132 68.2(5) . . ?
O203 K3 O158 133.8(5) . 2_646 ?
O203 K3 O162 137.0(5) . . ?
O203 K3 O166 121.1(5) . 2_646 ?
O203 K3 O195 123.8(5) . . ?
Mo1 O1 Ti1 110.0(5) . . ?
Mo1 O1 Ti2 109.0(4) . . ?
Ti2 O1 Ti1 93.6(4) . . ?
Ti2 O2 Mo9 106.8(5) . . ?
Ti2 O2 Ti12 147.4(6) . . ?
Ti12 O2 Mo9 105.5(5) . . ?
Mo3 O3 Ti4 109.8(5) . . ?
Mo3 O3 Ti5 110.0(5) . . ?
Ti4 O3 Ti5 94.3(4) . . ?
Mo2 O4 K2 141.9(6) . 2_656 ?
Mo6 O5 K2 94.4(4) . 2_656 ?
Mo6 O5 K3 95.0(4) . 2_656 ?
K2 O5 K3 74.1(3) 2_656 2_656 ?
Ti4 O6 Mo18 105.8(5) . . ?
Ti4 O6 Ti7 148.2(6) . . ?
Ti7 O6 Mo18 105.7(5) . . ?
Mo7 O7 Ti2 106.6(5) . . ?
Mo9 O7 Mo7 146.2(6) . . ?
Mo9 O7 Ti2 107.1(5) . . ?
Ti1 O8 Ti2 98.8(4) . . ?
Ti1 O8 K1 124.0(5) . . ?
Ti2 O8 K1 136.9(5) . . ?
O16 O8 Ti1 70.2(5) . . ?
O16 O8 Ti2 69.5(5) . . ?
O16 O8 K1 116.8(6) . . ?
Mo26 O9 K6 132.4(7) . . ?
Mo24 O11 Ti6 105.4(5) . . ?
Ti8 O11 Mo24 107.1(5) . . ?
Ti8 O11 Ti6 147.2(6) . . ?
Ti1 O12 Mo39 155.7(6) . . ?
Ti1 O12 Mo45 170.3(7) . . ?
Ti1 O12 Mo55 160.2(7) . . ?
Ti1 O12 Mo56 161.0(7) . . ?
Ti3 O13 Ti6 98.8(4) . . ?
O30 O13 Ti3 70.6(6) . . ?
O30 O13 Ti6 69.7(6) . . ?
Ti9 O14 Mo41 160.6(7) . . ?
Ti9 O14 Mo46 159.4(8) . . ?
Ti9 O14 Mo47 170.3(7) . . ?
Ti9 O14 Mo49 154.7(7) . . ?
Ti4 O15 Ti5 96.1(4) . . ?
O45 O15 Ti4 68.0(6) . . ?
O45 O15 Ti5 67.5(6) . . ?
Ti1 O16 Ti2 97.1(4) . . ?
O8 O16 Ti1 67.4(5) . . ?
O8 O16 Ti2 68.4(5) . . ?
Ti12 O17 Mo29 154.2(7) . . ?
Ti12 O17 Mo50 155.4(7) . . ?
Mo1 O19 Mo10 112.4(5) . . ?
Mo1 O19 Mo16 112.3(5) . . ?
Mo16 O19 Mo10 91.7(4) . . ?
Mo22 O20 Mo3 98.9(4) . . ?
Mo27 O20 Mo3 101.0(5) . . ?
Mo27 O20 Mo22 97.2(4) . . ?
Ti4 O20 Mo3 97.4(4) . . ?
Ti4 O20 Mo22 150.6(6) . . ?
Ti4 O20 Mo27 103.5(5) . . ?
Ti7 O21 Ti10 96.6(4) . . ?
O85 O21 Ti7 68.9(6) . . ?
O85 O21 Ti10 67.9(6) . . ?
Mo12 O22 Ti3 105.7(5) . . ?
Mo14 O22 Mo12 146.7(6) . . ?
Mo14 O22 Ti3 105.5(5) . . ?
Mo14 O23 Mo15 147.2(6) . . ?
Mo14 O23 Ti9 105.8(5) . . ?
Mo15 O23 Ti9 105.6(5) . . ?
Mo2 O24 Ti7 109.5(5) . . ?
Mo2 O24 Ti10 110.6(5) . . ?
Ti7 O24 Ti10 94.0(4) . . ?
Mo7 O25 Mo1 102.7(4) . . ?
Mo7 O25 Mo16 97.3(4) . . ?
Mo16 O25 Mo1 99.5(4) . . ?
Ti2 O25 Mo1 97.5(4) . . ?
Ti2 O25 Mo7 102.6(5) . . ?
Ti2 O25 Mo16 150.3(6) . . ?
Mo8 O26 Mo2 101.9(5) . . ?
Mo8 O26 Mo35 97.9(4) . . ?
Mo35 O26 Mo2 99.5(4) . . ?
Ti10 O26 Mo2 97.5(4) . . ?
Ti10 O26 Mo8 103.1(5) . . ?
Ti10 O26 Mo35 149.6(6) . . ?
Ti9 O27 Ti8 98.2(4) . . ?
O79 O27 Ti8 70.3(6) . . ?
O79 O27 Ti9 69.6(6) . . ?
Mo20 O29 Mo19 115.9(6) . . ?
Ti3 O30 Ti6 96.7(4) . . ?
O13 O30 Ti3 67.1(6) . . ?
O13 O30 Ti6 68.3(6) . . ?
Ti8 O31 Mo29 150.9(7) . . ?
Ti8 O31 Mo50 150.2(7) . . ?
Ti5 O32 Mo42 160.0(7) . . ?
Ti5 O32 Mo44 175.2(7) . . ?
Ti5 O32 Mo51 151.0(7) . . ?
Ti5 O32 Mo57 153.1(9) . . ?
Mo41 O34 K4 134.8(7) . . ?
Mo47 O34 K4 161.7(7) . . ?
Mo49 O34 K4 136.2(7) . . ?
Mo43 O35 Mo18 146.5(6) . . ?
Mo43 O35 Ti7 107.3(5) . . ?
Mo18 O35 Ti7 106.1(5) . . ?
Mo24 O36 Ti6 106.2(5) . . ?
Mo26 O36 Mo24 147.1(7) . . ?
Mo26 O36 Ti6 106.7(6) . . ?
Ti11 O37 Mo17 160.5(7) . . ?
Ti11 O37 Mo40 157.8(7) . . ?
Ti11 O37 Mo53 156.4(7) . . ?
Ti11 O37 Mo54 170.3(8) . . ?
Ti4 O38 Mo39 148.7(7) . . ?
Ti4 O38 Mo45 173.7(7) . . ?
Ti4 O38 Mo55 162.2(7) . . ?
Ti4 O38 Mo56 151.0(7) . . ?
Mo33 O39 Mo10 111.5(5) . . ?
Mo11 O41 Mo3 101.4(5) . . ?
Mo11 O41 Mo23 97.0(4) . . ?
Mo23 O41 Mo3 99.0(4) . . ?
Ti5 O41 Mo3 97.8(4) . . ?
Ti5 O41 Mo11 103.2(5) . . ?
Ti5 O41 Mo23 150.5(6) . . ?
Mo5 O42 Mo15 107.3(5) . . ?
Mo3 O43 Mo11 107.1(5) . . ?
Mo3 O43 K3 142.8(6) . 2_656 ?
Mo11 O43 K3 99.4(4) . 2_656 ?
Mo12 O44 Mo4 100.1(4) . . ?
Mo12 O44 Mo19 96.7(4) . . ?
Mo19 O44 Mo4 97.8(4) . . ?
Ti3 O44 Mo4 97.9(5) . . ?
Ti3 O44 Mo12 104.5(5) . . ?
Ti3 O44 Mo19 150.8(6) . . ?
Ti5 O45 Ti4 98.3(4) . . ?
O15 O45 Ti4 69.9(6) . . ?
O15 O45 Ti5 70.5(6) . . ?
Mo5 O46 Mo21 112.1(5) . . ?
Mo5 O46 Mo25 112.4(5) . . ?
Mo21 O46 Mo25 90.8(4) . . ?
Mo8 O47 Mo35 112.2(6) . . ?
Mo3 O48 Mo27 106.2(5) . . ?
Mo1 O49 K2 142.2(6) . . ?
Mo20 O51 K8 125.8(6) . 1_455 ?
Mo2 O54 Mo43 105.8(5) . . ?
Mo4 O56 Mo12 106.4(5) . . ?
Mo42 O58 Mo41 146.5(8) . . ?
Mo44 O58 Mo46 177.8(7) . . ?
Mo49 O58 Mo57 163.2(12) . . ?
Mo15 O63 Mo25 110.0(5) . . ?
Mo27 O65 Mo22 111.5(6) . . ?
Mo21 O66 K7 126.2(6) . . ?
Mo25 O66 Mo21 116.8(6) . . ?
Mo25 O66 K7 115.9(6) . . ?
Ti3 O67 Mo42 160.5(7) . . ?
Ti3 O67 Mo44 171.0(7) . . ?
Ti3 O67 Mo51 157.3(7) . . ?
Ti3 O67 Mo57 159.7(9) . . ?
Mo6 O68 Mo8 146.3(6) . . ?
Mo6 O68 Ti10 106.2(5) . . ?
Mo8 O68 Ti10 105.5(5) . . ?
Mo14 O70 K4 174.5(7) . . ?
Mo14 O70 K4 94.4(5) . 3_676 ?
K4 O70 K4 80.5(4) . 3_676 ?
Mo4 O71 Mo19 111.7(5) . . ?
Mo4 O71 Mo20 111.7(5) . . ?
Mo20 O71 Mo19 90.5(4) . . ?
Mo4 O73 Ti3 110.2(5) . . ?
Mo4 O73 Ti6 109.1(5) . . ?
Ti6 O73 Ti3 94.5(4) . . ?
Mo20 O74 K6 146.7(7) . . ?
Mo28 O75 Mo21 110.7(6) . . ?
Mo19 O76 K8 125.0(6) . 1_455 ?
Mo11 O77 Mo23 110.4(5) . . ?
Mo5 O78 Ti8 108.9(5) . . ?
Mo5 O78 Ti9 110.0(5) . . ?
Ti8 O78 Ti9 94.5(4) . . ?
Ti8 O79 K7 138.2(6) . . ?
Ti9 O79 Ti8 96.3(4) . . ?
Ti9 O79 K7 125.2(6) . . ?
O27 O79 Ti8 67.7(6) . . ?
O27 O79 Ti9 68.0(6) . . ?
O27 O79 K7 127.8(7) . . ?
Mo39 O80 K1 101.9(6) . . ?
Mo45 O80 K1 120.6(5) . . ?
Mo55 O80 K1 104.7(5) . . ?
Mo56 O80 K1 124.8(7) . . ?
Mo42 O81 K4 127.3(7) . . ?
Mo44 O81 K4 155.1(7) . . ?
Mo57 O81 K4 132.7(9) . . ?
O191 O83 Mo7 68.9(10) . . ?
Mo18 O84 Mo27 147.5(7) . . ?
Mo18 O84 Ti4 106.8(5) . . ?
Mo27 O84 Ti4 105.6(5) . . ?
Ti10 O85 Ti7 97.5(4) . . ?
O21 O85 Ti7 68.9(6) . . ?
O21 O85 Ti10 70.0(6) . . ?
Mo19 O86 K5 141.0(7) . . ?
Mo30 O87 K1 137.6(6) . . ?
Mo48 O87 K1 114.9(6) . . ?
Mo52 O87 K1 133.4(6) . . ?
Mo20 O88 Mo4 99.4(4) . . ?
Mo26 O88 Mo4 102.4(4) . . ?
Mo26 O88 Mo20 96.7(4) . . ?
Ti6 O88 Mo4 97.4(5) . . ?
Ti6 O88 Mo20 150.7(6) . . ?
Ti6 O88 Mo26 103.0(5) . . ?
Mo26 O89 Mo20 111.2(6) . . ?
Ti6 O90 Mo30 153.2(7) . . ?
Ti6 O90 Mo48 152.8(7) . . ?
Ti6 O90 Mo52 173.3(8) . . ?
Ti7 O91 Mo17 163.3(7) . . ?
Ti7 O91 Mo40 149.1(7) . . ?
Ti7 O91 Mo53 150.2(8) . . ?
Ti7 O91 Mo54 172.9(8) . . ?
Mo9 O96 Mo13 146.5(6) . . ?
Mo9 O96 Ti12 106.6(5) . . ?
Mo13 O96 Ti12 106.9(5) . . ?
Mo6 O97 Mo11 145.0(6) . . ?
Mo6 O97 Ti5 105.5(5) . . ?
Mo11 O97 Ti5 107.4(5) . . ?
Ti3 O98 Mo14 105.0(5) . . ?
Ti9 O98 Mo14 105.0(5) . . ?
Ti9 O98 Ti3 149.7(6) . . ?
Mo6 O99 Ti5 105.8(5) . . ?
Ti10 O99 Mo6 106.6(5) . . ?
Ti10 O99 Ti5 147.3(6) . . ?
Mo15 O100 Mo5 100.3(4) . . ?
Mo15 O100 Mo25 97.2(4) . . ?
Mo25 O100 Mo5 97.9(4) . . ?
Ti9 O100 Mo5 98.3(4) . . ?
Ti9 O100 Mo15 104.4(5) . . ?
Ti9 O100 Mo25 150.0(6) . . ?
Mo24 O101 Mo28 147.5(7) . . ?
Mo24 O101 Ti8 105.8(5) . . ?
Mo28 O101 Ti8 106.7(6) . . ?
Mo10 O102 Mo1 99.4(4) . . ?
Mo33 O102 Mo1 101.8(4) . . ?
Mo33 O102 Mo10 97.2(4) . . ?
Ti1 O102 Mo1 98.4(4) . . ?
Ti1 O102 Mo10 149.3(5) . . ?
Ti1 O102 Mo33 103.4(5) . . ?
Mo29 O103 Mo30 161.9(7) . . ?
Mo48 O103 Mo50 161.3(9) . . ?
Mo21 O104 Mo5 99.2(4) . . ?
Mo28 O104 Mo5 102.4(4) . . ?
Mo28 O104 Mo21 97.4(5) . . ?
Ti8 O104 Mo5 97.3(5) . . ?
Ti8 O104 Mo21 149.7(6) . . ?
Ti8 O104 Mo28 103.6(5) . . ?
Mo23 O105 Mo22 115.8(6) . . ?
Mo6 O107 K4 176.6(7) . . ?
Ti2 O108 Mo30 151.6(7) . . ?
Ti2 O108 Mo48 152.0(7) . . ?
Ti2 O108 Mo52 172.9(8) . . ?
Ti10 O109 Mo41 161.1(7) . . ?
Ti10 O109 Mo46 149.1(8) . . ?
Ti10 O109 Mo47 172.5(7) . . ?
Ti10 O109 Mo49 146.0(8) . . ?
Mo31 O110 Mo34 101.1(4) . . ?
Mo31 O110 Mo38 97.4(4) . . ?
Mo38 O110 Mo34 98.5(4) . . ?
Ti11 O110 Mo31 104.1(5) . . ?
Ti11 O110 Mo34 97.3(4) . . ?
Ti11 O110 Mo38 150.2(5) . . ?
Mo31 O111 Ti11 106.3(5) . . ?
Mo32 O111 Mo31 145.7(6) . . ?
Mo32 O111 Ti11 105.4(5) . . ?
Mo34 O112 Ti11 110.2(5) . . ?
Mo34 O112 Ti12 109.3(5) . . ?
Ti12 O112 Ti11 94.0(4) . . ?
Mo13 O113 Mo34 102.0(4) . . ?
Mo13 O113 Mo37 97.4(4) . . ?
Mo37 O113 Mo34 99.1(4) . . ?
Ti12 O113 Mo13 103.3(5) . . ?
Ti12 O113 Mo34 97.8(4) . . ?
Ti12 O113 Mo37 149.9(6) . . ?
Ti1 O114 Mo32 105.7(5) . . ?
Ti11 O114 Mo32 105.6(5) . . ?
Ti11 O114 Ti1 148.4(6) . . ?
Ti11 O115 Ti12 97.7(4) . . ?
Ti11 O115 K1 125.3(5) . . ?
Ti12 O115 K1 136.4(5) . . ?
O129 O115 Ti11 69.4(6) . . ?
O129 O115 Ti12 69.2(6) . . ?
O129 O115 K1 116.1(7) . . ?
Mo43 O116 Mo36 110.9(5) . . ?
Mo43 O118 Mo2 101.8(5) . . ?
Mo43 O118 Mo36 96.4(4) . . ?
Mo36 O118 Mo2 99.1(4) . . ?
Ti7 O118 Mo2 97.9(4) . . ?
Ti7 O118 Mo43 103.2(5) . . ?
Ti7 O118 Mo36 150.8(6) . . ?
Mo32 O119 Mo33 146.6(6) . . ?
Mo32 O119 Ti1 106.5(5) . . ?
Mo33 O119 Ti1 105.1(5) . . ?
Mo31 O120 K3 99.2(4) . . ?
Mo34 O120 Mo31 106.7(5) . . ?
Mo34 O120 K3 140.5(6) . . ?
Mo31 O123 Mo38 110.7(5) . . ?
Mo3 O124 Mo22 112.6(5) . . ?
Mo3 O124 Mo23 111.1(5) . . ?
Mo22 O124 Mo23 92.2(4) . . ?
Mo38 O125 K6 154.7(7) . 1_655 ?
Mo12 O126 Mo19 110.5(5) . . ?
Mo23 O127 K5 149.4(7) . . ?
Mo34 O128 Mo13 107.2(5) . . ?
Ti11 O129 Ti12 97.0(4) . . ?
O115 O129 Ti11 68.3(5) . . ?
O115 O129 Ti12 68.8(6) . . ?
Mo7 O130 Mo16 110.8(6) . . ?
Mo42 O131 K5 144.5(6) . . ?
Mo44 O131 K5 143.8(8) . . ?
Mo51 O131 K5 174.4(8) . . ?
Mo57 O131 K5 159.4(8) . . ?
Mo32 O132 K2 93.2(4) . . ?
Mo32 O132 K3 94.9(4) . . ?
K2 O132 K3 74.9(3) . . ?
Mo36 O133 K8 125.3(7) . . ?
Mo36 O134 K5 152.1(7) . 1_655 ?
Mo13 O135 Mo37 111.7(5) . . ?
Mo34 O137 Mo37 111.1(5) . . ?
Mo34 O137 Mo38 112.3(5) . . ?
Mo37 O137 Mo38 91.4(4) . . ?
Mo37 O138 K6 151.0(7) . 1_655 ?
Mo39 O140 K1 81.8(5) . . ?
Mo17 O140 Mo39 169.6(9) . . ?
Mo17 O140 K1 108.3(6) . . ?
Mo40 O140 K1 82.2(4) . . ?
Mo45 O140 K1 104.2(5) . . ?
Mo45 O140 Mo40 173.5(6) . . ?
Mo53 O140 K1 83.0(6) . . ?
Mo54 O140 K1 103.0(5) . . ?
Mo55 O140 K1 106.3(6) . . ?
Mo55 O140 Mo53 170.4(10) . . ?
Mo56 O140 K1 84.6(4) . . ?
Mo56 O140 Mo54 172.0(7) . . ?
O184 O142 Mo13 69.5(10) . . ?
Mo35 O143 Mo36 117.7(6) . . ?
Mo30 O144 K6 133.7(7) . . ?
Mo48 O144 K6 128.7(6) . . ?
Mo52 O144 K6 108.1(7) . . ?
Mo10 O146 Mo16 117.4(5) . . ?
Mo2 O147 Mo35 111.2(5) . . ?
Mo2 O147 Mo36 111.7(5) . . ?
Mo36 O147 Mo35 90.6(4) . . ?
Mo38 O151 K8 126.0(7) . . ?
Mo40 O153 K1 123.0(6) . . ?
Mo53 O153 K1 101.1(6) . . ?
Mo54 O153 K1 119.3(6) . . ?
Mo38 O154 Mo37 115.7(6) . . ?
Mo35 O156 K5 152.7(7) . 1_655 ?
Mo11 O158 K3 119.6(6) . 2_656 ?
O181 O158 Mo11 68.0(10) . . ?
O181 O158 K3 110.2(11) . 2_656 ?
O173 O159 Mo18 70.5(9) . . ?
O163 O160 Mo9 70.4(8) . . ?
O193 O161 Mo26 72.6(10) . . ?
Mo31 O162 K3 118.0(6) . . ?
O188 O162 Mo31 69.5(9) . . ?
O188 O162 K3 112.3(10) . . ?
O160 O163 Mo9 71.5(8) . . ?
Mo33 O164 K2 117.1(5) . . ?
O185 O164 Mo33 74.8(9) . . ?
O185 O164 K2 113.8(10) . . ?
Mo17 O165 K8 149.4(6) . . ?
Mo40 O165 K8 120.6(7) . . ?
Mo53 O165 K8 130.4(7) . . ?
Mo54 O165 K8 153.7(9) . . ?
Mo6 O166 K3 124.6(6) . 2_656 ?
O167 O166 Mo6 70.4(9) . . ?
O167 O166 K3 120.4(10) . 2_656 ?
Mo6 O167 K2 120.4(6) . 2_656 ?
O166 O167 Mo6 72.7(9) . . ?
O166 O167 K2 115.6(10) . 2_656 ?
O189 O168 Mo43 72.7(10) . . ?
Mo8 O170 K2 118.8(6) . 2_656 ?
O190 O170 Mo8 70.0(10) . . ?
O190 O170 K2 115.3(11) . 2_656 ?
O187 O171 Mo28 72.9(11) . . ?
O174 O172 Mo24 70.5(9) . . ?
O159 O173 Mo18 71.6(9) . . ?
O172 O174 Mo24 71.5(9) . . ?
Mo41 O176 K7 123.4(5) . . ?
Mo46 O176 K7 105.4(8) . . ?
Mo47 O176 K7 108.2(5) . . ?
Mo49 O176 K7 127.8(7) . . ?
O178 O177 Mo15 73.3(9) . . ?
O177 O178 Mo15 69.5(9) . . ?
O180 O179 Mo12 72.5(9) . . ?
O179 O180 Mo12 70.3(9) . . ?
O158 O181 Mo11 75.4(10) . . ?
Mo14 O182 K4 109.6(6) . 3_676 ?
O183 O182 Mo14 70.2(9) . . ?
O183 O182 K4 82.1(10) . 3_676 ?
Mo14 O183 K4 106.6(6) . 3_676 ?
O182 O183 Mo14 72.0(9) . . ?
O182 O183 K4 73.3(10) . 3_676 ?
O142 O184 Mo13 73.8(10) . . ?
O164 O185 Mo33 68.2(9) . . ?
O194 O186 Mo27 70.0(10) . . ?
O171 O187 Mo28 70.1(10) . . ?
O162 O188 Mo31 73.1(9) . . ?
O168 O189 Mo43 70.4(10) . . ?
O170 O190 Mo8 72.8(10) . . ?
O83 O191 Mo7 74.3(10) . . ?
Mo32 O192 K2 118.5(6) . . ?
O195 O192 Mo32 70.9(8) . . ?
O195 O192 K2 117.0(10) . . ?
O161 O193 Mo26 71.0(10) . . ?
O186 O194 Mo27 73.4(10) . . ?
Mo32 O195 K3 119.1(6) . . ?
O192 O195 Mo32 71.3(8) . . ?
O192 O195 K3 117.8(10) . . ?
Mo29 O197 K1 120.7(6) . . ?
Mo29 O197 K7 123.3(6) . . ?
K1 O197 K7 115.6(5) . . ?
Mo50 O197 K1 138.9(7) . . ?
Mo50 O197 K7 100.8(7) . . ?
Mo16 O198 K6 158.4(7) . . ?
O37 Mo40 K1 74.7(3) . . ?
O37 Mo40 O91 143.0(5) . . ?
O37 Mo40 O140 77.0(4) . . ?
O37 Mo40 O202 73.3(4) . . ?
O91 Mo40 K1 113.1(4) . . ?
O91 Mo40 O140 77.0(4) . . ?
O91 Mo40 O202 73.4(5) . . ?
O140 Mo40 K1 59.8(3) . . ?
O140 Mo40 O202 70.6(4) . . ?
O153 Mo40 K1 37.5(5) . . ?
O153 Mo40 O37 102.9(6) . . ?
O153 Mo40 O91 102.9(6) . . ?
O153 Mo40 O140 89.9(6) . . ?
O153 Mo40 O165 120.7(7) . . ?
O153 Mo40 O202 160.5(6) . . ?
O165 Mo40 K1 147.9(5) . . ?
O165 Mo40 O37 96.4(6) . . ?
O165 Mo40 O91 92.7(6) . . ?
O165 Mo40 O140 149.4(6) . . ?
O165 Mo40 O202 78.8(6) . . ?
O202 Mo40 K1 125.4(3) . . ?
O32 Mo44 O58 78.4(5) . . ?
O32 Mo44 O67 147.9(6) . . ?
O32 Mo44 O200 75.9(5) . . ?
O58 Mo44 O200 75.4(4) . . ?
O67 Mo44 O58 77.8(5) . . ?
O67 Mo44 O200 77.5(5) . . ?
O81 Mo44 O32 98.7(6) . . ?
O81 Mo44 O58 83.3(6) . . ?
O81 Mo44 O67 99.6(6) . . ?
O81 Mo44 O200 158.7(6) . . ?
O131 Mo44 O32 98.6(6) . . ?
O131 Mo44 O58 167.8(6) . . ?
O131 Mo44 O67 100.1(6) . . ?
O131 Mo44 O81 108.9(7) . . ?
O131 Mo44 O200 92.4(6) . . ?
O12 Mo45 O80 74.6(5) . . ?
O12 Mo45 O140 76.8(5) . . ?
O38 Mo45 O12 145.7(7) . . ?
O38 Mo45 O80 75.4(5) . . ?
O38 Mo45 O140 77.9(5) . . ?
O82 Mo45 O12 96.8(7) . . ?
O82 Mo45 O38 98.8(7) . . ?
O82 Mo45 O80 88.8(7) . . ?
O82 Mo45 O140 159.3(8) . . ?
O140 Mo45 O80 70.6(5) . . ?
O157 Mo45 O12 99.4(7) . . ?
O157 Mo45 O38 100.3(7) . . ?
O157 Mo45 O80 154.2(8) . . ?
O157 Mo45 O82 117.0(9) . . ?
O157 Mo45 O140 83.6(7) . . ?
O14 Mo46 O58 77.9(6) . . ?
O14 Mo46 O109 142.9(8) . . ?
O14 Mo46 K7 81.4(5) . . ?
O58 Mo46 K7 130.6(6) . . ?
O109 Mo46 O58 76.1(6) . . ?
O109 Mo46 K7 135.8(6) . . ?
O136 Mo46 O14 93.6(7) . . ?
O136 Mo46 O58 140.8(9) . . ?
O136 Mo46 O109 90.1(7) . . ?
O136 Mo46 K7 84.4(6) . . ?
O176 Mo46 O14 105.8(8) . . ?
O176 Mo46 O58 92.1(8) . . ?
O176 Mo46 O109 101.2(8) . . ?
O176 Mo46 O136 126.8(10) . . ?
O176 Mo46 K7 51.9(6) . . ?
O14 Mo47 O58 76.8(5) . . ?
O14 Mo47 O176 78.0(5) . . ?
O34 Mo47 O14 97.4(6) . . ?
O34 Mo47 O58 78.7(5) . . ?
O34 Mo47 O109 95.1(6) . . ?
O34 Mo47 O176 152.4(6) . . ?
O109 Mo47 O14 147.4(6) . . ?
O109 Mo47 O58 76.3(5) . . ?
O109 Mo47 O176 77.0(5) . . ?
O136 Mo47 O14 102.1(6) . . ?
O136 Mo47 O34 112.2(7) . . ?
O136 Mo47 O58 169.0(7) . . ?
O136 Mo47 O109 100.8(6) . . ?
O136 Mo47 O176 95.3(6) . . ?
O176 Mo47 O58 73.7(4) . . ?
O87 Mo48 K1 40.2(4) . . ?
O87 Mo48 O90 94.7(6) . . ?
O87 Mo48 O108 93.7(6) . . ?
O87 Mo48 O144 74.3(6) . . ?
O87 Mo48 O175 147.4(7) . . ?
O90 Mo48 K1 121.2(5) . . ?
O90 Mo48 O108 145.9(7) . . ?
O90 Mo48 O144 76.0(5) . . ?
O90 Mo48 O175 78.0(6) . . ?
O103 Mo48 K1 76.0(6) . . ?
O103 Mo48 O87 112.5(8) . . ?
O103 Mo48 O90 105.1(7) . . ?
O103 Mo48 O108 102.0(7) . . ?
O103 Mo48 O144 172.8(8) . . ?
O103 Mo48 O175 100.0(8) . . ?
O108 Mo48 K1 85.1(4) . . ?
O108 Mo48 O144 74.6(5) . . ?
O108 Mo48 O175 77.2(5) . . ?
O144 Mo48 K1 109.7(4) . . ?
O175 Mo48 K1 160.8(4) . . ?
O175 Mo48 O144 73.1(5) . . ?
O14 Mo49 O34 77.7(6) . . ?
O14 Mo49 O136 73.5(6) . . ?
O34 Mo49 O136 67.5(5) . . ?
O58 Mo49 O14 101.5(7) . . ?
O58 Mo49 O34 82.3(8) . . ?
O58 Mo49 O109 100.4(8) . . ?
O58 Mo49 O136 149.8(9) . . ?
O58 Mo49 O176 123.5(9) . . ?
O109 Mo49 O14 142.4(8) . . ?
O109 Mo49 O34 75.5(6) . . ?
O109 Mo49 O136 72.2(6) . . ?
O176 Mo49 O14 97.3(8) . . ?
O176 Mo49 O34 154.1(9) . . ?
O176 Mo49 O109 95.6(8) . . ?
O176 Mo49 O136 86.7(8) . . ?
O17 Mo50 O31 146.8(7) . . ?
O17 Mo50 O103 79.0(5) . . ?
O17 Mo50 O169 76.2(5) . . ?
O17 Mo50 K7 124.9(5) . . ?
O31 Mo50 O103 77.6(5) . . ?
O31 Mo50 O169 74.5(5) . . ?
O31 Mo50 K7 88.3(5) . . ?
O72 Mo50 O17 97.8(7) . . ?
O72 Mo50 O31 97.8(7) . . ?
O72 Mo50 O103 163.2(8) . . ?
O72 Mo50 O169 90.6(7) . . ?
O72 Mo50 O197 115.7(8) . . ?
O72 Mo50 K7 65.4(6) . . ?
O103 Mo50 O169 72.7(5) . . ?
O103 Mo50 K7 129.8(5) . . ?
O169 Mo50 K7 148.5(5) . . ?
O197 Mo50 O17 100.4(6) . . ?
O197 Mo50 O31 98.9(6) . . ?
O197 Mo50 O103 81.0(6) . . ?
O197 Mo50 O169 153.7(7) . . ?
O197 Mo50 K7 53.6(5) . . ?
O67 Mo51 O32 141.5(7) . . ?
O131 Mo51 O32 91.8(6) . . ?
O131 Mo51 O67 97.0(6) . . ?
O200 Mo51 O32 98.2(6) . . ?
O200 Mo51 O67 104.6(7) . . ?
O200 Mo51 O131 129.2(8) . . ?
O87 Mo52 K6 121.9(6) . . ?
O90 Mo52 O87 77.4(6) . . ?
O90 Mo52 O103 79.2(6) . . ?
O90 Mo52 O108 150.7(9) . . ?
O90 Mo52 K6 101.0(5) . . ?
O103 Mo52 O87 71.5(5) . . ?
O103 Mo52 K6 166.4(6) . . ?
O108 Mo52 O87 77.7(6) . . ?
O108 Mo52 O103 78.4(6) . . ?
O108 Mo52 K6 105.1(6) . . ?
O144 Mo52 O87 75.8(7) . . ?
O144 Mo52 O90 94.9(8) . . ?
O144 Mo52 O103 147.3(9) . . ?
O144 Mo52 O108 93.8(7) . . ?
O144 Mo52 K6 46.2(5) . . ?
O175 Mo52 O87 169.9(9) . . ?
O175 Mo52 O90 101.0(8) . . ?
O175 Mo52 O103 98.4(9) . . ?
O175 Mo52 O108 100.7(9) . . ?
O175 Mo52 O144 114.3(9) . . ?
O175 Mo52 K6 68.2(7) . . ?
O37 Mo53 K1 83.2(5) . . ?
O37 Mo53 O165 77.0(6) . . ?
O37 Mo53 O202 77.3(6) . . ?
O91 Mo53 K1 127.8(6) . . ?
O91 Mo53 O37 147.5(8) . . ?
O91 Mo53 O165 75.1(6) . . ?
O91 Mo53 O202 78.0(6) . . ?
O140 Mo53 K1 69.8(5) . . ?
O140 Mo53 O37 99.6(7) . . ?
O140 Mo53 O91 100.7(7) . . ?
O140 Mo53 O153 115.2(8) . . ?
O140 Mo53 O165 159.7(9) . . ?
O140 Mo53 O202 88.8(8) . . ?
O153 Mo53 K1 50.5(5) . . ?
O153 Mo53 O37 96.3(7) . . ?
O153 Mo53 O91 97.7(8) . . ?
O153 Mo53 O165 85.1(7) . . ?
O153 Mo53 O202 156.0(8) . . ?
O165 Mo53 K1 128.7(6) . . ?
O202 Mo53 K1 148.1(5) . . ?
O202 Mo53 O165 70.9(6) . . ?
O37 Mo54 O91 145.9(9) . . ?
O37 Mo54 O140 77.4(6) . . ?
O37 Mo54 O153 75.1(6) . . ?
O91 Mo54 O140 77.4(6) . . ?
O91 Mo54 O153 75.4(6) . . ?
O140 Mo54 O153 71.6(5) . . ?
O165 Mo54 O37 98.4(8) . . ?
O165 Mo54 O91 94.6(8) . . ?
O165 Mo54 O140 154.4(10) . . ?
O165 Mo54 O153 82.9(8) . . ?
O202 Mo54 O37 101.0(9) . . ?
O202 Mo54 O91 100.8(8) . . ?
O202 Mo54 O140 88.5(8) . . ?
O202 Mo54 O153 160.1(9) . . ?
O202 Mo54 O165 117.0(10) . . ?
O12 Mo55 O80 76.6(5) . . ?
O12 Mo55 O82 75.7(5) . . ?
O38 Mo55 O12 145.1(6) . . ?
O38 Mo55 O80 76.8(5) . . ?
O38 Mo55 O82 76.0(5) . . ?
O80 Mo55 O82 75.3(5) . . ?
O140 Mo55 O12 99.9(6) . . ?
O140 Mo55 O38 100.6(6) . . ?
O140 Mo55 O80 86.5(6) . . ?
O140 Mo55 O82 161.8(7) . . ?
O140 Mo55 O157 113.7(8) . . ?
O157 Mo55 O12 98.9(6) . . ?
O157 Mo55 O38 98.3(7) . . ?
O157 Mo55 O80 159.8(7) . . ?
O157 Mo55 O82 84.5(7) . . ?
O12 Mo56 K1 72.3(4) . . ?
O12 Mo56 O38 145.7(7) . . ?
O12 Mo56 O140 76.7(5) . . ?
O12 Mo56 O157 75.2(5) . . ?
O38 Mo56 K1 111.0(5) . . ?
O38 Mo56 O140 77.0(5) . . ?
O38 Mo56 O157 74.7(5) . . ?
O80 Mo56 K1 35.8(5) . . ?
O80 Mo56 O12 99.9(7) . . ?
O80 Mo56 O38 100.0(7) . . ?
O80 Mo56 O82 124.7(8) . . ?
O80 Mo56 O140 86.2(7) . . ?
O80 Mo56 O157 154.2(7) . . ?
O82 Mo56 K1 148.1(6) . . ?
O82 Mo56 O12 95.5(7) . . ?
O82 Mo56 O38 95.8(7) . . ?
O82 Mo56 O140 149.0(8) . . ?
O82 Mo56 O157 81.0(7) . . ?
O140 Mo56 K1 58.3(4) . . ?
O140 Mo56 O157 68.0(5) . . ?
O157 Mo56 K1 121.8(4) . . ?
O32 Mo57 O81 81.2(8) . . ?
O32 Mo57 O131 75.3(9) . . ?
O58 Mo57 O32 100.7(12) . . ?
O58 Mo57 O67 102.1(12) . . ?
O58 Mo57 O81 89.2(12) . . ?
O58 Mo57 O131 159.7(13) . . ?
O58 Mo57 O200 113.0(12) . . ?
O67 Mo57 O32 152.3(14) . . ?
O67 Mo57 O81 83.6(9) . . ?
O67 Mo57 O131 77.9(9) . . ?
O67 Mo57 O200 94.6(11) . . ?
O81 Mo57 O131 70.6(7) . . ?
O200 Mo57 O32 90.7(11) . . ?
O200 Mo57 O81 157.5(15) . . ?
O200 Mo57 O131 87.1(11) . . ?
Mo14 K4 Mo41 151.9(3) 3_676 . ?
Mo14 K4 K4 75.1(3) 3_676 3_676 ?
O34 K4 Mo14 136.5(5) . 3_676 ?
O34 K4 Mo41 16.9(3) . . ?
O34 K4 O70 130.8(5) . 3_676 ?
O34 K4 O70 66.9(4) . . ?
O34 K4 O81 81.8(4) . . ?
O34 K4 O107 77.9(4) . . ?
O34 K4 O182 138.9(6) . 3_676 ?
O34 K4 O183 117.5(5) . 3_676 ?
O34 K4 K4 103.5(5) . 3_676 ?
O34 K4 O207 74.2(5) . 3_676 ?
O34 K4 O207 129.1(5) . . ?
O70 K4 Mo14 127.4(4) . 3_676 ?
O70 K4 Mo14 28.0(2) 3_676 3_676 ?
O70 K4 Mo41 64.8(3) . . ?
O70 K4 Mo41 146.6(4) 3_676 . ?
O70 K4 O70 99.5(4) . 3_676 ?
O70 K4 K4 47.1(3) 3_676 3_676 ?
O70 K4 K4 52.3(3) . 3_676 ?
O81 K4 Mo14 141.1(5) . 3_676 ?
O81 K4 Mo41 65.3(3) . . ?
O81 K4 O70 137.8(5) . 3_676 ?
O81 K4 O70 66.1(4) . . ?
O81 K4 K4 107.1(5) . 3_676 ?
O81 K4 O207 131.8(5) . 3_676 ?
O107 K4 Mo14 103.3(3) . 3_676 ?
O107 K4 Mo41 70.8(3) . . ?
O107 K4 O70 129.3(5) . . ?
O107 K4 O70 131.3(4) . 3_676 ?
O107 K4 O81 73.9(4) . . ?
O107 K4 K4 178.4(5) . 3_676 ?
O107 K4 O207 137.0(6) . 3_676 ?
O182 K4 Mo14 27.3(3) 3_676 3_676 ?
O182 K4 Mo41 144.4(4) 3_676 . ?
O182 K4 O70 150.5(5) 3_676 . ?
O182 K4 O70 54.2(4) 3_676 3_676 ?
O182 K4 O81 122.3(6) 3_676 . ?
O182 K4 O107 78.2(4) 3_676 . ?
O182 K4 O183 24.6(2) 3_676 3_676 ?
O182 K4 K4 100.2(4) 3_676 3_676 ?
O182 K4 O207 102.7(5) 3_676 3_676 ?
O183 K4 Mo14 27.6(3) 3_676 3_676 ?
O183 K4 Mo41 128.5(4) 3_676 . ?
O183 K4 O70 149.0(5) 3_676 . ?
O183 K4 O70 53.1(4) 3_676 3_676 ?
O183 K4 O81 143.0(5) 3_676 . ?
O183 K4 O107 79.6(4) 3_676 . ?
O183 K4 K4 99.0(4) 3_676 3_676 ?
O183 K4 O207 85.0(5) 3_676 3_676 ?
K4 K4 Mo41 110.7(3) 3_676 . ?
O207 K4 Mo14 82.2(4) . 3_676 ?
O207 K4 Mo14 77.0(3) 3_676 3_676 ?
O207 K4 Mo41 88.9(4) 3_676 . ?
O207 K4 Mo41 122.5(4) . . ?
O207 K4 O70 64.9(4) . 3_676 ?
O207 K4 O70 66.2(4) 3_676 . ?
O207 K4 O70 57.7(4) 3_676 3_676 ?
O207 K4 O70 62.6(4) . . ?
O207 K4 O81 73.5(5) . . ?
O207 K4 O107 132.8(6) . . ?
O207 K4 O182 91.4(5) . 3_676 ?
O207 K4 O183 108.6(5) . 3_676 ?
O207 K4 K4 43.2(4) 3_676 3_676 ?
O207 K4 K4 47.0(4) . 3_676 ?
O207 K4 O207 90.2(5) . 3_676 ?
O9 K6 Mo52 62.6(3) . . ?
O74 K6 O9 64.4(4) . . ?
O74 K6 O125 74.8(4) . 1_455 ?
O74 K6 O138 88.3(4) . 1_455 ?
O74 K6 O144 59.7(4) . . ?
O74 K6 O198 100.3(5) . . ?
O74 K6 Mo52 73.6(4) . . ?
O125 K6 O9 134.2(5) 1_455 . ?
O125 K6 O138 61.6(4) 1_455 1_455 ?
O125 K6 O144 99.4(5) 1_455 . ?
O125 K6 Mo52 125.1(4) 1_455 . ?
O138 K6 O9 96.1(4) 1_455 . ?
O138 K6 O144 147.1(5) 1_455 . ?
O138 K6 Mo52 156.4(4) 1_455 . ?
O144 K6 O9 78.0(4) . . ?
O144 K6 Mo52 25.8(3) . . ?
O198 K6 O9 134.3(5) . . ?
O198 K6 O125 71.0(4) . 1_455 ?
O198 K6 O138 127.6(5) . 1_455 ?
O198 K6 O144 58.4(4) . . ?
O198 K6 Mo52 71.8(4) . . ?
K4 O207 K4 89.8(5) . 3_676 ?
O86 K5 O134 75.6(5) . 1_455 ?
O127 K5 O86 94.7(5) . . ?
O127 K5 O134 70.8(4) . 1_455 ?
O127 K5 O156 130.6(5) . 1_455 ?
O131 K5 O86 59.3(4) . . ?
O131 K5 O127 61.5(4) . . ?
O131 K5 O134 107.9(6) . 1_455 ?
O131 K5 O156 149.3(7) . 1_455 ?
O156 K5 O86 90.2(5) 1_455 . ?
O156 K5 O134 63.0(4) 1_455 1_455 ?
O206 K5 O86 108.3(6) . . ?
O206 K5 O127 106.8(5) . . ?
O206 K5 O131 73.3(4) . . ?
O206 K5 O134 175.8(7) . 1_455 ?
O206 K5 O156 118.1(6) . 1_455 ?
O66 K7 O176 126.4(6) . . ?
O66 K7 O197 115.8(5) . . ?
O66 K7 Mo46 105.6(5) . . ?
O66 K7 Mo50 95.6(5) . . ?
O66 K7 K8 124.5(5) . . ?
O66 K7 O209 134.5(7) . . ?
O79 K7 O66 63.9(4) . . ?
O79 K7 O176 79.3(5) . . ?
O79 K7 O197 65.8(4) . . ?
O79 K7 Mo46 73.4(4) . . ?
O79 K7 Mo50 64.9(4) . . ?
O79 K7 K8 171.4(5) . . ?
O79 K7 O209 141.4(7) . . ?
O176 K7 O197 77.9(5) . . ?
O176 K7 Mo46 22.8(3) . . ?
O176 K7 Mo50 102.7(5) . . ?
O176 K7 K8 95.2(4) . . ?
O197 K7 Mo46 95.4(5) . . ?
O197 K7 Mo50 25.6(3) . . ?
O197 K7 K8 106.8(4) . . ?
Mo46 K7 Mo50 117.5(4) . . ?
Mo46 K7 K8 104.0(4) . . ?
Mo50 K7 K8 110.5(4) . . ?
O208 K7 O66 135.7(7) . . ?
O208 K7 O79 135.8(7) . . ?
O208 K7 O176 97.9(6) . . ?
O208 K7 O197 70.5(5) . . ?
O208 K7 Mo46 117.8(6) . . ?
O208 K7 Mo50 73.0(5) . . ?
O208 K7 K8 38.0(4) . . ?
O208 K7 O209 61.3(5) . . ?
O209 K7 O176 62.7(5) . . ?
O209 K7 O197 109.7(5) . . ?
O209 K7 Mo46 68.9(4) . . ?
O209 K7 Mo50 127.8(5) . . ?
O209 K7 K8 35.1(4) . . ?
Mo38 K8 K7 104.8(4) . . ?
O51 K8 Mo38 84.1(4) 1_655 . ?
O51 K8 O76 59.0(4) 1_655 1_655 ?
O51 K8 O165 153.0(6) 1_655 . ?
O51 K8 K7 78.6(4) 1_655 . ?
O76 K8 Mo38 140.5(5) 1_655 . ?
O76 K8 O165 147.8(6) 1_655 . ?
O76 K8 K7 82.7(4) 1_655 . ?
O133 K8 Mo38 109.9(4) . . ?
O133 K8 O51 148.6(6) . 1_655 ?
O133 K8 O76 97.5(5) . 1_655 ?
O133 K8 O165 54.6(4) . . ?
O133 K8 K7 121.8(5) . . ?
O151 K8 Mo38 19.8(3) . . ?
O151 K8 O51 101.7(6) . 1_655 ?
O151 K8 O76 150.7(6) . 1_655 ?
O151 K8 O133 90.0(5) . . ?
O151 K8 O165 55.5(4) . . ?
O151 K8 K7 117.0(5) . . ?
O151 K8 O208 81.9(5) . . ?
O165 K8 Mo38 70.7(3) . . ?
O165 K8 K7 98.2(4) . . ?
O208 K8 Mo38 71.1(4) . . ?
O208 K8 O51 85.3(5) . 1_655 ?
O208 K8 O76 115.1(5) . 1_655 ?
O208 K8 O133 125.5(6) . . ?
O208 K8 O165 77.7(5) . . ?
O208 K8 K7 35.2(4) . . ?
O209 K8 Mo38 129.0(5) . . ?
O209 K8 O51 110.4(6) . 1_655 ?
O209 K8 O76 80.9(5) . 1_655 ?
O209 K8 O133 83.1(5) . . ?
O209 K8 O151 128.3(6) . . ?
O209 K8 O165 80.0(5) . . ?
O209 K8 K7 39.2(4) . . ?
O209 K8 O208 62.3(5) . . ?
K7 O208 K8 106.9(6) . . ?
K8 O209 K7 105.7(6) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Mo1 Ti1 O12 Mo39 -142.7(13) . . . . ?
Mo1 Ti1 O12 Mo55 154.6(17) . . . . ?
Mo1 Ti1 O12 Mo56 -79(2) . . . . ?
Mo1 Ti2 O108 Mo30 83.5(14) . . . . ?
Mo1 Ti2 O108 Mo48 140.3(12) . . . . ?
Mo2 Ti7 O91 Mo17 175(2) . . . . ?
Mo2 Ti7 O91 Mo40 -83.5(13) . . . . ?
Mo2 Ti7 O91 Mo53 -129.9(13) . . . . ?
Mo2 Ti10 O109 Mo41 -179(100) . . . . ?
Mo2 Ti10 O109 Mo46 89.1(15) . . . . ?
Mo2 Ti10 O109 Mo49 135.0(11) . . . . ?
Mo3 Ti4 O38 Mo39 128.2(11) . . . . ?
Mo3 Ti4 O38 Mo55 175(2) . . . . ?
Mo3 Ti4 O38 Mo56 81.9(16) . . . . ?
Mo3 Ti5 O32 Mo42 176.3(16) . . . . ?
Mo3 Ti5 O32 Mo51 -81.6(15) . . . . ?
Mo3 Ti5 O32 Mo57 -138(2) . . . . ?
Mo4 Ti3 O67 Mo42 -152.5(16) . . . . ?
Mo4 Ti3 O67 Mo51 71.7(19) . . . . ?
Mo4 Ti3 O67 Mo57 150(3) . . . . ?
Mo4 Ti6 O90 Mo30 -81.7(16) . . . . ?
Mo4 Ti6 O90 Mo48 -142.0(13) . . . . ?
Mo5 Ti8 O31 Mo29 134.2(11) . . . . ?
Mo5 Ti8 O31 Mo50 85.4(15) . . . . ?
Mo5 Ti9 O14 Mo41 147.4(17) . . . . ?
Mo5 Ti9 O14 Mo46 -82(2) . . . . ?
Mo5 Ti9 O14 Mo49 -147.8(16) . . . . ?
Mo6 Ti5 O32 Mo42 60(2) . . . . ?
Mo6 Ti5 O32 Mo51 162.3(13) . . . . ?
Mo6 Ti5 O32 Mo57 106(2) . . . . ?
Mo6 Ti10 O109 Mo41 -63(2) . . . . ?
Mo6 Ti10 O109 Mo46 -154.4(14) . . . . ?
Mo6 Ti10 O109 Mo49 -108.4(13) . . . . ?
Mo6 O166 O167 K2 -116.0(8) . . . 2_656 ?
Mo7 Mo16 O198 K6 58.4(18) . . . . ?
Mo7 Ti2 O108 Mo30 127.8(13) . . . . ?
Mo7 Ti2 O108 Mo48 -175.4(15) . . . . ?
Mo8 Mo35 O143 Mo36 -94.2(6) . . . . ?
Mo8 Mo35 O156 K5 124.3(14) . . . 1_655 ?
Mo8 Ti10 O109 Mo41 -135(2) . . . . ?
Mo8 Ti10 O109 Mo46 133.5(14) . . . . ?
Mo8 Ti10 O109 Mo49 179.5(13) . . . . ?
Mo9 Ti2 O108 Mo30 -159.7(12) . . . . ?
Mo9 Ti2 O108 Mo48 -102.9(15) . . . . ?
Mo9 Ti12 O17 Mo29 100.8(15) . . . . ?
Mo9 Ti12 O17 Mo50 157.3(16) . . . . ?
Mo10 Mo33 O164 K2 77.8(9) . . . . ?
Mo10 Mo33 O164 O185 -31.5(14) . . . . ?
Mo10 Mo33 O185 O164 162.7(8) . . . . ?
Mo11 Mo23 O127 K5 -59.5(13) . . . . ?
Mo11 Ti5 O32 Mo42 132(2) . . . . ?
Mo11 Ti5 O32 Mo51 -125.7(14) . . . . ?
Mo11 Ti5 O32 Mo57 178(2) . . . . ?
Mo12 Mo19 O76 K8 -177.4(4) . . . 1_455 ?
Mo12 Mo19 O86 K5 62.2(10) . . . . ?
Mo12 Ti3 O67 Mo42 -108(2) . . . . ?
Mo12 Ti3 O67 Mo51 116.5(18) . . . . ?
Mo12 Ti3 O67 Mo57 -166(3) . . . . ?
Mo13 Mo37 O138 K6 -125.2(12) . . . 1_655 ?
Mo13 Ti12 O17 Mo29 173.3(15) . . . . ?
Mo13 Ti12 O17 Mo50 -130.2(17) . . . . ?
Mo14 Ti3 O67 Mo42 -35(2) . . . . ?
Mo14 Ti3 O67 Mo51 -170.7(17) . . . . ?
Mo14 Ti3 O67 Mo57 -93(3) . . . . ?
Mo14 Ti9 O14 Mo41 31(2) . . . . ?
Mo14 Ti9 O14 Mo46 161(2) . . . . ?
Mo14 Ti9 O14 Mo49 95.9(19) . . . . ?
Mo14 O182 O183 K4 114.2(5) . . . 3_676 ?
Mo15 Ti9 O14 Mo41 104(2) . . . . ?
Mo15 Ti9 O14 Mo46 -126(2) . . . . ?
Mo15 Ti9 O14 Mo49 168.7(19) . . . . ?
Mo16 Mo7 O83 O191 29.7(15) . . . . ?
Mo16 Mo7 O191 O83 -164.2(8) . . . . ?
Mo43 Mo36 O133 K8 152.4(6) . . . . ?
Mo43 Mo36 O134 K5 -123.5(14) . . . 1_655 ?
Mo43 Ti7 O91 Mo17 132(3) . . . . ?
Mo43 Ti7 O91 Mo40 -126.6(12) . . . . ?
Mo43 Ti7 O91 Mo53 -173.0(15) . . . . ?
Mo18 Ti4 O38 Mo39 -115.9(12) . . . . ?
Mo18 Ti4 O38 Mo55 -69(2) . . . . ?
Mo18 Ti4 O38 Mo56 -162.2(14) . . . . ?
Mo18 Ti7 O91 Mo17 60(3) . . . . ?
Mo18 Ti7 O91 Mo40 161.0(11) . . . . ?
Mo18 Ti7 O91 Mo53 114.6(15) . . . . ?
Mo19 Mo12 O179 O180 -166.3(8) . . . . ?
Mo19 Mo12 O180 O179 27.1(15) . . . . ?
Mo20 Mo26 O9 K6 9.0(7) . . . . ?
Mo20 Mo26 O161 O193 -30.2(16) . . . . ?
Mo20 Mo26 O193 O161 163.0(9) . . . . ?
Mo21 Mo28 O171 O187 17.8(17) . . . . ?
Mo21 Mo28 O187 O171 -170.5(9) . . . . ?
Mo22 Mo27 O186 O194 28.3(15) . . . . ?
Mo22 Mo27 O194 O186 -164.8(8) . . . . ?
Mo23 Mo11 O158 K3 67.9(11) . . . 2_656 ?
Mo23 Mo11 O158 O181 -33.6(15) . . . . ?
Mo23 Mo11 O181 O158 162.8(8) . . . . ?
Mo24 Ti6 O90 Mo30 162.0(14) . . . . ?
Mo24 Ti6 O90 Mo48 101.7(16) . . . . ?
Mo24 Ti8 O31 Mo29 -107.8(14) . . . . ?
Mo24 Ti8 O31 Mo50 -156.6(13) . . . . ?
Mo25 Mo15 O177 O178 165.7(8) . . . . ?
Mo25 Mo15 O178 O177 -29.6(16) . . . . ?
Mo26 Mo20 O51 K8 171.0(5) . . . 1_455 ?
Mo26 Mo20 O74 K6 -48.5(12) . . . . ?
Mo26 Ti6 O90 Mo30 -125.2(14) . . . . ?
Mo26 Ti6 O90 Mo48 174.5(16) . . . . ?
Mo27 Ti4 O38 Mo39 171.8(13) . . . . ?
Mo27 Ti4 O38 Mo55 -141(2) . . . . ?
Mo27 Ti4 O38 Mo56 125.5(14) . . . . ?
Mo28 Ti8 O31 Mo29 179.6(14) . . . . ?
Mo28 Ti8 O31 Mo50 130.8(14) . . . . ?
Mo31 Mo38 O125 K6 130.2(14) . . . 1_655 ?
Mo31 Mo38 O151 K8 -155.0(7) . . . . ?
Mo31 Ti11 O37 Mo17 -106(2) . . . . ?
Mo31 Ti11 O37 Mo40 125.0(16) . . . . ?
Mo31 Ti11 O37 Mo53 -173.1(19) . . . . ?
Mo32 Ti1 O12 Mo39 100.9(16) . . . . ?
Mo32 Ti1 O12 Mo55 38(2) . . . . ?
Mo32 Ti1 O12 Mo56 165(2) . . . . ?
Mo32 Ti11 O37 Mo17 -33(2) . . . . ?
Mo32 Ti11 O37 Mo40 -162.5(16) . . . . ?
Mo32 Ti11 O37 Mo53 -100.5(19) . . . . ?
Mo32 O192 O195 K3 -113.7(8) . . . . ?
Mo33 Mo10 O146 Mo16 92.4(6) . . . . ?
Mo33 Ti1 O12 Mo39 173.4(16) . . . . ?
Mo33 Ti1 O12 Mo55 111(2) . . . . ?
Mo33 Ti1 O12 Mo56 -123(2) . . . . ?
Mo34 Ti11 O37 Mo17 -151.0(17) . . . . ?
Mo34 Ti11 O37 Mo40 79.7(18) . . . . ?
Mo34 Ti11 O37 Mo53 141.7(16) . . . . ?
Mo34 Ti12 O17 Mo29 -143.2(12) . . . . ?
Mo34 Ti12 O17 Mo50 -86.8(17) . . . . ?
Mo35 Mo8 O170 K2 -75.8(10) . . . 2_656 ?
Mo35 Mo8 O170 O190 32.8(14) . . . . ?
Mo35 Mo8 O190 O170 -162.3(8) . . . . ?
Mo36 Mo43 O168 O189 -22.0(15) . . . . ?
Mo36 Mo43 O189 O168 167.8(8) . . . . ?
Mo37 Mo13 O142 O184 -31.7(14) . . . . ?
Mo37 Mo13 O184 O142 162.7(8) . . . . ?
Mo38 Mo31 O162 K3 -76.3(9) . . . . ?
Mo38 Mo31 O162 O188 28.8(14) . . . . ?
Mo38 Mo31 O188 O162 -164.9(8) . . . . ?
Mo41 Mo42 O81 K4 -5.4(8) . . . . ?
Mo42 Mo41 O34 K4 10.1(9) . . . . ?
Mo42 Mo41 O109 Ti10 10(2) . . . . ?
Ti1 Mo1 O19 Mo10 -20.2(5) . . . . ?
Ti1 Mo1 O19 Mo16 81.6(5) . . . . ?
Ti1 Mo1 O49 K2 -90.8(8) . . . . ?
Ti1 Mo32 O192 K2 50.9(7) . . . . ?
Ti1 Mo32 O192 O195 161.9(7) . . . . ?
Ti1 Mo32 O195 K3 71.9(11) . . . . ?
Ti1 Mo32 O195 O192 -40.1(15) . . . . ?
Ti1 Mo33 O164 K2 -51.3(7) . . . . ?
Ti1 Mo33 O164 O185 -160.6(8) . . . . ?
Ti1 Mo33 O185 O164 43.3(15) . . . . ?
Ti1 Ti2 O108 Mo30 -13.9(16) . . . . ?
Ti1 Ti2 O108 Mo48 43.0(17) . . . . ?
Ti1 O8 O16 Ti2 -107.9(4) . . . . ?
Ti2 Mo1 O19 Mo10 -79.8(5) . . . . ?
Ti2 Mo1 O19 Mo16 21.9(5) . . . . ?
Ti2 Mo1 O49 K2 -58.0(11) . . . . ?
Ti2 Mo7 O83 O191 158.8(9) . . . . ?
Ti2 Mo7 O191 O83 -44.1(16) . . . . ?
Ti2 Mo9 O160 O163 161.6(7) . . . . ?
Ti2 Mo9 O163 O160 -39.9(15) . . . . ?
Ti2 Ti1 O12 Mo39 -46.4(18) . . . . ?
Ti2 Ti1 O12 Mo55 -109(2) . . . . ?
Ti2 Ti1 O12 Mo56 18(2) . . . . ?
Ti2 O8 O16 Ti1 107.9(4) . . . . ?
Ti3 Mo4 O56 Mo12 -39.4(4) . . . . ?
Ti3 Mo4 O71 Mo19 20.5(6) . . . . ?
Ti3 Mo4 O71 Mo20 -79.3(5) . . . . ?
Ti3 Mo12 O179 O180 -38.7(16) . . . . ?
Ti3 Mo12 O180 O179 162.3(8) . . . . ?
Ti3 Mo14 O70 K4 -147.8(3) . . . 3_676 ?
Ti3 Mo14 O182 O183 38.5(18) . . . . ?
Ti3 Mo14 O182 K4 112.0(11) . . . 3_676 ?
Ti3 Mo14 O183 O182 -163.5(8) . . . . ?
Ti3 Mo14 O183 K4 130.8(4) . . . 3_676 ?
Ti3 Ti6 O90 Mo30 17.6(17) . . . . ?
Ti3 Ti6 O90 Mo48 -42.6(19) . . . . ?
Ti3 O13 O30 Ti6 107.7(4) . . . . ?
Ti3 O67 Mo51 O32 162.3(14) . . . . ?
Ti3 O67 Mo51 O131 -95.7(18) . . . . ?
Ti3 O67 Mo51 O200 38(2) . . . . ?
Ti3 O67 Mo57 O32 -169.4(18) . . . . ?
Ti3 O67 Mo57 O58 46(3) . . . . ?
Ti3 O67 Mo57 O81 134(3) . . . . ?
Ti3 O67 Mo57 O131 -155(3) . . . . ?
Ti3 O67 Mo57 O200 -69(3) . . . . ?
Ti4 Mo3 O43 Mo11 71.4(7) . . . . ?
Ti4 Mo3 O43 K3 -62.2(12) . . . 2_656 ?
Ti4 Mo3 O48 Mo27 -40.2(4) . . . . ?
Ti4 Mo3 O124 Mo22 20.2(6) . . . . ?
Ti4 Mo3 O124 Mo23 -81.7(5) . . . . ?
Ti4 Mo18 O159 O173 -37.4(17) . . . . ?
Ti4 Mo18 O173 O159 163.5(8) . . . . ?
Ti4 Mo27 O65 Mo22 15.3(7) . . . . ?
Ti4 Mo27 O186 O194 157.3(9) . . . . ?
Ti4 Mo27 O194 O186 -47.1(16) . . . . ?
Ti4 Ti5 O32 Mo42 -87(2) . . . . ?
Ti4 Ti5 O32 Mo51 15.0(16) . . . . ?
Ti4 Ti5 O32 Mo57 -42(3) . . . . ?
Ti4 O15 O45 Ti5 -107.0(4) . . . . ?
Ti5 Mo3 O43 Mo11 39.1(4) . . . . ?
Ti5 Mo3 O43 K3 -94.4(9) . . . 2_656 ?
Ti5 Mo3 O48 Mo27 -72.8(7) . . . . ?
Ti5 Mo3 O124 Mo22 79.9(5) . . . . ?
Ti5 Mo3 O124 Mo23 -22.0(6) . . . . ?
Ti5 Mo6 O166 K3 47.4(8) . . . 2_656 ?
Ti5 Mo6 O166 O167 161.4(8) . . . . ?
Ti5 Mo6 O167 K2 71.6(10) . . . 2_656 ?
Ti5 Mo6 O167 O166 -38.4(14) . . . . ?
Ti5 Mo11 O158 K3 -59.0(7) . . . 2_656 ?
Ti5 Mo11 O158 O181 -160.5(8) . . . . ?
Ti5 Mo11 O181 O158 39.3(16) . . . . ?
Ti5 Ti4 O38 Mo39 30.5(15) . . . . ?
Ti5 Ti4 O38 Mo55 77(2) . . . . ?
Ti5 Ti4 O38 Mo56 -15.8(17) . . . . ?
Ti5 O15 O45 Ti4 107.0(4) . . . . ?
Ti5 O32 Mo57 O58 -58(3) . . . . ?
Ti5 O32 Mo57 O67 157(2) . . . . ?
Ti5 O32 Mo57 O81 -145.2(19) . . . . ?
Ti5 O32 Mo57 O131 143(2) . . . . ?
Ti5 O32 Mo57 O200 56(3) . . . . ?
Ti6 Mo4 O56 Mo12 -71.8(7) . . . . ?
Ti6 Mo4 O71 Mo19 80.6(5) . . . . ?
Ti6 Mo4 O71 Mo20 -19.1(6) . . . . ?
Ti6 Mo24 O172 O174 -163.6(8) . . . . ?
Ti6 Mo24 O174 O172 35.6(16) . . . . ?
Ti6 Mo26 O9 K6 88.1(7) . . . . ?
Ti6 Mo26 O89 Mo20 -15.0(7) . . . . ?
Ti6 Mo26 O161 O193 -159.5(9) . . . . ?
Ti6 Mo26 O193 O161 44.7(18) . . . . ?
Ti6 Ti3 O67 Mo42 112.0(19) . . . . ?
Ti6 Ti3 O67 Mo51 -24(2) . . . . ?
Ti6 Ti3 O67 Mo57 54(3) . . . . ?
Ti6 O13 O30 Ti3 -107.7(4) . . . . ?
Ti6 O90 Mo48 K1 23.0(19) . . . . ?
Ti6 O90 Mo48 O87 55.3(18) . . . . ?
Ti6 O90 Mo48 O103 -59.6(19) . . . . ?
Ti6 O90 Mo48 O108 158.9(13) . . . . ?
Ti6 O90 Mo48 O144 127.8(17) . . . . ?
Ti6 O90 Mo48 O175 -156.9(17) . . . . ?
Ti7 Mo2 O4 K2 55.5(11) . . . 2_656 ?
Ti7 Mo2 O54 Mo43 39.5(4) . . . . ?
Ti7 Mo2 O147 Mo35 79.9(5) . . . . ?
Ti7 Mo2 O147 Mo36 -19.7(6) . . . . ?
Ti7 Mo43 O116 Mo36 -17.3(6) . . . . ?
Ti7 Mo43 O168 O189 -156.1(8) . . . . ?
Ti7 Mo43 O189 O168 52.2(16) . . . . ?
Ti7 Mo18 O159 O173 -162.4(8) . . . . ?
Ti7 Mo18 O173 O159 38.9(16) . . . . ?
Ti7 Ti10 O109 Mo41 85(2) . . . . ?
Ti7 Ti10 O109 Mo46 -6.6(17) . . . . ?
Ti7 Ti10 O109 Mo49 39.4(16) . . . . ?
Ti7 O21 O85 Ti10 106.9(4) . . . . ?
Ti7 O91 Mo53 K1 1(2) . . . . ?
Ti7 O91 Mo53 O37 161.1(13) . . . . ?
Ti7 O91 Mo53 O140 -71.2(17) . . . . ?
Ti7 O91 Mo53 O153 46.4(17) . . . . ?
Ti7 O91 Mo53 O165 129.2(15) . . . . ?
Ti7 O91 Mo53 O202 -157.6(15) . . . . ?
Ti8 Mo5 O42 Mo15 70.7(7) . . . . ?
Ti8 Mo5 O46 Mo21 20.0(6) . . . . ?
Ti8 Mo5 O46 Mo25 -80.6(5) . . . . ?
Ti8 Mo24 O172 O174 -41.6(16) . . . . ?
Ti8 Mo24 O174 O172 161.8(8) . . . . ?
Ti8 Mo28 O171 O187 149.1(10) . . . . ?
Ti8 Mo28 O187 O171 -60.7(16) . . . . ?
Ti8 Ti9 O14 Mo41 -116.3(19) . . . . ?
Ti8 Ti9 O14 Mo46 14(2) . . . . ?
Ti8 Ti9 O14 Mo49 -52(2) . . . . ?
Ti8 O27 O79 Ti9 107.1(4) . . . . ?
Ti8 O27 O79 K7 -134.6(9) . . . . ?
Ti8 O31 Mo50 O17 156.1(11) . . . . ?
Ti8 O31 Mo50 O72 -86.6(15) . . . . ?
Ti8 O31 Mo50 O103 109.8(14) . . . . ?
Ti8 O31 Mo50 O169 -175.0(14) . . . . ?
Ti8 O31 Mo50 O197 31.1(16) . . . . ?
Ti8 O31 Mo50 K7 -21.6(14) . . . . ?
Ti9 Mo5 O42 Mo15 39.0(4) . . . . ?
Ti9 Mo5 O46 Mo21 79.8(5) . . . . ?
Ti9 Mo5 O46 Mo25 -20.8(6) . . . . ?
Ti9 Mo14 O70 K4 137.7(3) . . . 3_676 ?
Ti9 Mo14 O182 O183 163.6(8) . . . . ?
Ti9 Mo14 O182 K4 -122.9(4) . . . 3_676 ?
Ti9 Mo14 O183 O182 -35.5(17) . . . . ?
Ti9 Mo14 O183 K4 -101.2(10) . . . 3_676 ?
Ti9 Mo15 O177 O178 38.0(16) . . . . ?
Ti9 Mo15 O178 O177 -161.4(8) . . . . ?
Ti9 Ti8 O31 Mo29 39.7(16) . . . . ?
Ti9 Ti8 O31 Mo50 -9.2(16) . . . . ?
Ti9 O27 O79 Ti8 -107.1(4) . . . . ?
Ti9 O27 O79 K7 118.3(9) . . . . ?
Ti10 Mo2 O4 K2 88.5(8) . . . 2_656 ?
Ti10 Mo2 O54 Mo43 71.3(7) . . . . ?
Ti10 Mo2 O147 Mo35 20.0(6) . . . . ?
Ti10 Mo2 O147 Mo36 -79.6(5) . . . . ?
Ti10 Mo6 O166 K3 -69.9(11) . . . 2_656 ?
Ti10 Mo6 O166 O167 44.1(14) . . . . ?
Ti10 Mo6 O167 K2 -48.7(7) . . . 2_656 ?
Ti10 Mo6 O167 O166 -158.6(7) . . . . ?
Ti10 Mo8 O170 K2 50.8(7) . . . 2_656 ?
Ti10 Mo8 O170 O190 159.5(8) . . . . ?
Ti10 Mo8 O190 O170 -43.6(16) . . . . ?
Ti10 Ti7 O91 Mo17 -86(3) . . . . ?
Ti10 Ti7 O91 Mo40 14.8(15) . . . . ?
Ti10 Ti7 O91 Mo53 -31.6(18) . . . . ?
Ti10 O21 O85 Ti7 -106.9(4) . . . . ?
Ti11 Mo31 O162 K3 53.3(7) . . . . ?
Ti11 Mo31 O162 O188 158.3(8) . . . . ?
Ti11 Mo31 O188 O162 -45.7(15) . . . . ?
Ti11 Mo32 O192 K2 -76.4(11) . . . . ?
Ti11 Mo32 O192 O195 34.6(15) . . . . ?
Ti11 Mo32 O195 K3 -52.5(7) . . . . ?
Ti11 Mo32 O195 O192 -164.5(7) . . . . ?
Ti11 Mo34 O120 Mo31 -39.1(4) . . . . ?
Ti11 Mo34 O120 K3 89.5(8) . . . . ?
Ti11 Mo34 O128 Mo13 70.3(7) . . . . ?
Ti11 Mo34 O137 Mo37 -79.9(5) . . . . ?
Ti11 Mo34 O137 Mo38 20.9(5) . . . . ?
Ti11 Ti12 O17 Mo29 -46.4(17) . . . . ?
Ti11 Ti12 O17 Mo50 10.0(19) . . . . ?
Ti11 O115 O129 Ti12 107.2(4) . . . . ?
Ti12 Mo9 O160 O163 35.1(16) . . . . ?
Ti12 Mo9 O163 O160 -165.3(7) . . . . ?
Ti12 Mo13 O142 O184 -160.6(8) . . . . ?
Ti12 Mo13 O184 O142 42.6(16) . . . . ?
Ti12 Mo34 O120 Mo31 -72.3(6) . . . . ?
Ti12 Mo34 O120 K3 56.3(11) . . . . ?
Ti12 Mo34 O128 Mo13 39.4(4) . . . . ?
Ti12 Mo34 O137 Mo37 -20.1(6) . . . . ?
Ti12 Mo34 O137 Mo38 80.6(5) . . . . ?
Ti12 Ti11 O37 Mo17 113(2) . . . . ?
Ti12 Ti11 O37 Mo40 -16.0(19) . . . . ?
Ti12 Ti11 O37 Mo53 46(2) . . . . ?
Ti12 O17 Mo50 O31 -155.7(13) . . . . ?
Ti12 O17 Mo50 O72 87.0(17) . . . . ?
Ti12 O17 Mo50 O103 -109.7(17) . . . . ?
Ti12 O17 Mo50 O169 175.6(17) . . . . ?
Ti12 O17 Mo50 O197 -31.1(19) . . . . ?
Ti12 O17 Mo50 K7 22(2) . . . . ?
Ti12 O115 O129 Ti11 -107.2(4) . . . . ?
K1 Mo29 O31 Ti8 -13.4(16) . . . . ?
K1 Mo29 O103 Mo30 20(2) . . . . ?
K1 Mo29 O197 K7 171.6(11) . . . . ?
K1 Mo39 O140 Mo17 -166(5) . . . . ?
K1 O8 O16 Ti1 -118.9(6) . . . . ?
K1 O8 O16 Ti2 133.1(6) . . . . ?
K1 O80 Mo56 O12 -39.8(9) . . . . ?
K1 O80 Mo56 O38 112.1(7) . . . . ?
K1 O80 Mo56 O82 -143.6(7) . . . . ?
K1 O80 Mo56 O140 36.0(7) . . . . ?
K1 O80 Mo56 O157 36.7(18) . . . . ?
K1 O87 Mo48 O90 -135.1(6) . . . . ?
K1 O87 Mo48 O103 -26.5(9) . . . . ?
K1 O87 Mo48 O108 78.0(6) . . . . ?
K1 O87 Mo48 O144 150.9(6) . . . . ?
K1 O87 Mo48 O175 149.9(9) . . . . ?
K1 O115 O129 Ti11 120.2(6) . . . . ?
K1 O115 O129 Ti12 -132.6(6) . . . . ?
K1 O140 Mo53 O37 -79.0(6) . . . . ?
K1 O140 Mo53 O91 126.5(6) . . . . ?
K1 O140 Mo53 O153 22.7(7) . . . . ?
K1 O140 Mo53 O165 -157.6(19) . . . . ?
K1 O140 Mo53 O202 -155.9(4) . . . . ?
K1 O140 Mo55 O12 51.0(6) . . . . ?
K1 O140 Mo55 O38 -100.5(6) . . . . ?
K1 O140 Mo55 O80 -24.7(5) . . . . ?
K1 O140 Mo55 O82 -23(2) . . . . ?
K1 O140 Mo55 O157 155.4(6) . . . . ?
K1 O153 Mo40 O37 42.0(8) . . . . ?
K1 O153 Mo40 O91 -111.2(7) . . . . ?
K1 O153 Mo40 O140 -34.6(7) . . . . ?
K1 O153 Mo40 O165 147.6(7) . . . . ?
K1 O153 Mo40 O202 -34(2) . . . . ?
K1 O153 Mo53 O37 75.7(6) . . . . ?
K1 O153 Mo53 O91 -133.7(6) . . . . ?
K1 O153 Mo53 O140 -28.0(8) . . . . ?
K1 O153 Mo53 O165 152.1(5) . . . . ?
K1 O153 Mo53 O202 148.6(15) . . . . ?
K1 O197 Mo50 O17 -26.6(12) . . . . ?
K1 O197 Mo50 O31 126.3(9) . . . . ?
K1 O197 Mo50 O72 -130.6(10) . . . . ?
K1 O197 Mo50 O103 50.4(10) . . . . ?
K1 O197 Mo50 O169 53.3(19) . . . . ?
K1 O197 Mo50 K7 -152.4(12) . . . . ?
K2 Mo6 O166 K3 -73.1(6) 2_656 . . 2_656 ?
K2 Mo6 O166 O167 40.9(8) 2_656 . . . ?
K2 Mo6 O167 O166 -110.0(11) 2_656 . . . ?
K2 Mo8 O170 O190 108.6(12) 2_656 . . . ?
K2 Mo8 O190 O170 -42.3(8) 2_656 . . . ?
K2 Mo32 O192 O195 111.0(11) . . . . ?
K2 Mo32 O195 K3 70.6(5) . . . . ?
K2 Mo32 O195 O192 -41.4(8) . . . . ?
K2 Mo33 O164 O185 -109.3(11) . . . . ?
K2 Mo33 O185 O164 43.4(8) . . . . ?
K2 O164 O185 Mo33 -113.4(7) . . . . ?
K2 O170 O190 Mo8 113.2(8) 2_656 . . . ?
K2 O192 O195 Mo32 113.0(8) . . . . ?
K2 O192 O195 K3 -0.7(13) . . . . ?
K3 Mo31 O162 O188 105.1(11) . . . . ?
K3 Mo31 O188 O162 -45.0(8) . . . . ?
K3 O158 O181 Mo11 -114.7(7) 2_656 . . . ?
K3 O162 O188 Mo31 112.8(7) . . . . ?
K3 O166 O167 Mo6 119.3(9) 2_656 . . . ?
K3 O166 O167 K2 3.3(14) 2_656 . . 2_656 ?
O1 Mo1 O19 Mo10 -49.2(8) . . . . ?
O1 Mo1 O19 Mo16 52.5(9) . . . . ?
O1 Mo1 O49 K2 -55.2(9) . . . . ?
O2 Mo9 O160 O163 140.2(11) . . . . ?
O2 Mo9 O163 O160 -137.3(11) . . . . ?
O2 Ti2 O108 Mo30 -122.4(13) . . . . ?
O2 Ti2 O108 Mo48 -65.5(16) . . . . ?
O2 Ti12 O17 Mo29 63.0(16) . . . . ?
O2 Ti12 O17 Mo50 119.5(17) . . . . ?
O3 Mo3 O43 Mo11 74.5(5) . . . . ?
O3 Mo3 O43 K3 -59.1(10) . . . 2_656 ?
O3 Mo3 O48 Mo27 -75.4(5) . . . . ?
O3 Mo3 O124 Mo22 49.6(9) . . . . ?
O3 Mo3 O124 Mo23 -52.2(9) . . . . ?
O4 Mo2 O54 Mo43 -179.9(5) . . . . ?
O4 Mo2 O147 Mo35 -75.4(6) . . . . ?
O4 Mo2 O147 Mo36 -175.0(5) . . . . ?
O5 Mo6 O166 K3 -25.4(6) . . . 2_656 ?
O5 Mo6 O166 O167 88.6(9) . . . . ?
O5 Mo6 O167 K2 24.5(6) . . . 2_656 ?
O5 Mo6 O167 O166 -85.5(9) . . . . ?
O6 Mo18 O159 O173 -138.2(12) . . . . ?
O6 Mo18 O173 O159 137.9(12) . . . . ?
O6 Ti4 O38 Mo39 -77.8(13) . . . . ?
O6 Ti4 O38 Mo55 -31(2) . . . . ?
O6 Ti4 O38 Mo56 -124.1(14) . . . . ?
O6 Ti7 O91 Mo17 22(3) . . . . ?
O6 Ti7 O91 Mo40 123.0(12) . . . . ?
O6 Ti7 O91 Mo53 76.6(16) . . . . ?
O7 Mo7 O83 O191 166.8(10) . . . . ?
O7 Mo7 O191 O83 -15.6(12) . . . . ?
O7 Mo9 O160 O163 170.1(9) . . . . ?
O7 Mo9 O163 O160 -11.7(11) . . . . ?
O7 Ti2 O108 Mo30 163.9(13) . . . . ?
O7 Ti2 O108 Mo48 -139.3(15) . . . . ?
O8 Ti1 O12 Mo39 -22.8(17) . . . . ?
O8 Ti1 O12 Mo55 -85(2) . . . . ?
O8 Ti1 O12 Mo56 41(2) . . . . ?
O8 Ti2 O108 Mo30 -36.3(13) . . . . ?
O8 Ti2 O108 Mo48 20.5(16) . . . . ?
O9 Mo26 O89 Mo20 85.6(7) . . . . ?
O9 Mo26 O161 O193 93.3(11) . . . . ?
O9 Mo26 O193 O161 -95.6(11) . . . . ?
O10 Mo24 O172 O174 92.0(10) . . . . ?
O10 Mo24 O174 O172 -93.0(10) . . . . ?
O11 Mo24 O172 O174 -138.3(12) . . . . ?
O11 Mo24 O174 O172 136.7(12) . . . . ?
O11 Ti6 O90 Mo30 124.5(14) . . . . ?
O11 Ti6 O90 Mo48 64.3(17) . . . . ?
O11 Ti8 O31 Mo29 -70.4(14) . . . . ?
O11 Ti8 O31 Mo50 -119.2(14) . . . . ?
O12 Mo39 O80 K1 -74.7(5) . . . . ?
O12 Mo39 O140 Mo17 -86(4) . . . . ?
O12 Mo39 O140 K1 80.3(4) . . . . ?
O13 Ti3 O67 Mo42 88(2) . . . . ?
O13 Ti3 O67 Mo51 -47.6(18) . . . . ?
O13 Ti3 O67 Mo57 30(3) . . . . ?
O13 Ti6 O90 Mo30 38.7(15) . . . . ?
O13 Ti6 O90 Mo48 -21.6(17) . . . . ?
O14 Mo41 O34 K4 114.3(9) . . . . ?
O14 Mo41 O58 Mo42 -105.5(14) . . . . ?
O14 Mo41 O109 Ti10 -127(2) . . . . ?
O15 Ti4 O38 Mo39 50.0(13) . . . . ?
O15 Ti4 O38 Mo55 97(2) . . . . ?
O15 Ti4 O38 Mo56 3.7(15) . . . . ?
O15 Ti5 O32 Mo42 -106(2) . . . . ?
O15 Ti5 O32 Mo51 -3.7(14) . . . . ?
O15 Ti5 O32 Mo57 -60(2) . . . . ?
O16 Ti1 O12 Mo39 -65.3(16) . . . . ?
O16 Ti1 O12 Mo55 -128(2) . . . . ?
O16 Ti1 O12 Mo56 -1(2) . . . . ?
O16 Ti2 O108 Mo30 5.8(13) . . . . ?
O16 Ti2 O108 Mo48 62.7(15) . . . . ?
O17 Mo29 O31 Ti8 -155.6(11) . . . . ?
O17 Mo29 O103 Mo30 99(2) . . . . ?
O17 Mo29 O197 K1 -69.1(6) . . . . ?
O17 Mo29 O197 K7 102.5(7) . . . . ?
O18 Mo13 O142 O184 93.9(10) . . . . ?
O18 Mo13 O184 O142 -95.2(10) . . . . ?
O19 Mo1 O49 K2 158.8(8) . . . . ?
O19 Mo10 O146 Mo16 23.7(5) . . . . ?
O19 Mo16 O198 K6 125(2) . . . . ?
O20 Mo3 O48 Mo27 -3.3(4) . . . . ?
O20 Mo3 O124 Mo22 2.8(5) . . . . ?
O20 Mo3 O124 Mo23 -99.1(5) . . . . ?
O20 Mo27 O65 Mo22 18.7(6) . . . . ?
O20 Mo27 O186 O194 115.1(11) . . . . ?
O20 Mo27 O194 O186 -121.6(11) . . . . ?
O20 Ti4 O38 Mo39 133.2(13) . . . . ?
O20 Ti4 O38 Mo55 -180(100) . . . . ?
O20 Ti4 O38 Mo56 86.9(15) . . . . ?
O21 Ti7 O91 Mo17 -106(3) . . . . ?
O21 Ti7 O91 Mo40 -5.2(12) . . . . ?
O21 Ti7 O91 Mo53 -51.6(16) . . . . ?
O21 Ti10 O109 Mo41 104(2) . . . . ?
O21 Ti10 O109 Mo46 11.6(14) . . . . ?
O21 Ti10 O109 Mo49 57.6(14) . . . . ?
O22 Mo12 O179 O180 -13.1(12) . . . . ?
O22 Mo12 O180 O179 168.8(10) . . . . ?
O22 Mo14 O70 K4 -109.4(4) . . . 3_676 ?
O22 Mo14 O182 O183 10.8(12) . . . . ?
O22 Mo14 O182 K4 84.3(7) . . . 3_676 ?
O22 Mo14 O183 O182 -171.0(10) . . . . ?
O22 Mo14 O183 K4 123.4(6) . . . 3_676 ?
O22 Ti3 O67 Mo42 -72(2) . . . . ?
O22 Ti3 O67 Mo51 152.8(17) . . . . ?
O22 Ti3 O67 Mo57 -129(3) . . . . ?
O23 Mo14 O70 K4 99.4(5) . . . 3_676 ?
O23 Mo14 O182 O183 171.5(11) . . . . ?
O23 Mo14 O182 K4 -115.0(6) . . . 3_676 ?
O23 Mo14 O183 O182 -9.8(12) . . . . ?
O23 Mo14 O183 K4 -75.5(7) . . . 3_676 ?
O23 Mo15 O177 O178 13.8(12) . . . . ?
O23 Mo15 O178 O177 -167.9(10) . . . . ?
O23 Ti9 O14 Mo41 68(2) . . . . ?
O23 Ti9 O14 Mo46 -162(2) . . . . ?
O23 Ti9 O14 Mo49 132.3(19) . . . . ?
O24 Mo2 O4 K2 53.3(9) . . . 2_656 ?
O24 Mo2 O54 Mo43 74.8(5) . . . . ?
O24 Mo2 O147 Mo35 49.1(9) . . . . ?
O24 Mo2 O147 Mo36 -50.5(9) . . . . ?
O25 Mo1 O19 Mo10 -97.9(5) . . . . ?
O25 Mo1 O19 Mo16 3.9(4) . . . . ?
O25 Mo7 O83 O191 116.1(11) . . . . ?
O25 Mo7 O191 O83 -120.7(10) . . . . ?
O25 Mo16 O198 K6 97.9(18) . . . . ?
O25 Ti2 O108 Mo30 89.1(13) . . . . ?
O25 Ti2 O108 Mo48 146.0(15) . . . . ?
O26 Mo2 O4 K2 125.5(9) . . . 2_656 ?
O26 Mo2 O147 Mo35 2.3(4) . . . . ?
O26 Mo2 O147 Mo36 -97.3(5) . . . . ?
O26 Mo8 O170 K2 7.5(12) . . . 2_656 ?
O26 Mo8 O170 O190 116.1(11) . . . . ?
O26 Mo8 O190 O170 -120.0(10) . . . . ?
O26 Mo35 O143 Mo36 -96.3(6) . . . . ?
O26 Mo35 O156 K5 79(2) . . . 1_655 ?
O26 Ti10 O109 Mo41 -173(2) . . . . ?
O26 Ti10 O109 Mo46 95.2(14) . . . . ?
O26 Ti10 O109 Mo49 141.2(13) . . . . ?
O27 Ti8 O31 Mo29 15.5(14) . . . . ?
O27 Ti8 O31 Mo50 -33.3(14) . . . . ?
O27 Ti9 O14 Mo41 -92(2) . . . . ?
O27 Ti9 O14 Mo46 38(2) . . . . ?
O27 Ti9 O14 Mo49 -27.5(19) . . . . ?
O29 Mo19 O76 K8 25.8(8) . . . 1_455 ?
O29 Mo19 O86 K5 -170.8(10) . . . . ?
O29 Mo20 O51 K8 -31.3(8) . . . 1_455 ?
O29 Mo20 O74 K6 -176.8(12) . . . . ?
O30 Ti3 O67 Mo42 130(2) . . . . ?
O30 Ti3 O67 Mo51 -5.2(18) . . . . ?
O30 Ti3 O67 Mo57 73(3) . . . . ?
O30 Ti6 O90 Mo30 -3.4(15) . . . . ?
O30 Ti6 O90 Mo48 -63.7(17) . . . . ?
O31 Mo29 O103 Mo30 -101(2) . . . . ?
O31 Mo29 O197 K1 139.3(6) . . . . ?
O31 Mo29 O197 K7 -49.1(7) . . . . ?
O32 Mo42 O58 Mo41 -106.9(13) . . . . ?
O32 Mo42 O81 K4 101.7(8) . . . . ?
O33 Mo18 O159 O173 93.5(10) . . . . ?
O33 Mo18 O173 O159 -91.5(10) . . . . ?
O34 Mo41 O58 Mo42 0.2(16) . . . . ?
O34 Mo41 O109 Ti10 108(2) . . . . ?
O35 Mo43 O116 Mo36 -38.7(12) . . . . ?
O35 Mo43 O168 O189 -163.5(10) . . . . ?
O35 Mo43 O189 O168 20.0(12) . . . . ?
O35 Mo18 O159 O173 -170.6(10) . . . . ?
O35 Mo18 O173 O159 11.2(12) . . . . ?
O35 Ti7 O91 Mo17 97(3) . . . . ?
O35 Ti7 O91 Mo40 -162.1(12) . . . . ?
O35 Ti7 O91 Mo53 151.5(15) . . . . ?
O36 Mo24 O172 O174 -172.1(10) . . . . ?
O36 Mo24 O174 O172 9.2(12) . . . . ?
O36 Mo26 O9 K6 125.3(8) . . . . ?
O36 Mo26 O89 Mo20 -34.4(13) . . . . ?
O36 Mo26 O161 O193 -169.3(11) . . . . ?
O36 Mo26 O193 O161 12.9(13) . . . . ?
O36 Ti6 O90 Mo30 -161.2(14) . . . . ?
O36 Ti6 O90 Mo48 138.5(16) . . . . ?
O37 Mo17 O140 Mo39 117(4) . . . . ?
O37 Mo17 O140 K1 -48.7(6) . . . . ?
O38 Mo39 O80 K1 134.1(5) . . . . ?
O38 Mo39 O140 Mo17 66(4) . . . . ?
O38 Mo39 O140 K1 -128.2(4) . . . . ?
O39 Mo10 O146 Mo16 53.4(12) . . . . ?
O39 Mo33 O164 K2 95.1(6) . . . . ?
O39 Mo33 O164 O185 -14.2(11) . . . . ?
O39 Mo33 O185 O164 167.1(10) . . . . ?
O40 Mo10 O146 Mo16 -65.1(7) . . . . ?
O41 Mo3 O43 Mo11 2.6(4) . . . . ?
O41 Mo3 O43 K3 -130.9(10) . . . 2_656 ?
O41 Mo3 O124 Mo22 97.8(6) . . . . ?
O41 Mo3 O124 Mo23 -4.1(5) . . . . ?
O41 Mo11 O158 K3 -19.0(12) . . . 2_656 ?
O41 Mo11 O158 O181 -120.5(11) . . . . ?
O41 Mo11 O181 O158 117.2(11) . . . . ?
O41 Mo23 O127 K5 -99.7(13) . . . . ?
O41 Ti5 O32 Mo42 171(2) . . . . ?
O41 Ti5 O32 Mo51 -87.0(14) . . . . ?
O41 Ti5 O32 Mo57 -144(2) . . . . ?
O42 Mo5 O46 Mo21 174.3(6) . . . . ?
O42 Mo5 O46 Mo25 73.7(6) . . . . ?
O42 Mo15 O177 O178 86.6(10) . . . . ?
O42 Mo15 O178 O177 -87.4(10) . . . . ?
O43 Mo3 O48 Mo27 178.8(5) . . . . ?
O43 Mo3 O124 Mo22 175.0(5) . . . . ?
O43 Mo3 O124 Mo23 73.2(6) . . . . ?
O43 Mo11 O158 K3 12.6(6) . . . 2_656 ?
O43 Mo11 O158 O181 -88.9(10) . . . . ?
O43 Mo11 O181 O158 84.7(10) . . . . ?
O44 Mo4 O56 Mo12 -3.3(4) . . . . ?
O44 Mo4 O71 Mo19 3.1(4) . . . . ?
O44 Mo4 O71 Mo20 -96.7(5) . . . . ?
O44 Mo12 O179 O180 -122.7(11) . . . . ?
O44 Mo12 O180 O179 123.5(11) . . . . ?
O44 Mo19 O76 K8 135.1(12) . . . 1_455 ?
O44 Mo19 O86 K5 102.0(10) . . . . ?
O44 Ti3 O67 Mo42 -146(2) . . . . ?
O44 Ti3 O67 Mo51 78.3(18) . . . . ?
O44 Ti3 O67 Mo57 156(3) . . . . ?
O45 Ti4 O38 Mo39 7.9(13) . . . . ?
O45 Ti4 O38 Mo55 55(2) . . . . ?
O45 Ti4 O38 Mo56 -38.4(15) . . . . ?
O45 Ti5 O32 Mo42 -64(2) . . . . ?
O45 Ti5 O32 Mo51 38.4(14) . . . . ?
O45 Ti5 O32 Mo57 -18(2) . . . . ?
O46 Mo5 O42 Mo15 -71.7(6) . . . . ?
O47 Mo8 O170 K2 -94.9(7) . . . 2_656 ?
O47 Mo8 O170 O190 13.8(12) . . . . ?
O47 Mo8 O190 O170 -167.7(10) . . . . ?
O47 Mo35 O143 Mo36 -57.3(13) . . . . ?
O47 Mo35 O156 K5 123.7(16) . . . 1_655 ?
O48 Mo3 O43 Mo11 -179.8(5) . . . . ?
O48 Mo3 O43 K3 46.6(10) . . . 2_656 ?
O48 Mo3 O124 Mo22 -75.2(6) . . . . ?
O48 Mo3 O124 Mo23 -177.1(5) . . . . ?
O48 Mo27 O65 Mo22 90.7(6) . . . . ?
O48 Mo27 O186 O194 87.3(10) . . . . ?
O48 Mo27 O194 O186 -85.8(10) . . . . ?
O49 Mo1 O19 Mo10 75.2(6) . . . . ?
O49 Mo1 O19 Mo16 176.9(5) . . . . ?
O51 Mo20 O74 K6 79.9(13) . . . . ?
O53 Mo4 O56 Mo12 179.9(5) . . . . ?
O53 Mo4 O71 Mo19 175.5(5) . . . . ?
O53 Mo4 O71 Mo20 75.7(6) . . . . ?
O54 Mo2 O4 K2 -53.3(10) . . . 2_656 ?
O54 Mo2 O147 Mo35 175.7(5) . . . . ?
O54 Mo2 O147 Mo36 76.1(6) . . . . ?
O54 Mo43 O116 Mo36 -92.2(6) . . . . ?
O54 Mo43 O168 O189 -85.3(10) . . . . ?
O54 Mo43 O189 O168 88.5(10) . . . . ?
O55 Mo5 O42 Mo15 -179.7(5) . . . . ?
O55 Mo5 O46 Mo21 -75.7(6) . . . . ?
O55 Mo5 O46 Mo25 -176.3(5) . . . . ?
O56 Mo4 O71 Mo19 -74.5(6) . . . . ?
O56 Mo4 O71 Mo20 -174.3(5) . . . . ?
O56 Mo12 O179 O180 -85.6(10) . . . . ?
O56 Mo12 O180 O179 88.8(10) . . . . ?
O58 Mo41 O34 K4 10.0(11) . . . . ?
O58 Mo41 O109 Ti10 -6(2) . . . . ?
O58 Mo42 O81 K4 -4.7(10) . . . . ?
O59 Mo9 O160 O163 85.8(9) . . . . ?
O59 Mo9 O163 O160 -89.0(9) . . . . ?
O60 Mo7 O83 O191 -95.9(11) . . . . ?
O60 Mo7 O191 O83 93.9(11) . . . . ?
O61 Mo15 O177 O178 -91.9(10) . . . . ?
O61 Mo15 O178 O177 96.7(10) . . . . ?
O63 Mo15 O177 O178 169.5(10) . . . . ?
O63 Mo15 O178 O177 -12.1(12) . . . . ?
O64 Mo24 O172 O174 -88.0(10) . . . . ?
O64 Mo24 O174 O172 87.0(10) . . . . ?
O65 Mo27 O186 O194 11.0(12) . . . . ?
O65 Mo27 O194 O186 -170.1(11) . . . . ?
O67 Mo42 O58 Mo41 105.3(13) . . . . ?
O67 Mo42 O81 K4 -112.7(8) . . . . ?
O68 Mo6 O166 K3 -100.4(7) . . . 2_656 ?
O68 Mo6 O166 O167 13.7(11) . . . . ?
O68 Mo6 O167 K2 -58.2(6) . . . 2_656 ?
O68 Mo6 O167 O166 -168.2(9) . . . . ?
O68 Mo8 O170 K2 60.0(6) . . . 2_656 ?
O68 Mo8 O170 O190 168.6(10) . . . . ?
O68 Mo8 O190 O170 -13.4(12) . . . . ?
O68 Ti10 O109 Mo41 -98(2) . . . . ?
O68 Ti10 O109 Mo46 169.7(14) . . . . ?
O68 Ti10 O109 Mo49 -144.4(13) . . . . ?
O69 Mo43 O116 Mo36 81.6(7) . . . . ?
O69 Mo43 O168 O189 98.5(10) . . . . ?
O69 Mo43 O189 O168 -91.6(11) . . . . ?
O70 Mo14 O182 O183 -92.5(10) . . . . ?
O70 Mo14 O182 K4 -19.0(7) . . . 3_676 ?
O70 Mo14 O183 O182 93.0(10) . . . . ?
O70 Mo14 O183 K4 27.3(7) . . . 3_676 ?
O71 Mo4 O56 Mo12 72.0(5) . . . . ?
O71 Mo19 O76 K8 98.5(7) . . . 1_455 ?
O71 Mo19 O86 K5 136.1(13) . . . . ?
O71 Mo20 O51 K8 -104.1(8) . . . 1_455 ?
O71 Mo20 O74 K6 -121.1(17) . . . . ?
O72 Mo29 O31 Ti8 -123.6(15) . . . . ?
O72 Mo29 O197 K1 -144.6(6) . . . . ?
O72 Mo29 O197 K7 27.1(6) . . . . ?
O73 Mo4 O56 Mo12 -74.5(5) . . . . ?
O73 Mo4 O71 Mo19 49.9(9) . . . . ?
O73 Mo4 O71 Mo20 -49.9(9) . . . . ?
O74 Mo20 O51 K8 70.1(9) . . . 1_455 ?
O75 Mo28 O171 O187 2.5(13) . . . . ?
O75 Mo28 O187 O171 -177.8(12) . . . . ?
O76 Mo19 O86 K5 -67.8(11) . . . . ?
O77 Mo11 O158 K3 87.5(7) . . . 2_656 ?
O77 Mo11 O158 O181 -13.9(12) . . . . ?
O77 Mo11 O181 O158 167.8(10) . . . . ?
O77 Mo23 O127 K5 -26.5(14) . . . . ?
O78 Mo5 O42 Mo15 74.1(5) . . . . ?
O78 Mo5 O46 Mo21 50.3(10) . . . . ?
O78 Mo5 O46 Mo25 -50.3(10) . . . . ?
O78 Ti8 O31 Mo29 80(3) . . . . ?
O78 Ti8 O31 Mo50 31(4) . . . . ?
O79 Ti8 O31 Mo29 57.4(14) . . . . ?
O79 Ti8 O31 Mo50 8.6(14) . . . . ?
O79 Ti9 O14 Mo41 -135(2) . . . . ?
O79 Ti9 O14 Mo46 -5(2) . . . . ?
O79 Ti9 O14 Mo49 -70.0(19) . . . . ?
O80 Mo39 O140 Mo17 169(4) . . . . ?
O80 Mo39 O140 K1 -24.4(6) . . . . ?
O81 Mo42 O58 Mo41 -2.2(16) . . . . ?
O82 Mo39 O80 K1 -150.3(5) . . . . ?
O82 Mo39 O140 Mo17 -10(5) . . . . ?
O82 Mo39 O140 K1 156.4(11) . . . . ?
O84 Mo18 O159 O173 -8.5(12) . . . . ?
O84 Mo18 O173 O159 172.9(10) . . . . ?
O84 Mo27 O65 Mo22 35.8(13) . . . . ?
O84 Mo27 O186 O194 165.8(11) . . . . ?
O84 Mo27 O194 O186 -16.7(12) . . . . ?
O84 Ti4 O38 Mo39 -151.9(13) . . . . ?
O84 Ti4 O38 Mo55 -105(2) . . . . ?
O84 Ti4 O38 Mo56 161.8(14) . . . . ?
O85 Ti7 O91 Mo17 -64(3) . . . . ?
O85 Ti7 O91 Mo40 37.1(12) . . . . ?
O85 Ti7 O91 Mo53 -9.2(16) . . . . ?
O85 Ti10 O109 Mo41 61(2) . . . . ?
O85 Ti10 O109 Mo46 -30.6(14) . . . . ?
O85 Ti10 O109 Mo49 15.4(14) . . . . ?
O86 Mo19 O76 K8 -74.1(9) . . . 1_455 ?
O87 Mo30 O144 K6 175.0(8) . . . . ?
O88 Mo4 O71 Mo19 97.5(5) . . . . ?
O88 Mo4 O71 Mo20 -2.3(5) . . . . ?
O88 Mo20 O51 K8 -140.7(11) . . . 1_455 ?
O88 Mo20 O74 K6 -88.6(12) . . . . ?
O88 Mo26 O9 K6 51.1(9) . . . . ?
O88 Mo26 O89 Mo20 -18.8(5) . . . . ?
O88 Mo26 O161 O193 -114.9(12) . . . . ?
O88 Mo26 O193 O161 121.2(11) . . . . ?
O88 Ti6 O90 Mo30 -86.5(15) . . . . ?
O88 Ti6 O90 Mo48 -146.8(16) . . . . ?
O89 Mo20 O51 K8 171.6(8) . . . 1_455 ?
O89 Mo20 O74 K6 -17.0(13) . . . . ?
O89 Mo26 O9 K6 -26.9(9) . . . . ?
O89 Mo26 O161 O193 -13.3(13) . . . . ?
O89 Mo26 O193 O161 167.6(12) . . . . ?
O90 Mo30 O87 K1 -116.7(9) . . . . ?
O90 Mo30 O144 K6 71.1(9) . . . . ?
O91 Mo17 O140 Mo39 -97(4) . . . . ?
O91 Mo17 O140 K1 97.3(6) . . . . ?
O92 Mo11 O158 K3 -163.8(6) . . . 2_656 ?
O92 Mo11 O158 O181 94.8(10) . . . . ?
O92 Mo11 O181 O158 -94.3(10) . . . . ?
O93 Mo8 O170 K2 156.3(6) . . . 2_656 ?
O93 Mo8 O170 O190 -95.0(10) . . . . ?
O93 Mo8 O190 O170 95.3(10) . . . . ?
O94 Mo23 O127 K5 68.8(14) . . . . ?
O95 Mo18 O159 O173 -87.1(10) . . . . ?
O95 Mo18 O173 O159 87.8(10) . . . . ?
O96 Mo9 O160 O163 7.7(11) . . . . ?
O96 Mo9 O163 O160 -173.6(9) . . . . ?
O96 Mo13 O142 O184 -170.0(10) . . . . ?
O96 Mo13 O184 O142 12.0(12) . . . . ?
O96 Ti12 O17 Mo29 137.4(15) . . . . ?
O96 Ti12 O17 Mo50 -166.2(16) . . . . ?
O97 Mo6 O166 K3 57.6(7) . . . 2_656 ?
O97 Mo6 O166 O167 171.7(9) . . . . ?
O97 Mo6 O167 K2 100.3(6) . . . 2_656 ?
O97 Mo6 O167 O166 -9.7(11) . . . . ?
O97 Mo11 O158 K3 -66.5(6) . . . 2_656 ?
O97 Mo11 O158 O181 -168.0(10) . . . . ?
O97 Mo11 O181 O158 13.8(12) . . . . ?
O97 Ti5 O32 Mo42 97(2) . . . . ?
O97 Ti5 O32 Mo51 -160.9(13) . . . . ?
O97 Ti5 O32 Mo57 142(2) . . . . ?
O98 Mo14 O70 K4 174.9(4) . . . 3_676 ?
O98 Mo14 O182 O183 134.8(11) . . . . ?
O98 Mo14 O182 K4 -151.7(9) . . . 3_676 ?
O98 Mo14 O183 O182 -130.9(12) . . . . ?
O98 Mo14 O183 K4 163.5(9) . . . 3_676 ?
O98 Ti3 O67 Mo42 3(2) . . . . ?
O98 Ti3 O67 Mo51 -132.5(18) . . . . ?
O98 Ti3 O67 Mo57 -55(3) . . . . ?
O98 Ti9 O14 Mo41 -7(2) . . . . ?
O98 Ti9 O14 Mo46 123(2) . . . . ?
O98 Ti9 O14 Mo49 57.5(19) . . . . ?
O99 Mo6 O166 K3 13.6(14) . . . 2_656 ?
O99 Mo6 O166 O167 127.6(10) . . . . ?
O99 Mo6 O167 K2 -15.8(14) . . . 2_656 ?
O99 Mo6 O167 O166 -125.8(11) . . . . ?
O99 Ti5 O32 Mo42 23(2) . . . . ?
O99 Ti5 O32 Mo51 125.1(14) . . . . ?
O99 Ti5 O32 Mo57 68(2) . . . . ?
O99 Ti10 O109 Mo41 -25(2) . . . . ?
O99 Ti10 O109 Mo46 -117.3(14) . . . . ?
O99 Ti10 O109 Mo49 -71.3(14) . . . . ?
O100 Mo5 O42 Mo15 3.1(4) . . . . ?
O100 Mo5 O46 Mo21 97.5(5) . . . . ?
O100 Mo5 O46 Mo25 -3.1(5) . . . . ?
O100 Mo15 O177 O178 119.2(11) . . . . ?
O100 Mo15 O178 O177 -124.0(11) . . . . ?
O100 Ti9 O14 Mo41 142(2) . . . . ?
O100 Ti9 O14 Mo46 -88(2) . . . . ?
O100 Ti9 O14 Mo49 -153.4(19) . . . . ?
O101 Mo24 O172 O174 -10.8(12) . . . . ?
O101 Mo24 O174 O172 171.0(10) . . . . ?
O101 Mo28 O171 O187 158.5(12) . . . . ?
O101 Mo28 O187 O171 -25.5(14) . . . . ?
O101 Ti8 O31 Mo29 -144.7(14) . . . . ?
O101 Ti8 O31 Mo50 166.5(14) . . . . ?
O102 Mo1 O19 Mo10 -2.7(4) . . . . ?
O102 Mo1 O19 Mo16 99.0(5) . . . . ?
O102 Mo1 O49 K2 -127.2(9) . . . . ?
O102 Mo10 O146 Mo16 94.8(6) . . . . ?
O102 Mo33 O164 K2 -7.1(11) . . . . ?
O102 Mo33 O164 O185 -116.5(10) . . . . ?
O102 Mo33 O185 O164 121.1(10) . . . . ?
O102 Ti1 O12 Mo39 -148.1(16) . . . . ?
O102 Ti1 O12 Mo55 149(2) . . . . ?
O102 Ti1 O12 Mo56 -84(2) . . . . ?
O103 Mo29 O31 Ti8 65.2(15) . . . . ?
O103 Mo29 O197 K1 35.3(7) . . . . ?
O103 Mo29 O197 K7 -153.0(6) . . . . ?
O103 Mo30 O87 K1 -40.2(9) . . . . ?
O103 Mo30 O144 K6 -8(3) . . . . ?
O104 Mo5 O46 Mo21 2.3(5) . . . . ?
O104 Mo5 O46 Mo25 -98.2(5) . . . . ?
O104 Mo28 O171 O187 106.3(13) . . . . ?
O104 Mo28 O187 O171 -126.4(11) . . . . ?
O104 Ti8 O31 Mo29 141.0(14) . . . . ?
O104 Ti8 O31 Mo50 92.2(14) . . . . ?
O105 Mo23 O127 K5 171.9(12) . . . . ?
O106 Mo1 O19 Mo10 -175.9(5) . . . . ?
O106 Mo1 O19 Mo16 -74.2(6) . . . . ?
O106 Mo1 O49 K2 50.6(10) . . . . ?
O107 Mo6 O166 K3 154.2(7) . . . 2_656 ?
O107 Mo6 O166 O167 -91.8(10) . . . . ?
O107 Mo6 O167 K2 -154.7(6) . . . 2_656 ?
O107 Mo6 O167 O166 95.3(9) . . . . ?
O108 Mo30 O87 K1 35.7(10) . . . . ?
O108 Mo30 O144 K6 -80.7(8) . . . . ?
O109 Mo41 O34 K4 -95.0(9) . . . . ?
O109 Mo41 O58 Mo42 105.2(14) . . . . ?
O110 Mo31 O162 K3 12.3(12) . . . . ?
O110 Mo31 O162 O188 117.4(10) . . . . ?
O110 Mo31 O188 O162 -121.7(10) . . . . ?
O110 Mo34 O120 Mo31 -2.7(4) . . . . ?
O110 Mo34 O120 K3 125.9(9) . . . . ?
O110 Mo34 O137 Mo37 -97.7(5) . . . . ?
O110 Mo34 O137 Mo38 3.0(4) . . . . ?
O110 Mo38 O125 K6 83(2) . . . 1_655 ?
O110 Mo38 O151 K8 -115.4(7) . . . . ?
O110 Ti11 O37 Mo17 -144(2) . . . . ?
O110 Ti11 O37 Mo40 86.8(17) . . . . ?
O110 Ti11 O37 Mo53 148.8(19) . . . . ?
O111 Mo31 O162 K3 60.9(6) . . . . ?
O111 Mo31 O162 O188 166.0(9) . . . . ?
O111 Mo31 O188 O162 -16.5(11) . . . . ?
O111 Mo32 O192 K2 -101.8(6) . . . . ?
O111 Mo32 O192 O195 9.2(11) . . . . ?
O111 Mo32 O195 K3 -60.1(6) . . . . ?
O111 Mo32 O195 O192 -172.1(9) . . . . ?
O111 Ti11 O37 Mo17 -70(2) . . . . ?
O111 Ti11 O37 Mo40 160.8(16) . . . . ?
O111 Ti11 O37 Mo53 -137.3(19) . . . . ?
O112 Mo34 O120 Mo31 -74.6(5) . . . . ?
O112 Mo34 O120 K3 54.0(9) . . . . ?
O112 Mo34 O128 Mo13 74.6(5) . . . . ?
O112 Mo34 O137 Mo37 -51.2(9) . . . . ?
O112 Mo34 O137 Mo38 49.6(9) . . . . ?
O113 Mo13 O142 O184 -117.1(11) . . . . ?
O113 Mo13 O184 O142 120.8(10) . . . . ?
O113 Mo34 O128 Mo13 2.7(4) . . . . ?
O113 Mo34 O137 Mo37 -2.5(4) . . . . ?
O113 Mo34 O137 Mo38 98.2(5) . . . . ?
O113 Mo37 O138 K6 -81(2) . . . 1_655 ?
O113 Ti12 O17 Mo29 -148.1(15) . . . . ?
O113 Ti12 O17 Mo50 -91.6(17) . . . . ?
O114 Mo32 O192 K2 20.3(14) . . . . ?
O114 Mo32 O192 O195 131.3(11) . . . . ?
O114 Mo32 O195 K3 -21.5(14) . . . . ?
O114 Mo32 O195 O192 -133.5(10) . . . . ?
O114 Ti1 O12 Mo39 63.3(17) . . . . ?
O114 Ti1 O12 Mo55 1(2) . . . . ?
O114 Ti1 O12 Mo56 127(2) . . . . ?
O114 Ti11 O37 Mo17 5(2) . . . . ?
O114 Ti11 O37 Mo40 -124.8(16) . . . . ?
O114 Ti11 O37 Mo53 -62.8(19) . . . . ?
O115 Ti11 O37 Mo17 90(2) . . . . ?
O115 Ti11 O37 Mo40 -39.7(17) . . . . ?
O115 Ti11 O37 Mo53 22.3(19) . . . . ?
O115 Ti12 O17 Mo29 -23.1(16) . . . . ?
O115 Ti12 O17 Mo50 33.4(17) . . . . ?
O116 Mo43 O168 O189 -8.9(12) . . . . ?
O116 Mo43 O189 O168 171.7(11) . . . . ?
O116 Mo36 O133 K8 -175.9(7) . . . . ?
O116 Mo36 O134 K5 -121.8(15) . . . 1_655 ?
O117 Mo31 O162 K3 157.7(6) . . . . ?
O117 Mo31 O162 O188 -97.2(10) . . . . ?
O117 Mo31 O188 O162 92.3(10) . . . . ?
O118 Mo2 O54 Mo43 2.8(4) . . . . ?
O118 Mo2 O147 Mo35 96.9(5) . . . . ?
O118 Mo2 O147 Mo36 -2.7(5) . . . . ?
O118 Mo43 O116 Mo36 -20.3(5) . . . . ?
O118 Mo43 O168 O189 -111.7(12) . . . . ?
O118 Mo43 O189 O168 126.1(10) . . . . ?
O118 Mo36 O133 K8 112.2(7) . . . . ?
O118 Mo36 O134 K5 -75(2) . . . 1_655 ?
O118 Ti7 O91 Mo17 171(3) . . . . ?
O118 Ti7 O91 Mo40 -87.9(12) . . . . ?
O118 Ti7 O91 Mo53 -134.3(15) . . . . ?
O119 Mo32 O192 K2 59.1(6) . . . . ?
O119 Mo32 O192 O195 170.1(9) . . . . ?
O119 Mo32 O195 K3 100.4(7) . . . . ?
O119 Mo32 O195 O192 -11.6(11) . . . . ?
O119 Mo33 O164 K2 -59.8(6) . . . . ?
O119 Mo33 O164 O185 -169.2(9) . . . . ?
O119 Mo33 O185 O164 13.0(11) . . . . ?
O119 Ti1 O12 Mo39 136.9(16) . . . . ?
O119 Ti1 O12 Mo55 74(2) . . . . ?
O119 Ti1 O12 Mo56 -159(2) . . . . ?
O120 Mo31 O162 K3 -18.1(5) . . . . ?
O120 Mo31 O162 O188 87.0(9) . . . . ?
O120 Mo31 O188 O162 -86.2(9) . . . . ?
O120 Mo34 O128 Mo13 -179.8(5) . . . . ?
O120 Mo34 O137 Mo37 -175.1(5) . . . . ?
O120 Mo34 O137 Mo38 -74.4(6) . . . . ?
O121 Mo9 O160 O163 -94.9(10) . . . . ?
O121 Mo9 O163 O160 90.7(10) . . . . ?
O122 Mo32 O192 K2 155.8(6) . . . . ?
O122 Mo32 O192 O195 -93.2(9) . . . . ?
O122 Mo32 O195 K3 -154.8(6) . . . . ?
O122 Mo32 O195 O192 93.2(9) . . . . ?
O123 Mo31 O162 K3 -93.9(7) . . . . ?
O123 Mo31 O162 O188 11.2(11) . . . . ?
O123 Mo31 O188 O162 -169.9(10) . . . . ?
O123 Mo38 O125 K6 130.0(16) . . . 1_655 ?
O123 Mo38 O151 K8 172.8(7) . . . . ?
O124 Mo3 O43 Mo11 -71.7(5) . . . . ?
O124 Mo3 O43 K3 154.7(9) . . . 2_656 ?
O124 Mo3 O48 Mo27 70.5(5) . . . . ?
O124 Mo23 O127 K5 -133.2(17) . . . . ?
O125 Mo38 O151 K8 76.5(8) . . . . ?
O126 Mo12 O179 O180 -168.8(10) . . . . ?
O126 Mo12 O180 O179 12.7(12) . . . . ?
O126 Mo19 O76 K8 -179.0(7) . . . 1_455 ?
O126 Mo19 O86 K5 30.4(11) . . . . ?
O128 Mo13 O142 O184 -90.8(10) . . . . ?
O128 Mo13 O184 O142 83.4(10) . . . . ?
O128 Mo34 O120 Mo31 178.8(5) . . . . ?
O128 Mo34 O120 K3 -52.5(10) . . . . ?
O128 Mo34 O137 Mo37 75.2(6) . . . . ?
O128 Mo34 O137 Mo38 175.9(5) . . . . ?
O129 Ti11 O37 Mo17 132(2) . . . . ?
O129 Ti11 O37 Mo40 2.7(17) . . . . ?
O129 Ti11 O37 Mo53 64.7(19) . . . . ?
O129 Ti12 O17 Mo29 -65.2(16) . . . . ?
O129 Ti12 O17 Mo50 -8.7(17) . . . . ?
O130 Mo7 O83 O191 13.0(12) . . . . ?
O130 Mo7 O191 O83 -168.3(11) . . . . ?
O130 Mo16 O198 K6 26.2(19) . . . . ?
O131 Mo42 O58 Mo41 -176.9(12) . . . . ?
O131 Mo42 O81 K4 173.7(8) . . . . ?
O132 Mo32 O192 K2 -23.9(5) . . . . ?
O132 Mo32 O192 O195 87.1(9) . . . . ?
O132 Mo32 O195 K3 22.7(6) . . . . ?
O132 Mo32 O195 O192 -89.3(9) . . . . ?
O133 Mo36 O134 K5 135.0(15) . . . 1_655 ?
O134 Mo36 O133 K8 -79.2(8) . . . . ?
O135 Mo13 O142 O184 -14.5(11) . . . . ?
O135 Mo13 O184 O142 166.9(10) . . . . ?
O135 Mo37 O138 K6 -123.3(14) . . . 1_655 ?
O136 Mo41 O34 K4 -170.2(9) . . . . ?
O136 Mo41 O58 Mo42 -179(100) . . . . ?
O136 Mo41 O109 Ti10 -169(2) . . . . ?
O137 Mo34 O120 Mo31 71.4(5) . . . . ?
O137 Mo34 O120 K3 -160.0(8) . . . . ?
O137 Mo34 O128 Mo13 -72.3(5) . . . . ?
O137 Mo37 O138 K6 -38.9(14) . . . 1_655 ?
O137 Mo38 O125 K6 46.1(16) . . . 1_655 ?
O137 Mo38 O151 K8 -81.2(19) . . . . ?
O139 Mo33 O164 K2 -156.6(6) . . . . ?
O139 Mo33 O164 O185 94.0(10) . . . . ?
O139 Mo33 O185 O164 -95.0(10) . . . . ?
O140 Mo39 O80 K1 30.0(7) . . . . ?
O143 Mo35 O156 K5 -32.5(17) . . . 1_655 ?
O143 Mo36 O133 K8 24.5(8) . . . . ?
O143 Mo36 O134 K5 32.8(16) . . . 1_655 ?
O144 Mo30 O87 K1 139.1(9) . . . . ?
O145 Mo10 O146 Mo16 -171.1(6) . . . . ?
O146 Mo16 O198 K6 -173.6(18) . . . . ?
O147 Mo2 O4 K2 -160.0(8) . . . 2_656 ?
O147 Mo2 O54 Mo43 -72.5(5) . . . . ?
O147 Mo35 O143 Mo36 -24.3(5) . . . . ?
O147 Mo35 O156 K5 39.3(16) . . . 1_655 ?
O147 Mo36 O133 K8 78(2) . . . . ?
O147 Mo36 O134 K5 -39.0(15) . . . 1_655 ?
O148 Mo14 O182 O183 87.1(10) . . . . ?
O148 Mo14 O182 K4 160.6(6) . . . 3_676 ?
O148 Mo14 O183 O182 -88.9(10) . . . . ?
O148 Mo14 O183 K4 -154.6(6) . . . 3_676 ?
O149 Mo37 O138 K6 135.3(13) . . . 1_655 ?
O150 Mo16 O198 K6 -70.6(19) . . . . ?
O151 Mo38 O125 K6 -127.8(15) . . . 1_655 ?
O152 Mo12 O179 O180 93.8(10) . . . . ?
O152 Mo12 O180 O179 -94.3(10) . . . . ?
O154 Mo37 O138 K6 33.9(14) . . . 1_655 ?
O154 Mo38 O125 K6 -26.4(17) . . . 1_655 ?
O154 Mo38 O151 K8 -27.6(8) . . . . ?
O155 Mo35 O143 Mo36 169.8(7) . . . . ?
O155 Mo35 O156 K5 -135.9(16) . . . 1_655 ?
O156 Mo35 O143 Mo36 62.2(8) . . . . ?
O157 Mo39 O80 K1 -152.5(15) . . . . ?
O157 Mo39 O140 Mo17 -10(4) . . . . ?
O157 Mo39 O140 K1 156.5(4) . . . . ?
O161 Mo26 O9 K6 -144.7(8) . . . . ?
O161 Mo26 O89 Mo20 -164.8(6) . . . . ?
O165 Mo17 O140 Mo39 -170(4) . . . . ?
O165 Mo17 O140 K1 24.2(15) . . . . ?
O166 Mo6 O167 K2 110.0(11) . . . 2_656 ?
O167 Mo6 O166 K3 -114.0(12) . . . 2_656 ?
O168 Mo43 O116 Mo36 -168.4(6) . . . . ?
O169 Mo29 O31 Ti8 155.5(15) . . . . ?
O169 Mo29 O103 Mo30 180(100) . . . . ?
O169 Mo29 O197 K1 -146.8(14) . . . . ?
O169 Mo29 O197 K7 25(2) . . . . ?
O175 Mo30 O87 K1 -42(2) . . . . ?
O175 Mo30 O144 K6 -4.8(8) . . . . ?
O176 Mo41 O34 K4 -168.4(11) . . . . ?
O176 Mo41 O58 Mo42 179.7(14) . . . . ?
O176 Mo41 O109 Ti10 -91(2) . . . . ?
O181 Mo11 O158 K3 101.5(12) . . . 2_656 ?
O182 Mo14 O70 K4 15.3(6) . . . 3_676 ?
O182 Mo14 O183 K4 -65.7(10) . . . 3_676 ?
O183 Mo14 O70 K4 -23.0(6) . . . 3_676 ?
O183 Mo14 O182 K4 73.5(10) . . . 3_676 ?
O185 Mo33 O164 K2 109.3(11) . . . . ?
O186 Mo27 O65 Mo22 165.0(6) . . . . ?
O188 Mo31 O162 K3 -105.1(11) . . . . ?
O189 Mo43 O116 Mo36 -173.9(7) . . . . ?
O190 Mo8 O170 K2 -108.6(12) . . . 2_656 ?
O192 Mo32 O195 K3 112.0(11) . . . . ?
O193 Mo26 O9 K6 -107.3(8) . . . . ?
O193 Mo26 O89 Mo20 -172.8(8) . . . . ?
O194 Mo27 O65 Mo22 171.6(8) . . . . ?
O195 Mo32 O192 K2 -111.0(11) . . . . ?
O196 Mo27 O65 Mo22 -84.6(7) . . . . ?
O196 Mo27 O186 O194 -96.9(11) . . . . ?
O196 Mo27 O194 O186 92.8(11) . . . . ?
O197 Mo29 O31 Ti8 -41.0(15) . . . . ?
O197 Mo29 O103 Mo30 -1(2) . . . . ?
O199 Mo28 O171 O187 -104.3(12) . . . . ?
O199 Mo28 O187 O171 87.1(12) . . . . ?
O200 Mo42 O58 Mo41 -179.7(13) . . . . ?
O200 Mo42 O81 K4 169.5(8) . . . . ?
O202 Mo17 O140 Mo39 12(5) . . . . ?
O202 Mo17 O140 K1 -153.9(7) . . . . ?
Mo49 O58 Mo57 O32 103(4) . . . . ?
Mo49 O58 Mo57 O67 -93(4) . . . . ?
Mo49 O58 Mo57 O81 -177(3) . . . . ?
Mo49 O58 Mo57 O131 179(100) . . . . ?
Mo49 O58 Mo57 O200 7(4) . . . . ?
Mo50 O103 Mo48 K1 -23(2) . . . . ?
Mo50 O103 Mo48 O87 -5(3) . . . . ?
Mo50 O103 Mo48 O90 96(2) . . . . ?
Mo50 O103 Mo48 O108 -105(2) . . . . ?
Mo50 O103 Mo48 O175 177(2) . . . . ?
Mo57 O58 Mo49 O14 99(4) . . . . ?
Mo57 O58 Mo49 O34 175(4) . . . . ?
Mo57 O58 Mo49 O109 -111(4) . . . . ?
Mo57 O58 Mo49 O136 176(3) . . . . ?
Mo57 O58 Mo49 O176 -8(4) . . . . ?
K4 Mo14 O182 O183 -73.5(10) 3_676 . . . ?
K4 Mo14 O183 O182 65.7(10) 3_676 . . . ?
K4 Mo41 O58 Mo42 4.9(13) . . . . ?
K4 Mo41 O109 Ti10 80(2) . . . . ?
K4 Mo42 O58 Mo41 -4.9(13) . . . . ?
K4 O34 Mo47 O14 95(2) . . . . ?
K4 O34 Mo47 O58 20(2) . . . . ?
K4 O34 Mo47 O109 -54(2) . . . . ?
K4 O34 Mo47 O136 -158(2) . . . . ?
K4 O34 Mo47 O176 17(3) . . . . ?
K4 O81 Mo44 O32 65.8(17) . . . . ?
K4 O81 Mo44 O58 -11.4(16) . . . . ?
K4 O81 Mo44 O67 -87.7(17) . . . . ?
K4 O81 Mo44 O131 168.0(15) . . . . ?
K4 O81 Mo44 O200 -8(3) . . . . ?
K4 O182 O183 Mo14 -114.2(5) 3_676 . . . ?
K6 O144 Mo52 O87 176.2(6) . . . . ?
K6 O144 Mo52 O90 100.5(7) . . . . ?
K6 O144 Mo52 O103 178.2(11) . . . . ?
K6 O144 Mo52 O108 -107.4(7) . . . . ?
K6 O144 Mo52 O175 -3.9(10) . . . . ?
K5 O131 Mo44 O32 101.3(12) . . . . ?
K5 O131 Mo44 O58 175.9(19) . . . . ?
K5 O131 Mo44 O67 -105.0(12) . . . . ?
K5 O131 Mo44 O81 -1.0(13) . . . . ?
K5 O131 Mo44 O200 177.3(11) . . . . ?
K7 O176 Mo46 O14 65.1(8) . . . . ?
K7 O176 Mo46 O58 143.1(5) . . . . ?
K7 O176 Mo46 O109 -140.6(6) . . . . ?
K7 O176 Mo46 O136 -42.0(11) . . . . ?
K7 O176 Mo49 O14 23.5(11) . . . . ?
K7 O176 Mo49 O34 -53(2) . . . . ?
K7 O176 Mo49 O58 132.6(9) . . . . ?
K7 O176 Mo49 O109 -121.1(8) . . . . ?
K7 O176 Mo49 O136 -49.4(9) . . . . ?
K7 O197 Mo50 O17 125.9(6) . . . . ?
K7 O197 Mo50 O31 -81.2(6) . . . . ?
K7 O197 Mo50 O72 21.9(8) . . . . ?
K7 O197 Mo50 O103 -157.1(5) . . . . ?
K7 O197 Mo50 O169 -154.2(12) . . . . ?
K8 Mo38 O125 K6 -94.6(16) . . . 1_655 ?
K8 O165 Mo40 K1 32.0(13) . . . . ?
K8 O165 Mo40 O37 103.4(7) . . . . ?
K8 O165 Mo40 O91 -112.6(7) . . . . ?
K8 O165 Mo40 O140 178.7(7) . . . . ?
K8 O165 Mo40 O153 -5.8(10) . . . . ?
K8 O165 Mo40 O202 174.9(7) . . . . ?
K8 O165 Mo54 O37 63.1(19) . . . . ?
K8 O165 Mo54 O91 -85.3(17) . . . . ?
K8 O165 Mo54 O140 -15(3) . . . . ?
K8 O165 Mo54 O153 -10.7(17) . . . . ?
K8 O165 Mo54 O202 170.1(14) . . . . ?

_olex2_submission_special_instructions 'No special instructions were received'
# start Validation Reply Form
_vrf_PLAT306_1                   
;
PROBLEM: Isolated Oxygen Atom (H-atoms Missing ?) .......       O201 Check 
RESPONSE: These oxygen atoms are coordinated with K atoms.
;
